Download Rubber Basics...
Rubber Basics Edited by R.B. Simpson
Rubber Basics Edited by
Richard B. Simpson
Shawbury, Shrewsbury, Shropshire, SY4 4NR, United Kingdom Telephone: +44 (0)1939 250383 Fax: +44 (0)1939 251118 http://www.rapra.net
First published in 2002 by
Rapra Technology Limited Shawbury, Shrewsbury, Shropshire, SY4 4NR, UK
© 2002, Rapra Technology Limited
All rights reserved. Except as permitted under current legislation no part of this publication may be photocopied, reproduced or distributed in any form or by any means or stored in a retrieval system, without the prior permission from the copyright holder.
A catalogue record for this book is available from the British Library.
Typeset by Rapra Technology Limited Printed and bound by Rapra Technology Limited
Foreword The Rubber Industry has a long history going back several hundred years and during its development the terminology used has not always been the most logical or descriptive. For example, Hancock described his masticator and mixing device as a ‘Pickle’ to avoid conveying any knowledge of what it did or how it worked. As it carries the baggage of this considerable period of time, some new to the industry find it difficult to understand. With terms such as spew, mould dope, pig, drug room and cracking all having their own rubber-related meaning, it is little wonder that the industry is regarded by outsiders as a Black Art. Consequently, this book has been compiled to be used as a quick reference. It includes a glossary of terms, tables of technical data, and, for those who require more detail, there are more comprehensive text sections covering the major rubber types, compounding ingredients and the equipment used in the most common processes. It should prove useful to those coming into the Rubber Industry, those in other businesses who have to work with it, and as a reference document for the everyday practitioner. R. B. Simpson
Disclaimer The data presented in this book is intended as a guide only. Whilst due care has been taken in the compilation of this information, it is published on the basis that no responsibility or liability shall attach to Rapra Technology Limited or its employees arising out of or in connection with the utilisation in any form of the material contained within it.
Contents Section 1
Glossary of Rubber Terms ………………………………………... 1 Conversion Factors for Units of Measurement ………………………………….. 67
Specific Gravities of Some Rubbers and Compounding Ingredients ……..…………………………... 69 2.1 2.2
Rubbers …………………………………………………………….. 75 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8 3.9 3.10 3.11 3.12 3.13 3.14 3.15 3.16 3.17 3.18 3.19 3.20 3.21 3.22 3.23 3.24 3.25 3.26 3.27
Specific Gravities of Some Compounding Ingredients ……………….….. 71 Specific Gravities of Rubbers ………………………………………………. 74
Natural Rubber (NR) ………………………………………………...………. 77 Polyisoprene (synthetic natural rubber) (IR) …………………………….… 79 Polybutadiene (BR) ……………………………………………………..…... 80 Nitrile Rubbers (NBR/HNBR) ………………………………………..……... 81 Epichlorohydrin Polymers (CO/ECO/ETER) ………………………………. 83 Polychloroprene (CR) ………………………………………………..……… 84 Polynorbornene …………………………………………………………….... 86 Butyl Rubbers (IIR/BIIR/CIIR) ……………………………………….…….... 87 Styrene-Butadiene Rubber (SBR) ………………………………………….. 88 Ethylene-Propylene Rubber (EPM/EPDM) ……………………………...… 89 Chlorinated Polyethylene (CPE, CM) ………………………………………. 91 Chlorosulphonated Polyethylene (CSM, CSPE) ………………………….. 92 Ethylene-Vinyl Acetate Copolymer (EVA, EAM) ………………………….. 93 Ethylene-Acrylic Rubber (EACM, AEM) ………………………………...…. 93 Polyacrylate Rubbers (ACM) ………………………………………..….…... 94 Silicone Rubbers (MQ, VMQ, FVMQ, PVMQ) …………………………….. 96 Ebonite ………………………………………………………………………… 97 Polysulphide Rubber (OT, EOT) ……………………………………………. 98 Propylene Oxide-Allyl Glycidyl Ether Copolymer (PO, GPO) …………… 99 Polyurethane Elastomers (AU, EU, PU) …..……………………………... 100 Fluorocarbon Rubber (FPM, FKM) …………………………………….…. 103 Thermoplastic Elastomers - General Description ……………………..... 106 Thermoplastic Urethane Elastomers (TPAU, TPEU, TPU) …………….. 109 Styrenic Block Copolymers: SBS and SIS ……………………………….. 111 Styrenic Block Copolymers: SEBS ………………………………...……... 112 Copolyether Ester TPE …………………………………………..………... 113 Polyester Amide TPE …………………………………………………..….. 114
Rubber Compounding Ingredients …………………………… 117 4.1 4.2 4.3 4.4 4.5 4.6 4.7 4.8 4.9 4.10 4.11 4.12 4.13 4.14 4.15 4.16 4.17 4.18
Accelerators ……………………………………………………………..….. 121 Activators ……………………………………………………………………. 123 Antidegradants ……………………………………………………………… 126 Antireversion Agents ……………………………………………………….. 128 Antistatic Agents ……………………………………………………………. 128 Biocides and Fungicides …………………………………………………… 128 Blowing Agents ……………………………………………………………… 129 Bonding Additives …………………………………………………………... 131 Deodorants and Reodorants ………………………………………………. 132 Desiccants …………………………………………………………………… 132 Dusting and Anti-Tack Agents …………………………………………….. 132 Factice ……………………………………………………………………….. 133 Fillers ………………………………………………………………………… 134 Fire Retardants ……………………………………………………………… 141 Peroxides ……………………………………………………………………. 142 Petroleum Oils ………………………………………………………………. 144 Pigments …………………………………………………………………….. 147 Plasticisers for Polar Synthetic Rubbers …………………………………. 148
4.19 4.20 4.21 4.22 4.23 4.24
Prevulcanisation Inhibitors ………………………………………………… 149 Process Additives …………………………………………………………... 149 Release Agents …………………………………………………………….. 151 Resins ……………………………………………………………………….. 151 Vulcanising Agents …………………………………………………………. 153 Waxes ……………………………………………………………………….. 154
Rubber Processing Equipment …………….………………….. 157 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9 5.10 5.11 5.12 5.13 5.14 5.15 5.16 5.17 5.18 5.19 5.20 5.21 5.22 5.23 5.24 5.25 5.26 5.27 5.28 5.29 5.30 5.31 5.32 5.33 5.34 5.35 5.36 5.37 5.38 5.39 5.40 5.41 5.42 5.43 5.44 5.45 5.46 5.47 5.48 5.49
Autoclaves ……………………………………….…………….……………. 161 Cable Manufacturing ………………………………...….………………….. 161 Calenders ………………………..……………………….………………….. 162 Compound Drying/Cooling ………………………..……………………….. 164 Compression Moulding Presses ………………………………………...... 165 Continuous Vulcanisation ………………………..………………………… 165 Conveyors, Material/Haul-Off ……………………………………………… 167 Cutting Equipment ………………………..………………………………… 167 Deflashing ………………………..………………………………………….. 168 Dipping ………………………..……………………………………………… 168 Dusting Devices ………………………..…………………………………… 170 Extruders, Cavity Transfer Mixer ………………………………………….. 170 Extruders, Cold-Feed ………………………………………………………. 171 Extruders, Dump/Pelletiser/Strainer/Roller Die ………………………….. 172 Extruders, Gear Pump ………………………..……………………………. 173 Extruders, Heads and Dies ………………………..………………………. 174 Extruders, Hot-Feed ………………………..………………………………. 174 Extruders, Mixers ………………………..……………….…………………. 175 Extruders, Piggy Back Systems …………………………………………… 176 Extruders, Pin Barrel ………………………..……………………………… 176 Extruders, Ram ………………………..……………………………………. 177 Extruders, Vacuum ………………………..………………….…………….. 177 Granulators/Shredders/Grinders ………………………………………….. 178 Hose Machinery ………………………..…………………………………… 179 Hydraulic Drives ………………………..…………………………………… 180 Injection Moulding Machines ……………………..……………………….. 180 Internal Mixers ………………………..……………………….…………….. 183 Laboratory Processing Equipment ………………………….…………….. 185 Marking Devices ………………………..…………………………………… 185 Metal Preparation for Bonding …………………………………………….. 186 Microwave Heating …………………………………………………………. 187 Mills, Cracker ………………………………………………………………... 187 Mills, Mixing …………………………………………………………………. 187 Mills, Stock Blenders ……………………………………………………….. 188 Mixers for Rubber Cement/Dough and Solution ………………………… 189 Mould Cleaning ………………………..……………………………………. 190 Moulds ………………………..……………………………………………… 190 Ovens for Cure, Post-Cure and Ageing Applications …………………… 191 Preheating Bales ………………………..………………………………….. 191 Preheaters Other Than Microwave ……………………………………….. 191 Presses, Lead ………………………..……………………………………… 192 Presses, Rotary Curing ………………………..…………………………… 192 Spreading/Coating Machines ………………………..……...…………….. 192 Temperature Control Units ………………………………………………… 193 Thickness Gauges ………………………………………………………….. 193 Transfer Moulding ………………………………………………………….. 194 Tyre Building Equipment ………………………..…………………………. 195 Tyre Retreading Equipment ……………………………………………….. 196 Weighing Equipment ……………………………………………………….. 197
Index ………………………………………………………………………………………………………. 199
Section 1 Glossary of Rubber Terms
1,1,3-Tributyl Thiourea TBTU, accelerator. 1,3-Diethyl-2-Thiourea DETU, accelerator. 1,3-Diphenyl-2-thiourea DPTU, accelerator. 2,2´-Dihydroxy-5,5’-Dichloro-Diphenylmethane DDM, latex auxiliary. 2-Mercaptobenzimidazole MBI, antidegradant – non-staining. 2-(Morpholinothio) benzothiazole MBS, accelerator. 4,4´-Dithiodimorpholine DTDM, vulcanising agent. 6-Ethoxy-2,2,4-Trimethyl-1,2-Dihydroquinoline ETMQ, antidegradant – staining. 6PPD N-1,3-Dimethylbutyl-N’-phenyl-pphenylenediamine, antidegradant – staining. 77PD N,N´-Bis(1,4-dimethylpentyl)-pphenylenediamine, antidegradant – staining.
Accelerated Ageing (Air Oven) This is carried out in a heated oven through which air is circulating; the temperature ranges from 70 °C to > 200 °C, depending on the base polymer and application. The temperature used should be the lowest that gives a measurable deterioration within a reasonable test period. Higher temperatures are likely to involve different ageing mechanisms and hence correlation with real ageing will be poor. Accelerator A compounding ingredient which speeds up the vulcanisation reaction, enabling it to take place in a shorter time or at a lower temperature or both; the physical properties of the vulcanisate and its resistance to ageing are also improved. ACGIH American Conference of Governmental Industrial Hygienists ACN Abbreviation for acrylonitrile. ACOP Approved Code of Practice (UK) Acrylic Rubbers Rubbers based on polymers of organic acrylates. Acrylonitrile CH2CHCN (vinyl cyanide); raw material for the manufacture of nitrile rubber, synthetic fibres and plastics. Acrylonitrile-Butadiene Rubber See Nitrile Rubber. Activator A compounding ingredient that enables an accelerator to exercise its maximum effect. Inorganic activators are metallic oxides (such as zinc, lead and magnesium oxides) and organic activators are long-chain saturated fatty acids, e.g., stearic and oleic. ADC Azodicarbonamide, blowing agent. ADCA Abbreviation for azodicarbonamide. Adhesives Polymeric materials are commonly used for bonding materials. Impact or contact adhesives are mainly based on highly crystalline polychloroprene (Neoprene), NR latex is used as a flexible adhesive very suitable for use with fabrics. Rigid adhesives based on materials such as polystyrene cement, epoxy resin or cyanoacrylates are suitable for bonding of rigid materials. The bond is provided by intermolecular forces between the adhesive and the adherend. Adiabatic Taking place without gain or loss of heat. ADPA Acetone-diphenylamine condensation product, antidegradant – staining. ADS Abbreviation for air-dried sheets of rubber. Adsorption The taking up of molecules of a gas or of a dissolved substance by the surface of a solid; adsorption is a surface effect only. See Absorption. AEM Abbreviation for ethylene-acrylic terpolymer.
$ AAS Atomic absorption spectroscopy. Ablation Literally ‘removal’, but applied particularly in space technology to the process of using up the frictional heat developed on re-entry of the vehicle into the Earth’s atmosphere by degradation of the heat shield. Certain thermoplastics, thermosetting resins and polytetrafluoroethylene have been evaluated as ablative materials. Abrasion Resistance The ability of a rubber article to withstand wearing away in service. Standard BS 903: Part A9. Determination of abrasion resistance. ABS Abbreviation for acrylonitrile-butadiene-styrene, an amorphous thermoplastic. Absolute Pressure Pressure measured with respect to zero pressure. See Gauge Pressure. Absolute Zero Zero on the absolute or Kelvin scale of temperature; 0 K = –273 °C. Absorption The taking up of gases or liquids into solids. Absorption occurs throughout the whole mass of the absorbing medium, whereas adsorption is confined only to the surface. Accumulator A device for storing hydraulic pressure; in its simplest form it is a long vertical hydraulic cylinder, on top of the ram on which weights may be placed or suspended. Acetylene C2H2, a colourless poisonous flammable gas; the starting material for many organic compounds, e.g., chloroprene. See Neoprene. ACM An abbreviation for acrylic rubbers.
Rubber Basics Aftercure In the vulcanisation of rubber products, aftercure is the amount of cure received after the termination of the cure proper, e.g., the cure effect resulting from the heat remaining in the product after removal from the mould or autoclave. The term is also applied to the continuation of the curing effect that results from exposure of the article to heat in use, or from accelerated ageing. See Post Cure. Ageing The deterioration of the physical properties of rubber products when exposed to service conditions; also the controlled exposure of rubber samples to a variety of deteriorating influences in the evaluation of antioxidants and antiozonants. See Accelerated Ageing. Air Oven Ageing See Accelerated Ageing. Air Spring An inflatable bellows used in a pneumatic suspension system for motor transport; irrespective of load the centre of gravity of the vehicle can be maintained at a constant height above ground level with appropriate control systems. Alcohols A family of organic compounds obtained by removing one or more -H atoms from a paraffin and substituting the hydroxyl radical -OH. The best-known alcohols are ethyl alcohol (ethanol) and methyl alcohol (methanol). Glycerine is a trihydric alcohol. Allotropy Many elements including sulphur, carbon and oxygen can exist in two or more forms with different physical, and often chemical, properties; such elements are said to exhibit allotropy and the different forms are known as allotropes or allotropic forms. Alumina Aluminium hydroxide, inorganic filler. Aluminium Hydroxide Alumina, inorganic filler. Ammonium Polyphosphate AP, flame retardant. Amorphous Having no definite shape; non-crystalline. Anatase One of the crystalline forms of titanium dioxide. Anisotropic Describes a material that has different physical properties in different directions. See Calender Grain. Anticoagulant Any substance used to prevent premature coagulation of rubber latex; the commonest are ammonia, sodium sulphite and formaldehyde. Antidegradant A term applied to compounding ingredients, mainly antioxidants, which inhibit premature degradation of elastomers. Antimony Trioxide Flame retardant. Antioxidant An ingredient added to a rubber compound to protect the product against deterioration by
oxygen. Antioxidants belong to the class of compounding ingredients known as protective agents, and their mode of action is considered to be removal of free radicals which are generated by the interaction of oxygen and the polymer at elevated temperatures. Failure to remove these free radicals will result in an ongoing deterioration of the polymer. Antiozonant An ingredient added to rubber compounds to protect the product against the deteriorating influence of ozone. The function of antiozonants is not limited to protection against ozone attack, they also give a high level of protection against oxidative and thermal degradation, and against fatigue failure (flex cracking). Antirad A compounding ingredient added to elastomers to increase their resistance to ionising radiation. Antistatic Rubber Rubber so compounded as to produce a vulcanisate having an electrical resistivity of about 107 to 109 ohm-cm. See Conductive Rubber. AP Abbreviation for ammonium polyphosphate. ASTM Abbreviation for American Society for Testing and Materials. Atactic A term applied to high polymers which are irregular in their stereo configuration, i.e., which do not show stereoregularity. Atomic Absorption Spectroscopy This technique is used to detect metals in rubber analysis. AU Abbreviation for polyester type polyurethane rubbers. Autoclave A pressure vessel constructed of steel, used for the vulcanisation of rubber products by the ‘open steam’ method. The autoclave may be horizontal (vulcanisation of footwear, cables, hose), or vertical and fitted with a hydraulic ram (e.g., moulding pneumatic tyres). AZDN Azobis-isobutyronitrile, blowing agent. Azobis-Isobutyronitrile AZDN, blowing agent. Azodicarbonamide ADC, blowing agent.
% BAA Butyraldehyde-aniline condensation product, accelerator. Back Rinding Tearing or distortion of a moulded rubber product at the line of separation of the two mould halves (the spew line) due to the sudden release, on opening the mould, of the high pressures developed by the thermal expansion of the heated rubber; other names are suck back, flash back and retracted spew.
Band (1) A strip of rubber from a previous batch left running round the front roll of an open mill to facilitate loading of the next batch. (2) An assembly of plies of rubberised cord fabric used in ‘building’ or making; the casing of a pneumatic tyre. Bank (1) On an open mill, the proportion of the mill load which runs in the space immediately adjacent to the nip between the rolls. (2) The amount of rubber compound running at the nip or nips of a calender during the operations of frictioning, sheeting, coating or profiling. Balata The hard thermoplastic hydrocarbon obtained from the latex of Mimusops globosa. Balata has the same molecular formula as natural rubber (C5H8)n but has the trans polyisoprene structure whereas natural rubber has cis-structure. Ball Mill A cylindrical container half to two-thirds filled with a grinding charge consisting of unglazed porcelain, glass balls, pebbles or flint gravel; it is used in the preparation of aqueous dispersions of ingredients for use in the manufacture of products direct from latex. Ballotini A material used in fluid bed vulcanisation. It consists of very small spherical particles of glass of a narrow size distribution, approximately 0.1 to 0.2 mm. Banbury Mixer The type of internal mixer designed by F.H. Banbury; the name ‘Banbury’ is often erroneously applied to any type of internal mixer. Barium Sulphate See Barytes and Blanc Fixe. Barrel That part of an extruder in which the screw rotates. Barwell Preformer/Ram Extruder An apparatus for preparing moulding blanks. It is a development of the Barwell ram extruder which feeds through interchangeable dies to give the correct profile of blank, while an electronically operated cutter, working across the face of the die, cuts the blanks. Oil is admitted to the ram of the extruder in controlled quantities, set by a metering device, so that the compound is forced from the die in the correct amount to form each blank. Barytes Naturally occurring barium sulphate, BaSO4; it has the high specific gravity of approximately 4.45 and is used as a filler, especially when a high specific gravity rubber compound is desired or is not a disadvantage. Is also used as an acid resistant white filler. BCMA British Colour Makers’ Association BCUP Tert.-Butyl cumylperoxide, organic peroxide. BDMC Bismuth dimethyl dithiocarbamate, accelerator.
Bead (1) In a pneumatic tyre, that portion of the structure which holds the tyre on the wheel; it consists of a circular assembly of steel wires insulated with rubber, suitably wrapped and covered with rubberised fabric to enable the bead assembly to be built into the uncured casing. (2) In dipped goods, a reinforcing edge made by rolling back for a short distance the film of rubber deposited on the former. Bead to Bead Remoulding A tyre retreading process in which new rubber is applied as tread, on the tyre shoulders and on the tyre sidewalls. Bentonite A colloidal clay used as a thickener in latex compounding and as a filler in dry rubber compounding; the reaction of bentonite with amines has produced several useful rubber reinforcing fillers. Benzene C6 H6, the simplest member of the aromatic series of hydrocarbons; it is a colourless liquid with b.p. of 80 °C and is used in the manufacture of many organic compounds. Benzoyl Peroxide A vulcanising agent particularly for silicone rubber and fluoroelastomers; it has been used as a non-sulphur vulcanising agent for natural rubber. It is also a catalyst in emulsion polymerisation. Beta Rays Streams of swiftly moving electrons given off by some radioactive substances; they are used in beta ray gauges which give continuous measurement of the thickness of films of rubber or plastics. BgVV Bundesinstituts für gesundheitlichen Verbraucherschutz und Veterinärmedizin, German body which sets legislation on compounding ingredients and migration testing for rubbers which come into contact with food. BHT Butylated hydroxytoluene, (2,6-Di-tert.-butyl-pcresol), antidegradant – non-staining. Bias In the manufacture of pneumatic tyres and some types of hose, the angle at which the textile material is cut with respect to the running edge of the fabric. BIBRA British Industrial Biological Research Association BiDD Bismuth dimethyl dithiocarbamate, accelerator. BIIR Abbreviation for bromobutyl rubber. Biodeterioration Deterioration of rubbers, fibres or plastics resulting from attack by living organisms. Birefringence The existence in a high polymer (elastomer, fibre or plastic) of two refractive indices. The ratio of the two indices is a measure of the crystallinity of the polymer.
Rubber Basics Bismuth Dimethyl Dithiocarbamate BDMC and BiDD, accelerator. Bisphenol AF 2,2’-Bis(4-hydroxyphenyl)perfluoropropane, vulcanising agent. Black Abbreviation of carbon black. Bladder Another name for the inflatable diaphragm which takes the place of the curing bag in the automatic curing of pneumatic tyres in a diaphragm press. Blanc Fixe Precipitated barium sulphate. Blank A piece of uncured rubber compound of suitable shape and volume to fill the cavity of the mould in which it is to be vulcanised; also termed a ‘slug’. Blanket - Compressible A printing blanket with a specially manufactured layer designed to ‘give’ or compress, under pressure from the printing plate and impression cylinder. Compressible blankets resist smashing and usually print a sharper halftone dot. Blanket Crepe A grade of natural rubber inferior to estate brown crepe and formerly known as thick remilled brown crepe; cuttings removed in the inspection of smoked sheet rubber are washed, creped and designated ‘smoked blanket crepe’. Bleaching Agent A substance added to latex in the preparation of pale crepe rubber; sodium bisulphate prevents darkening of the crepe due to the presence of oxidising enzymes, xylyl mercaptan is an effective bleaching agent proper. BLIC Bureau de Liaison des Industries du Caoutchouc de L’Union Européenne. Block Copolymer A copolymer in which blocks of one polymer are inserted in a primary chain of the other or where the arrangement of the different monomers is not random but in distinct multiple monomer blocks. Blocking The tendency of sheets of rubber to stick together, dusting and anti-tack agents are used to overcome this problem. Blooming The formation on the surface of uncured or cured rubber of a thin coating of a compounding ingredient, often, but not necessarily, sulphur, which is present in excess of the amount which the rubber can dissolve. Blowing Agent Used in the manufacture of sponge rubber. (1) Chemical blowing agents undergo decomposition at the vulcanisation temperature to form a gaseous species such as nitrogen or carbon dioxide, e.g., azo compounds, nitroso compounds, sulphonyl hydrazide compounds, ammonium carbonate, ammonium bicarbonate and sodium bicarbonate. (2) Physical blowing agents are low boiling point organic compounds (e.g., dichloromethane or
pentane), which volatilise at the processing temperature. Blow Moulding A manufacturing method predominately used by the thermoplastic industry for the manufacture of hollow components, also used for thermosetting rubber. The polymer is forced against the inside of the mould surface by gas pressure applied either by a hollow needle or by the decomposition of a blowing agent. BNPD 2-Bromo-2-nitropropane-1,3-diol, latex auxiliary. Bound Rubber The rubber in unvulcanised filler-rubber mixes which is insoluble in a usual rubber solvent. Bonding Agent A material used to promote the bonding of rubber to other materials, principally metal and textiles. Bowl Another name for a calender roll. BPH 2,2’-Methylene-bis(4-methyl-6-tert.butylphenol), antidegradant – non-staining. BPO Dibenzoyl peroxide, organic peroxide. BR Abbreviation for rubber based on butadiene. Brabender Plasti-Corder and Plastograph An apparatus for the determination of the processibility of polymers. It measures cure rate, scorch characteristics, extrusion rate and similar screw properties. BRABENDER® single measuring extruders and Extrusiograph® are interchangeable measuring heads which, in connection with a Plasti-Corder® Lab-Station or Plastograph®, serve for testing the extrudability of polymers and for studying problems occurring in research and development as well as in practical application. The BRABENDER® modular system allows the complete instrumentation of the extruders for raw material checks and development. Manifold screws, die heads, and downstream equipment fulfil many kinds of extrusion tasks. Braid Angle Angle between the braid and the axis of the hose in fabric- or wire-braided hose. Braided Fabric A structure produced by interlacing several ends or yarns in a manner such that the paths of the yarns are not parallel to the fabric axis. Braided Hose Hose in which the textile or steel wire reinforcement is applied by a braiding method. The braiding may be applied to the hose, supported either horizontally or vertically. Breakdown The plasticising of raw rubber prior to the incorporation of compounding ingredients or the plasticising (warming or warming-up) of mixed compound prior to subsequent processing. Breaker (1) In a pneumatic tyre, a strip or strips of textile or metallic fabric of more open construction than the casing fabric, placed circumferentially around the tyre underneath
Buna The name originally applied to all synthetic rubbers produced by the sodium polymerisation of butadiene; it is derived from Bu for butadiene and Na for sodium. The name was subsequently used in various forms, e.g., Buna N for nitrile rubber or NBR, and Buna S for SBR. The tradename Perbunan (Bayer) is also derived from Buna. Butadiene A gas, CH2CHCHCH2 (buta-1,3-diene), used in the manufacture of polybutadiene rubber and as one of the copolymers in the manufacture of styrene-butadiene and nitrile rubbers. Tert-Butyl Cumylperoxide BCUP, organic peroxide. Butyl Rubber (Isobutylene Isoprene Rubber – IIR) A synthetic rubber made by copolymerising isobutylene with 1% to 3% of isoprene, depending on the degree of unsaturation required. The percentage of isoprene determines the cure rate of the compound, the higher the isoprene content the faster the cure. Butyl has high gum strength, high resistance to ozone attack, low permeability to gases, good flex and tear resistance and good electrical properties. A characteristics of butyl is its low resilience compared to natural rubber at room temperature, but at higher temperatures, about 100 °C, its resilience matches that of natural rubber. Butyl has poor resistance to mineral oils and organic solvents. Butyl rubber is not compatible with natural rubber, SBR, nitrile rubber or with any other elastomer having an appreciable degree of unsaturation; modified butyls (chlorobutyl and bromobutyl) are compatible with such elastomers and used as liners in tubeless tyres to improve air retention. Butyl can be processed without great difficulty on standard rubber machinery, but equipment should be well cleaned before and after processing butyl, since contamination can result in local undercure and delamination. In the early days of development in the 1940s, butyl was largely used for tyre inner tubes because of its excellent air-retention properties, but it is now finding wide application in mechanicals and cables. Butylated Hydroxytoluene BHT, 2,6-di-tert.-butyl-p-cresol, antidegradant – non-staining.
the tread; in belting a similar fabric fitted as an outer ply. (2) The term is also applied to a cracker mill. British Standards Institution The recognised body in the United Kingdom for the preparation of specifications for quality, performance or dimensions, methods of test, definitions and symbols, codes of practice, etc. British Standards are prepared under the guidance of representative committees and are widely circulated before they are authorised for publication. BSI co-operates in preparing international standards for rubber and plastics through ISO/TC45 and ISO/TC61 respectively. See ISO. British Thermal Unit The amount of heat required to raise the temperature of 1 lb of water by 1 degree Farenheit. Brittle Point When an elastomer sample is subjected to low temperatures, the brittle point is the highest temperature at which the sample breaks when subjected to a sharp blow. The brittle point is one indication of low temperature flexibility and is usually somewhat higher than the glass transition temperature. BRMA British Rubber Manufacturers’ Association Brown Crepe Crepe rubber of lower quality than pale crepe; it is made from the pre-coagulated lumps which form in the latex before the coagulation process is carried out. Brownian Movement The rapid motion in all directions of the particles in a colloidal solution; it results from the irregular bombardment of the suspended particles by the molecules of the liquid. BS Abbreviation for British Standard. BSI Abbreviation for British Standards Institution. Bud Grafting A means of reproducing high yielding or other desirable characteristics in the rubber tree; a bud taken from a seedling bred from a tree known to yield large quantities of good quality latex is grafted onto the stem of a young rubber plant. Buffing Worn tyres are prepared for retreading by a buffing/grinding process to provide a fresh rubber surface. Bulk Density The ratio of the apparent volume of a material in powder form to the volume of the material in solid form, i.e., after removal of the air entrapped between the particles. In moulding (plastics or rubber) using powdered material, the bulk factor is thus the ratio of the volume of the powder to the volume of the moulding made from it. Bumping In the moulding of rubber products, the operation of opening and closing the press rapidly in the early stages of the cure to drive out any trapped air.
& CAD Abbreviation for computer-aided design. Calcium Carbonate CaCO3, a white solid which occurs in nature as chalk, limestone and marble; the ground product, often termed whiting, is used as an extending filler in rubber compounding.
Rubber Basics Calcium Nitrate Ca(NO3)2, used in an alcoholic solution in coagulant dipping for the manufacture of latex dipped goods. Calcium Silicate CaSiO3, a reinforcing filler in rubber compounding. Calender A machine having two, three or four heavy rolls, used in the rubber manufacturing techniques of coating, doubling, embossing, frictioning, profiling and sheeting. Calender Bowl Deflection The distortion suffered by calender rolls resulting from the pressure of the rubber running between them. If uncorrected the deflection produces a rubber sheet thicker in the middle than at the edges. See Camber, Crossed Axes and Roll Bending, all techniques to compensate for calender bowl deflection. Calender Grain The name given to the differences in properties lengthwise and crosswise in calendered sheet. In the direction of calendering tensile strength is high and extensibility low; at right angles to the direction in which it leaves the calender rolls, strength is relatively low and extensibility high. In some non-moulded articles the heat of vulcanisation may cause distortion, the grain effect causing the sheet to contract in length and become wider and thicker. This distortion may be minimised by plying up two thin sheets at right angles or by subjecting the sheet to the process of shrinking. Calendering The various processes carried out on a calender. See Coating, Doubling, Embossing, Frictioning, Profiling and Sheeting. CAM Abbreviation for computer-aided manufacture. Camber The slight curvature given to calender bowls to counteract the deflection produced when the calender is running, thus enabling a rubber sheet of uniform thickness across its width to be obtained. Camelback Tread-type rubber compound extruded in a variety of thicknesses and widths for use in tyre retreading. The standard section is in the shape of a regular trapezium, but variations are made to suit particular types of tyre and different makes of moulding equipment. Caoutchouc The French word for rubber, formerly used to denote highly purified natural rubber, also termed rubber hydrocarbon. Caprolactam 1,6-hexanolactam, the monomer from which nylon 6 is prepared; nylon 6 is polycaprolactam. Carbon Black The name given to a variety of forms of fine particle carbon which have the property of conferring reinforcement on rubber compounds, the degree of reinforcement increasing with decreasing particle size.
Carbon Black Structure When electron microscope studies first showed clearly the anisotropy of carbon black particles the appearance was of a chain of particles fused together, to which the term ‘reticulate chain structure’ was given, later abbreviated simply to ‘structure’. The degree of structure has an influence on the level of reinforcement conferred by the carbon black. Carbon Gel Bound rubber in an unvulcanised carbon blackrubber mix. It results from the production of free radicals in the mastication of rubber; these radicals attach themselves chemically to the particles of carbon black and form a proportion of carbon gel which is insoluble in the usual rubber solvents. Carcinogenicity The capacity of some agent or chemical substance to induce cancer in man or other animal species. Casein A pale yellow solid, the main protein in milk. It is used as a stabilising agent in latex compounding. Casting A method of manufacturing rubber articles by pouring a compounded latex into an absorbent hollow mould; the skin of rubber thus formed is removed, dried and vulcanised. The term is also applied to the pouring into moulds of liquid polymer systems based on silicone or polyurethane elastomers. Catalyst A substance which alters the rate of a chemical reaction, but which exists chemically unchanged at the end of the reaction. Cavity Transfer Mixer The cavity transfer mixer (CTM) is a distributive mixing device used as an add-on unit to extruders; the barrel and screw have hemispheres cut out of their surfaces to give an overlap of half a pitch. CBS Abbreviation for cyclohexylbenzothiazole sulphenamide, the first of the sulphenamide range of delayed action accelerators. CEFIC European Council of Chemical Manufacturers Federations. Celsius A scale of temperature in which the interval between freezing point and boiling point of water is divided into one hundred degrees. This scale therefore came to be known as the centigrade scale, although the official designation is Celsius. Centrifuge An apparatus which rotates at very high speed, used for separating solids from liquids, or liquids from other liquids; there must be a difference in specific gravity between the two substances. Centrifuging A process for separating particles from a suspension by using centrifugal force. It is the most popular method for concentrating natural rubber latex before shipment from plantation to country of use.
Cetyltrimethylammonium Bromide See CTAB. Chafer The reinforcing rubber and fabric around the bead in the rim area of a tyre to prevent chafing of the tyre by the rim. Chalk Natural calcium carbonate, CaCO3, formed from the shells of tiny marine organisms, used as an extending filler in rubber compounding and as a release agent. The term is often loosely applied to any dusting agent. See Whiting. Chalking The release of filler particles at the surface of a product due to oxidation of the rubber. The term is also used in the sense of ‘dusting’ an uncured rubber surface to prevent adhesion. Chelating Agent A substance which results in the chemical inactivation of a metal. The catalytic effect of heavy metals, mainly copper and manganese, on the oxidation of unsaturated compounds such as rubber, results in very rapid deterioration. Chelating agents convert the metal into a chelate co-ordination compound and thus render the metal inactive. The term ‘sequestering agents’ has been applied to chelating agents but this infers that the metal has been removed and not merely inactivated. CHIP Chemicals (Hazard Information and Packaging for Supply) Regulations (UK). Chlorinated Rubber A white fibrous product obtained when chlorine is passed into a solution of rubber. It was used mainly in corrosion-resistant paints and varnishes but has been superseded by tailored synthetic polymers systems. Chlorobutadiene 2-chloro-1,3-butadiene (chloroprene), a volatile colourless liquid, the monomer for the preparation of polychloroprene rubbers. Chlorobutyl Chlorinated butyl rubber. Chlorination or bromination of butyl rubber overcomes the difficulty of vulcanising butyl rubber in mixtures with more highly unsaturated substances due to the preferential absorption of the sulphur by the more highly unsaturated component. Chlorohydrin Rubbers A class of synthetic elastomers based on epichlorohydrin. Chloroprene Rubber (CR) This is the preferred designation for all chloroprene polymers and copolymers. Chloroprene rubber was first introduced commercially in 1931 by DuPont and their trade name, originally DuPrene, later Neoprene, has almost become a generic term for all such rubber. See Chlorobutadiene. Chlorosulphonated Polyethylene (CSPE) An elastomer made by substituting chlorine and sulphonyl chloride groups into polyethylene. The material is best known by the trade name Hypalon, which is the DuPont trade mark for their brand of chlorosulphonated polyethylene.
Chromatography A technique of chemical analysis in which the components of a liquid mixture are adsorbed in separate layers in a column of adsorbing material. Variations of the technique are paper chromatography and gas chromatography. CI Abbreviation for Colour Index. CIIR Abbreviation for chlorobutyl rubber. CIPG Abbreviation for cured-in-place gasket. Cis-trans Isomerism A form of isomerism associated with compounds containing a double bond; similar groups of atoms may be either on the same side of the plane of the double bond (cis-form), or on opposite sides (trans-form). The terms are from the Latin, cis, on this side and trans, across. The important properties of a polymer are determined by the geometrical arrangement of its building units. Natural rubber (polyisoprene) has the cis-form giving a highly elastic material, while guttapercha has the trans-form and is relatively nonelastic and more crystalline. Clay This term is applied to a wide variety of materials known chemically as hydrated aluminium silicates, used as inorganic fillers. China clay (kaolin) shows a slight reinforcing effect; ‘treated’ clays show considerably greater reinforcement. Clone A group of trees (of, for example, Hevea Brasiliensis) derived by bud grafting from a single mother tree. Cloth Count The number of warp ends and the number of weft picks per unit length in a woven fabric; written, e.g., 23 x 23, the unit length being 1 inch on the imperial system of measurement. CM Abbreviation for chlorinated polyethylene. CNR Abbreviation for Cameroon Natural Rubber. CO Epichlorohydrin homopolymer. Coacervation Any process which brings about destabilisation of a latex to such an extent that the particles coalesce. Depending on the form resulting from the agglomeration, the coacervation may be described as either coagulation, flocculation or gelation. Coagulant Any substance which will bring about coagulation. In the preparation of natural rubber the usual coagulants are acetic or formic acids. In the manufacture of dipped goods from latex, the coagulant used depends on the method of dipping employed. Coagulation In rubber latex, the process whereby the dispersed rubber globules separate out from the watery serum; the globules clot together to form a jelly-like mass, the coagulum. In the preparation of natural rubber, coagulation of the latex is
Rubber Basics Cold Rubber This is styrene-butadiene rubber polymerised at a temperature of 5 °C (41 °F) in contrast to the original polymerisation temperature of 50 °C (122 °F). It is also known as Low Temperature Polymer (LTP). Nitrile rubber can also be made by a low temperature process. Such polymers are characterised by improved processibility. Colloid A colloid is a suspension of particles with diameters between 1 nm and 100 nm. The particles are charged and can be subjected to cataphoresis (electrophoresis). They are subject to Brownian movement and have a large amount of surface activity. Their properties lie between those of true solutions and coarse suspensions. Colloidal State A state of subdivision of matter with a particle size between 10-7 and 10-5 cm (1 nm to 100 nm). The properties of colloids lie between those of true solutions and coarse suspensions. Colour Index (CI) Pigments are classified by an internationally recognised convention, published in the International Colour Index by the Society of Dyers and Colourists in Bradford, in association with the American Association of Textile Chemists and Colorists. The Index issues a generic name to chemically identical products (e.g., titanium dioxide is classified as C.I. Pigment White 6). Where structures are known, pigments are also given a constitution number (e.g., titanium dioxide has the constitution number CI 77891).This number is reserved for the essential colorant, other ingredients, such as the carriers used in a masterbatch, do not affect this classification. Compound In chemistry a compound is defined as a substance consisting of two or more elements chemically united in definite proportions by weight. However, many technologists use the term ‘compound’ in the sense of a mixture. In rubber technology, a compound is a composition obtained by adding to an elastomer substances known as compounding ingredients and blending to produce a homogeneous mixture or mix. Other terms for this unvulcanised mix are mixing, stock, blend or quality. The term may also be used in the sense of the mix formulation, i.e., the kinds and amounts of the elastomers and compounding ingredients used to give the requisite properties in the end product. Compounding The development of rubber compounds which will effectively withstand the conditions under which the products made from them are to be used; the mixes so developed must be capable of being processed in the factory without undue difficulty. The term is also applied to the assembling of elastomer and compounding ingredients ready for the mixing proper. Compounding Ingredient Any substance added to an elastomer to produce a rubber compound.
brought about by the addition of either acetic or formic acid but it may occur spontaneously through the action of microorganisms in the latex. Coagulum In the preparation of natural rubber, the coagulum is the soft clot or mass of rubber particles which separates out from the serum after addition of the coagulant. Coacervant A coacervant is a material, solid or liquid, which destabilises a latex so that the particles coalesce in large numbers. May also be described as coagulant or flocculant. Coating Coating, skim-coating or topping is a calendering process in which a thin sheet of rubber formed at one nip is applied to the surface of a textile material as it passes through a second nip. The term ‘coating’ may also be used in the wider sense of applying rubber to a textile by any noncalendering method such as spreading, dipping or spraying. Coefficient of Friction Static friction is the force which must be overcome in order to start the motion of a body over a surface. Kinetic friction is the force which must be continuously overcome in order to maintain uniform motion of the body over the surface. The coefficient of friction (static or kinetic respectively) is the frictional force divided by the perpendicular or normal force between the surfaces in contact. Coefficient of Thermal Expansion (Volume) Increase in volume per unit volume resulting from a temperature rise of 1 °C. The coefficient of thermal expansion of rubber compounds varies from 0.00066 for a pure gum mix down to approximately 0.00048 depending on the amount of the loading. This high expansion relative to steel (about 10 to 20 times greater) can result in moulding defects. See Back Rinding, Shrinkage. Cold Cure A now obsolete process for vulcanising coated, usually spread fabrics. No sulphur was added to the mix from which the spreading dough was made, the curing effect being obtained by exposing the fabric to the action of sulphur monochloride diluted with a petroleum solvent. The cloth was passed over a roller which ran in a trough containing the curing solvent. Combinations of ultra accelerators are now used. Cold End A section at each end of the platens of a hydraulic press used for curing belting, where the temperature is lower than that of the remainder of the platens. The object is to reduce overcure at the overlapped areas, which would otherwise receive a double cure. Cold Mastication Mastication of rubber which is carried out at temperatures below 90 °C is termed ‘cold’. The masticating effect is at a minimum at temperatures around 105 °C, breakdown occurring much more rapidly at higher or lower temperatures.
Compression Moulding The method of manufacture of solid rubber products by simultaneous shaping and vulcanising. An uncured blank of rubber compound is placed in the bottom half of a mould, the top half of the mould placed in position and the mould placed in a heated hydraulic press. The press performs the dual function of both closing and heating the mould. See Transfer Moulding and Injection Moulding. Compression Set The residual decrease in thickness of a rubber test piece, expressed as a percentage of the original thickness, after the test piece has been subjected to a compression stress under specified conditions of time of loading, time of recovery and temperature. BS 903: Part A6. Determination of compression set. Concentrated Latex Natural rubber latex as obtained from the tree contains only about 30% by weight of rubber. Concentration of the latex is done by either centrifuging, creaming, electro-decantation or evaporation. Condensate Water formed in a steam supply system when the steam has given up its heat and returned to the liquid state. Since condensate still contains useful heat it is returned to the boiler as make-up water. Condensation A chemical reaction in which two or more molecules react, with the elimination of water or of some other simple substance. Condensation Polymerisation Polymerisation resulting from a chemical reaction involving condensation. The synthetic elastomers produced by condensation polymerisation include polysulphide rubbers, silicone rubbers and the ester and isocyanate rubbers. Conductive Rubber Rubber which is deliberately rendered electrically conductive by the inclusion in the unvulcanised mix of certain types of carbon black. Conductive rubber for use in, e.g., aircraft tyres has a resistivity below about 105 to 107 ohm-cm. The changeover from the use of channel blacks to oilbased furnace blacks has conferred a degree of conductivity (sometimes unwanted) on many black rubber products, and it should no longer be assumed that any black rubber is a good electrical insulator. See Antistatic Rubber. Conductivity The ability of a substance to permit the passage of heat (thermal conductivity) or of electricity (electrical conductivity). Conjugated Double Bonds An arrangement of alternate single and double bonds between the carbon atoms in diolefinic compounds. Continuous Filament In the manufacture of man-made and synthetic textiles the base materials are extruded through tiny orifices producing continuous lengths of very fine fibres or filaments. The textiles are mostly used in this ‘continuous filament’ form, but for some purposes the filaments may be cut up into short fibres and spun into a yarn.
Continuous Vulcanisation Any method of vulcanising rubber products which proceeds without interruption from start to finish as compared to the method of vulcanising separate batches of products or sections of a product. Continuous vulcanisation processes include the cold curing of proofed cloth, the vulcanisation of belting and flooring, of cables and certain extruded products by either the Liquid Curing Medium, Fluid Bed, Microwave, or Hot Air techniques. Conveyor Belting Belting used mainly in the transmission of materials, although increasing use is being made of conveyor belting in the transportation of passengers. Co-ordination Polymerisation A process related to ionic polymerisation where the catalyst system complexes of aluminium alkyls and titanium halides governs the way in which a monomer and a growing chain approach each other. Copolymer A ‘high polymer’ resulting from the polymerisation of a mixture of two different monomers; styrene-butadiene rubber, butyl (isoprene-isobutylene) rubber and nitrile (acrylonitrile-butadiene) rubber are typical copolymers. Copolymerisation The chemical reaction which brings about the formation of a copolymer. Copper Dimethyl Dithiocarbamate A fast accelerator for SBR compounds. It is used as either a primary or as a secondary accelerator along with a thiazole type. Copper Inhibitor Certain antioxidants also offer protection against the deleterious effects of copper and manganese, and are thus termed copper inhibitors. Cord (1) A solid circular extruded section of rubber compound generally of small diameter used as blanks in moulding O-rings and similar products. (2) The twisted fibre of polyester, rayon, nylon or steel, which imparts strength to the tyre carcase and belt. See Tyre Cord. Corona A luminous discharge resulting from air breakdown in the vicinity of high voltage cables. Corona produces ozone (from the oxygen in the air) and may result in rapid deterioration of the cable insulation and other unsaturated rubber in the vicinity. COSHH Control of Substances Hazardous to Health Regulations (UK). Cotton A natural fibre which has been superseded by the various synthetic fibres for use as reinforcement in rubber articles. Coumarone-Indene Resins Resins resulting from the polymerisation of one of the fractions of coal tar. Used as processing aids, tackifiers and as non-black organic reinforcing agents in rubber compounding.
Rubber Basics Count The count of a rubber thread is the number of threads which measure exactly one inch across when placed side by side. See Cloth Count and Yarn Count. Covalency A valency bond created by the sharing of a pair of electrons; also termed a ‘non-polar’ bond. CPE Abbreviation for chlorinated polyethylene. CR Abbreviation for chloroprene rubbers. Cracker A heavy type of open mill with deeply corrugated rolls, used for the preliminary breakdown of rubber compound prior to the processes of extrusion and calendering. Cracking (1) The tearing apart or breaking down of rubber compound on a cracker. (2) The appearance on the surface of rubber products of cracks or fissures as a result of exposure to the atmosphere (atmospheric cracking) or to repeated bending or stretching (flex cracking). (3) Decomposition of a chemical substance by heat; particularly the decomposition of heavier petroleum distillates to produce a larger supply of lighter fractions. Crazing The name given to the surface appearance of a vulcanised elastomer which has suffered oxidation catalysed by light. The inelastic skin first formed gradually thickens and cracks in random directions. Creamed Latex Latex which has been concentrated by creaming. Creaming One of the methods of concentrating normal rubber latex; the rubber globules rise to the surface of the heavier serum, the process usually being hastened by the addition of creaming agents such as ammonium alginate. Creep That characteristic of vulcanised elastomers or thermoplastics in showing a gradual increase in deformation under constant load with passage of time; also known as strain relaxation or drift. Crepe Rubber Any form of natural rubber which is marketed with the rough surface produced by passing the rubber through a series of mills with grooved rolls travelling at differential speeds. The main types are pale crepe, sole crepe, brown crepe and flat bark crepe. Crimp The difference in length between the ends of a yarn as it lies in the woven cloth and its length when removed from the cloth and straightened out, expressed as a percentage of the length in the cloth. Crocking The staining of a surface by light rubbing contact with a pigmented rubber. Crossed Axes A method of producing the effect of a variable camber on a calender. By skewing or crossing the
axis of one roll in relation to the other the nip is thus opened more at the ends of the roll than in the middle. Crosslink Density The number of moles of physically effective crosslinks per gram of vulcanisate. Crosslinking The joining of polymer molecules to each other by valency bonds. In very long chain-like elastomer molecules crosslinking introduces lateral links between either two separate molecules or different parts of the same molecule. See Vulcanisation. Crown With reference to a calender, another term for camber. Crows’ Feet Arrow-shaped markings on the surface of calendered sheet rubber due either to the use of insufficiently warmed stock or to too low temperature of the calender rolls. Crumb Rubber Vulcanised waste rubber which has been ground down to a desired mesh size (18, 20, 24, 30 or 40) for addition to new compound as a filler; a better term is vulcanised rubber crumb. See Powdered Rubber. Crystallinity Degree of crystallisation. Although no polymer is completely crystalline, the term ‘crystalline polymer’ is applied to one with an appreciable degree of crystallinity. Crystallisation In high polymers crystallisation means the formation of areas of regularity in chain aggregation rather than the formation of discrete crystals, as in simple chemical compounds. Crystallite A crystalline region in a polymer matrix. See Crystallisation. CSM Abbreviation for chlorosulphonated polyethylene. CSPE Abbreviation for chlorosulphonated polyethylene. CTAB Cetyltrimethylammonium bromide, latex auxiliary. Also used as an adsorbent to measure the total surface area of carbon black. CTM Abbreviation for cavity transfer mixer. CTP N-(Cyclohexylthio)phthalimide, retarder. Cup Lump A blanket crepe rubber produced from the dried films and lumps of rubber found in the tapping cups at the beginning of the next tapping. Cup lump results from the spontaneous coagulation of the latex which has dripped from the tree after the cup has been emptied of the main flow. Curing This term is synonymous with vulcanisation but is generally applied to the factory methods of vulcanising rubber products, e.g., press curing, open steam curing, cold curing. Curing Bag In pneumatic tyre manufacture, the heavy rubber tube to which is admitted the inflation medium
which provides the pressure for moulding. Air, steam or hot water have all been used for inflation and curing bags may therefore be termed air bag, steam bag or water bag. See Bladder. Curometer An apparatus for determining the curing characteristics of rubber compounds. Cut Edge Term applied to belting made without a moulded edge. Cut Thread Rubber in the form of fine ‘threads’ produced by vulcanising a thin sheet of rubber compound, winding it on a drum and slitting it to the required size by revolving the drum against a number of sharp, wetted knives which revolve at high speed. Cyclised Rubber An isomeric derivative of natural rubber produced by a variety of chemical treatments. The products are resinous and find application as reinforcing agents in natural rubber compounds (particularly in shoe soles) and as rubber-to-metal adhesives.
trimming machine or by ‘tumbling’ the products in a barrel held at a temperature low enough to harden the flash and permit it to be rubbed off by the motion of the products in the barrel. Defo Plastometer A type of parallel plate plastometer developed in Germany; it differs from the conventional parallel plate instrument in that it measures the load required to deform the test sample by a specified amount in a fixed time. Degradation Deterioration usually by chemical or physical means rather than by a mechanical process. Degraded Modulus After a test specimen of an elastomer has been subjected to repeated deformation, the modulus at some lesser deformation is lower than the initial value. The modulus after such stress softening has been termed the degraded modulus. See Mullins Effect. DEHP Di-2-ethylhexyl phthalate, ester plasticiser. Dehydration Simply removal of water, but the term is usually applied to the removal of chemically-combined water. Delamination Splitting into layers; usually applied to the separation of the plies from which a composite rubber article has been built up. Delayed Action Accelerator An accelerator which permits processing of rubber compounds to be carried out with less risk of scorching but which does not slow down the rate of cure at normal vulcanisation temperatures. Demoulding The operation of removing a vulcanised product from the mould in which it has been cured. Denier A system of numbering yarns and filaments, generally of man-made and synthetic fibres. Denier is the weight in grams of 9000 m of the filament or yarn. Density The weight of unit volume of a substance. See Specific Gravity. Deodorant Compounding ingredient used to neutralise unpleasant odours in rubber. Depolymerisation Breaking down of a long chain molecule into relatively short chain molecules of the same empirical composition as the original substance or in some cases to the original monomer. Depolymerised Rubber (DPR) Natural rubber which has been reduced to an easy flowing consistency by prolonged mastication in the presence of peptising agents. Suitably compounded, DPR may be cast into moulds and vulcanised; ebonite products from DPR are also possible. Desiccant A substance added to rubber compounds to absorb and retain (even at curing temperatures) moisture which would otherwise be a factor in producing porosity.
' Damping Decrease in the amplitude of an oscillation or wave motion with time. Damping in rubber testing results from hysteresis. Daylight Press An apparatus, usually operated by hydraulic pressure, in which the vulcanisation of moulded rubber products is carried out. The ‘daylight’ is the space between the heated platens on which the moulds are placed. A press is specified by the platen area, the number of daylights and the press tonnage. DBP Abbreviation for dibutyl phthalate, a plasticiser for natural and synthetic rubbers. DBTU N,N´-Dibutylthiourea, accelerator. DCBS N,N-Dicyclohexyl-2-benzothiazole sulphenamide, accelerator. DDM 2,2’-Dihydroxy-5,5’-dichloro-diphenylmethane, latex auxiliary. De Mattia Flex Test A test method for comparing the resistance of rubbers to the formation and growth of cracks. Moulded samples with a central groove are repeatedly bent from a straight to a doubled position. The degree of cracking is estimated by comparison with photographs of standard samples. BS ISO 132 Determination of flex cracking and crack growth (De Mattia). Dead Milled Applied to rubber which has been subjected to prolonged mastication, often carried out with periods of rest between mastication stages; such rubber shows little or no elastic recovery. Deflashing The removal of flash or spew from moulded rubber products. This may be done by hand, by
Rubber Basics DETU Abbreviation for 1,3-diethyl-2-thiourea, accelerator. Dew Point That temperature at which the water vapour present in the air saturates the air and therefore begins to condense as ‘dew’. DHBP 2,5-Dimethylhexane-2,5-di-tert.-butyl peroxide, organic peroxide. Di-2-Ethylhexyl Adipate DOA, ester plasticiser. Di-2-Ethylhexyl Phthalate DEHP, ester plasticiser. Di-2-Ethylhexyl Sebacate DOS, ester plasticiser. Di-o-tolyl guanidine DOTG, accelerator. Di-tert.-Butyl Peroxide DTBP, organic peroxide. Diaphragm (1) A sheet of rubber or of rubber-textile composite moulded, if desired, to a particular shape and used in a wide variety of applications in industry, e.g., diaphragm packings, diaphragm-operated valves for steam, air or liquids. (2) The flexible membrane or ‘bladder’ which supplies internal pressure in the curing of pneumatic tyres in diaphragm presses of the Bag-o-matic or Autoform type. Diaphragm Press In tyre manufacture, a press which uses a flexible diaphragm to supply to the inside of the tyre the internal inflation medium for both shaping and vulcanising. The diaphragm replaces the heavy curing bag used in the now obsolete autoclave moulding of tyres. Diaphragm presses are generally automated. Dibenzoyl Peroxide BPO, organic peroxide. Dibenzthiazyl Disulphide MBTS, an organic accelerator of the thiazole class. Dibutyl Phthalate (DBP) An organic (ester) compound used as a plasticiser in nitrile rubbers and in polyvinyl chloride. N,N´-Dibutylthiourea DBTU, accelerator. Dicumyl Peroxide A non-sulphur vulcanising agent for natural rubber and some types of synthetic rubber. One trade name is Dicup. N,N-Dicyclohexyl-2-benzothiazole sulphenamide DCBS, accelerator. DIDP Abbreviation for diisodecyl phthalate, plasticiser. Die (1) In extrusion of solid rubber sections, the shaped metal plate fitted in the head of the extruder to produce the desired contour; in extrusion of hollow tubing the outer circular part which fits over the pin, pencil or nozzle to give the hollow section. (2) A sharp tool used in punching out special shapes of rubber or rubbered fabric or used in
preparing test-pieces of vulcanised rubber, e.g., dumbbell strips for tensile testing. Dielectric Heating Also termed electronic or high frequency (HF) heating. Heating is carried out by placing the object between plates connected to a source of high-frequency current. Vulcanising of rubber products may be done by HF heating but the method finds its greatest application in the preheating of blanks prior to moulding. It has also been used for thawing out frozen rubber. Dielectric Strength The electrical stress required to puncture a sample of a material of known thickness; usually expressed in kilovolts per mm of thickness. The standard BS EN 60243-1 gives details of the test procedure. Diene Another name for diolefin. Die Swell The increase in dimensions of an extruded section as it leaves the die; the swell is mainly due to elastic recovery. Diethylene Glycol A plasticiser of particular use in compounds containing silica or silicate fillers. Differential Scanning Calorimetry This technique is used to generate thermograms, which can be used in quality control and to identify additives in rubber. Diffusion The migration of the molecules of a fluid (liquid or gas) into another medium. Diffusion results from the kinetic energy of the molecules and is therefore speedy in gases, slower in liquids and almost negligible in solids. Dimethyl Butadiene CH2C(CH3)C(CH3)CH2, a diolefin from which was manufactured ‘methyl rubber’ in Germany during World War I. DIN Abbreviation for Deutsche Industrie Normen German Industrial Standard. The organisation issuing these standards is the Deutscher Normenausschuss (DNA), the German equivalent of the BSI. Dinitroso-Pentamethylenetetramine DNPT, blowing agent. DINP Abbreviation for diisononyl phthalate, plasticiser. Dioctyl Phthalate An organic (ester) compound used as a plasticiser in nitrile rubbers and in polyvinyl chloride. Diolefin A hydrocarbon of the ethylene series, containing two double bonds in the molecule. Dipentamethylene Thiuram Tetrasulphide DPTT, accelerator. N,N´-Diphenyl Guanidine DPG, accelerator. N,N´-Diphenyl-p-Phenylenediamine DPPD, antidegradant – staining. Dipping A method of manufacturing rubber articles by dipping a former of the shape required into a rubber ‘solution’ or into compounded,
concentrated latex which may be either unvulcanised or vulcanised. Direct Moulding of Footwear A method of manufacturing footwear by simultaneously forming and vulcanising the rubber sole and heel direct to a leather upper, as compared to moulding the unit separately and sticking it to the upper. Dispersion The uniform distribution of particles throughout a medium, e.g., particles of compounding ingredients in rubber. Dithiocarbamates A class of very fast accelerators for rubber, particularly useful in latex work. The principal member of the class is zinc diethyl dithiocarbamate. DMC Abbreviation for dough moulding compound. DMS Abbreviation for direct moulded soling. See Direct Moulding of Footwear. DMTA Abbreviation for dynamic mechanical thermal analysis. DNPT Dinitroso-pentamethylenetetramine, blowing agent. DOA Di-2-ethylhexyl adipate, ester plasticiser. Doctor Knife or Doctor Blade (1) The blunt-edged blade which spreads rubber dough on to fabrics in the spreading process. (2) A blade fitted to a refiner mill to enable the thin sheet of rubber to be removed. (3) An elastomeric (usually polyurethane) blade used to clean the rollers in laser printers and copiers. Dolly A roll of masticated rubber cut from an open mill, also known as a pig. Dolomite Calcium magnesium carbonate, inorganic filler. DOP Abbreviation for dioctylphthalate, a plasticiser for natural and synthetic rubbers. DOPD N,N´-Bis(1-ethyl-3-methylpentyl)-pphenylenediamine, antidegradant – staining. DOS Di-2-ethylhexyl sebacate, ester plasticiser. DOTG Abbreviation for diorthotolylguanidine, an organic accelerator. Double Bond Also termed bivalent gap and ethylenic linkage. The type of bond in which two valency bonds link two atoms in a molecule. It is typical of compounds showing unsaturation, such as ethylene. A double bond does not indicate extra strength of the bond but rather chemical instability and reactivity. Doubling Sticking two layers of uncured rubber or rubbered fabric together and consolidating them by applying pressure in a doubling machine or doubling calender. In textile technology doubling
is the twisting together of two or more threads to make yarn for weaving of fabrics, and also the operation of combining and twisting yarns to make cord for use in pneumatic tyre casings. Dough Rubber compounded and swollen in solvent and worked on a ‘wet’ mill until it reaches the consistency of dough. It is then applied behind the doctor blade of a spreading machine through which the fabric to be coated is passing. Selfcuring doughs are used in the repair of rubber products (tyre tread cut-filling) and the splicing of belting. Dough Moulding Compound A plastics material of particular application in electrical components. It consists of a thermosetting polyester resin, mineral fillers, fibrous reinforcement and a liquid crosslinking medium such as diallyl phthalate. Down-Stroking Press In a conventional rubber moulding press the main ram travels upwards. In a down-stroking press the main ram is situated above the movable top platen to which pressure is applied by a downward movement of the ram. DPG Abbreviation for diphenylguanidine, an organic accelerator. DPPD N,N´-Diphenyl-p-phenylenediamine, antidegradant – staining. DPR Abbreviation for depolymerised rubber. DPTT Dipentamethylene thiuram tetrasulphide/hexasulphide, accelerator. DPTU 1,3-Diphenyl-2-thiourea, accelerator. DRC Abbreviation for dry rubber content, generally of latices and similar dispersions. Drafting Apron A driven, fabric reinforced, beltlike component over which loosely formed textile fibres (slub) are drafted (orientated and drawn) to improve yarn formation and consolidation. Two aprons work face to face, between which the yarn being formed is drawn. The aprons separate two sets of cots and fluted steel rollers, revolving at different speeds to create the stretching required. Drop In curing thick articles in open steam it is sometimes necessary to reduce the temperature of cure at the end of the ‘hold’ period at a slow yet uniform rate. This part of the cure schedule is the ‘drop’. Drug Room An obsolescent term for compound room - the area where the elastomers and compounding ingredients are weighed out in the proportions called for by the compound formula, prior to the mixing process. Dry Said of uncured rubber surfaces which have lost their natural tack.
Rubber Basics Dry Heat Cure Also called hot air cure. A method of curing, mainly used for footwear. The articles are placed in a double-walled vulcaniser, the heat for curing being obtained from steam circulating between the double walls. Steam does not therefore come in contact with the articles in the vulcaniser itself. Dry Rubber Compound The use of compounds based on solid elastomers (natural or synthetic) as opposed to their use in the latex or ‘wet’ form. Dry Saturated Steam Steam at the same temperature as the water from which it was formed, but not containing any particles of entrained water. DSC Abbreviation for differential scanning calorimetry. DTBP Di-tert.-butyl peroxide, organic peroxide. DTDM 4,4’-Dithiodimorpholine, vulcanising agent. Duck A strong, firm, tightly woven, durable fabric usually of cotton but sometimes of linen, hemp or other fibres. It is produced in a variety of weights. Dunlop Process A method of manufacturing latex foam. Compounded latex is foamed and gelling agent added; the mould is filled and the gelled foam vulcanised by steam at 100 °C; the product is stripped from the mould, washed and dried. See Talalay Process. Durometer An instrument for the determination of the hardness of vulcanised rubber. The name is usually, but not necessarily, applied to a pockettype instrument made by the Shore Instrument and Manufacturing Co. Inc. The use of the term in the sense of hardness (a durometer of 60°) is not recommended. Dusting The operation of applying a dusting agent to rubber. Dusting Agent Any powder or liquid used for reducing the surface tack of unvulcanised rubber. Dry dusting agents are traditionally applied to rubber by the very uneconomical and unhealthy procedure of shaking a cloth bag containing the powder over the rubber surface. Extrudates may be coated by passing them through a chalk ‘tank’ between rotating brushes. Dynamic Mechanical Thermal Analysis This is very useful for generating modulus versus temperature data on rubber compounds. The effects of temperature on this important material property can be obtained over a wide temperature range (typically –150 to +200 °C), along with the glass transition temperature and information on thermal stability. Dynamic Properties The study of the response of elastomers to forces which produce changes of motion in them. See Heat Build-up, Hysteresis and Resilience.
Dynamometer Any apparatus used for the measurement of power. Various types of dynamometer are used in the testing of pneumatic tyres and belting.
( EACM Abbreviation for ethylene-acrylic terpolymer. EAM Abbreviation for ethylene-vinyl acetate. EBC Abbreviation for estate brown crepe. Ebonite Also known as vulcanite and (mainly in the USA) ‘hard rubber’. The hard, horn-like product obtained when natural rubber and some synthetic rubbers such as nitrile (NBR) are vulcanised with a high proportion of sulphur or organic nonsulphur vulcanising agent. Butyl rubber and polysulphide rubber do not form ebonites. Ebullioscopy A technique for determining the boiling point of liquids, especially for determining the alcoholic strength of a mixture by the temperature at which it boils. The method has been used to give an indication of the molecular weight of a substance by observing the elevation of the boiling point of a dilute solution of the substance in a suitable solvent. Eccentricity Displacement with reference to a centre; an offcentre condition of, say, a cable conductor in relation to its rubber covering, a section of tubing thicker on one side than the other, or a lateral displacement of the two halves of a circular mould. See Off Centre. ECETOC European Centre for Ecotoxicology and Toxicology of Chemicals. ECO Epichlorohydrin copolymer with ethylene oxide. EDAX Energy dispersive analysis combines SEM and XRF and is used to analyse small samples, sample surfaces or contaminants in samples. EFA Formaldehyde-ammonia-ethyl chloride condensation product, accelerator. Efficient Vulcanisation A term applied to vulcanisation systems in which sulphur or a sulphur donor is used very efficiently for crosslinking the rubber. EV systems produce vulcanisates with crosslinks that are mainly monosulphidic, which are thermally and mechanically stable. Elasticity The ability of a material to regain its original shape, on removal of the force which has caused the change of shape. Elastomer A collective term for rubber and rubber-like substances. Tree rubber is a natural elastomer and man-made rubbers are synthetic elastomers. Electric Strength An alternative term for dielectric strength.
Electrode A conductor whereby an electric current is led into a liquid or a gas. The positive electrode is the anode, the negative one is the cathode. Electrodecantation A method of concentrating latex by passing an electric current through the latex contained in a rectangular tank. The rubber particles move toward the anode and also tend to rise because of their lower specific gravity. The separation is facilitated by a large number of semi-permeable membranes fitted between the electrodes. Electrodeposition A process, now obsolescent, of forming rubber articles on an anode by the migration of coagulating ions resulting from the passage of an electric current. Electrolysis Chemical decomposition of certain substances by the passage of an electric current through a solution of the substance or of the substance in a molten condition. Electrolyte A substance which, in the molten state or dissolved in a suitable solvent, conducts electricity and is simultaneously decomposed by it. Electronic Theory of Valency An explanation of valency on the basis of modern views of atomic structure. It is assumed that certain arrangements of outer electrons in atoms (‘octets’ or outer shells of eight electrons) are stable and tend to be formed by the transfer or sharing of electrons between atoms. See Covalency and Electrovalency. Electron Microscope The ordinary microscope uses a beam of light to illuminate the object; the electron microscope uses a beam of electrons which pass through the object (in the form of a very thin film of the material). Differential scattering of the beam produces an image of the object which is seen on a fluorescent screen and recorded, if required, by a camera. When the beam passes through the object this is known as a Transmission Electron Microscope (TEM). Alternatively the electrons can be used to ‘illuminate’ the surface of the object and in this case it is termed a Scanning Electron Microscope (SEM). The TEM is used on thin sections, the SEM can be used with 3 dimensional objects. Electron Spin Resonance A type of spectroscopy used in the study of molecules which contain one or more unpaired electrons. Electrostatic Spraying A method of (1) dusting uncured rubber surfaces or (2) painting a metal surface, by giving the dusting agent or powder paint a charge. The charged powder, driven by a low air pressure, is attracted to the oppositely-charged surface, thus coating it completely and evenly. Electrovalency A valency bond formed by the transfer of electrons from one atom to another.
Element A substance which cannot be decomposed by chemical means into simpler substances; a substance consisting entirely of atoms of the same atomic number. Elongation In tensile testing of rubber, elongation is the increase in the distance between bench marks on a dumbbell strip or the distance apart of the grips holding a ring test piece, on the application of a load to the test sample. It is expressed as a percentage of the original distance between the marks. Elongation at Break See Ultimate Elongation. ELS Evaporative light scattering. Embossing The impressing of a design on an uncured rubber surface by passing it through a calender fitted with an auxiliary roll engraved in the negative with the desired pattern. Empirical Formula The formula for a chemical compound which gives only the proportions of the different elements in the molecule and not their actual number, which may be calculated only from the molecular weight of the compound. Emulsifying Agent A substance added to an emulsion to increase its stability and reduce the risk of separation of the two components. In latex work soaps are widely used as emulsifying agents. Emulsion A two-phase system consisting of minute droplets of one liquid dispersed in a second liquid with which it is incompletely miscible. Emulsion Polymerisation Polymerisation of a monomer or mixture of monomers which have been emulsified with soap in water. SBR, neoprene and nitrile rubbers are manufactured by the emulsion polymerisation process. Endothermic Accompanied by the absorption of heat. Ends The warp threads of a woven fabric. EPA Environmental Protection Agency (USA) EPDM The preferred systematic abbreviation for ethylene-propylene terpolymer, also designated EPT. The use of the term EPR for a copolymer of ethylene and propylene, and the use of EPT for a terpolymer of these monomers with a small amount of a diene to provide double bonds is common but is not recommended. Epichlorohydrin 1-chloro-2,3-epoxypropane, the basis of epoxy resin and chlorohydrin elastomers. Epichlorohydrin Elastomers See Chlorohydrin Rubbers. EPM Abbreviation for ethylene-propylene rubber. Epoxide Resins Another term for Epoxy Resins.
Rubber Basics Epoxy Resins These are thermosetting viscous liquids or brittle solids, the most widely used being those based on the condensation reaction between epichlorohydrin and bisphenol A. The name is derived from the Greek prefix ‘epi’ meaning ‘over’ or ‘between’, an epoxy material being an ‘oxygen between’ compound. They are used mainly as adhesives and as surface coatings on metals, wood, other plastics and glass. EPR Abbreviation for ethylene-propylene rubber. EPSOM Syndicat des Fabricants d’Emaux, Pigments, Sels et Oxydes Métalliques EPT Abbreviation for ethylene-propylene terpolymer. Ergonomics The engineering aspects of the study of the relation between human workers and their working environment. Escalator A slatted conveyor fitted above an open mixing mill and used to increase the efficiency of mastication by cooling the rubber before returning it to the mill nip. Estate Brown Crepe Grades of crepe rubber made from lump and other high quality scrap made on rubber estates. Both Thin Brown Crepe and Thick Brown Crepe are produced, in no. 1, no. 2 and no. 3 qualities. Esters Organic compounds derived by replacing the hydrogen of an acid by an organic radical or group. Examples of ester plasticisers are tritolyl phosphate, dioctyl phthalate and dioctyl sebacate. ETAD Ecological and Toxicological Association of Dyes and Organic Pigments Manufacturers ETER ASTM designation for epichlorohydrin terpolymers. Ethane The second member of the paraffin series of hydrocarbons. It is a constituent of the natural gas found in association with oil fields. Ethanol Another term for ethyl alcohol. Ethanolamines Organic compounds derived from ethanol and amino groups (—NH2). See Triethanolamine. Ethenoid Plastics Those plastics made from substances containing an ethylenic linkage or double bond; the acrylic, vinyl and styrene groups of plastics. Ethers A group of organic compounds derived from two molecules of an alcohol by elimination of one molecule of water. The compound commonly called ‘ether’ is diethyl ether. Ethyl Alcohol The commonest alcohol (see Alcohols) and therefore often called simply ‘alcohol’. It is used as a solvent, as a fuel and in the manufacture of many other organic compounds.
Ethylene C2H4, a colourless flammable gas; first stable member of the olefin series of hydrocarbons. Ethylene-Acrylic Terpolymer This terpolymer is formed from methyl acrylate, ethylene and a carboxylic monomer. It has properties comparable to those of an acrylic. Ethylene Dichloride A liquid produced by the addition of chlorine to the ethylene double bond. It is reacted with sodium polysulphide to produce polysulphide polymers, trade name Thiokol. Ethylene Glycol A colourless, syrupy, sweet-tasting liquid; the synthetic fibre Terylene is made by condensation polymerisation of terephthalic acid and ethylene glycol. Ethylene-Propylene Rubber A stereospecific polymer produced by the copolymerisation of ethylene and propylene with Ziegler-type catalysts. Ethylene-Propylene Terpolymer An elastomer consisting of a terpolymer of ethylene, propylene and a diene, e.g., dicyclopentadiene. Ethylene Thiourea ETU, accelerator. Ethylene-Vinyl Acetate A copolymer of ethylene and vinyl acetate which processes like a plastic and performs like a rubber. The copolymer, of which there are various grades, is similar to rubber in softness and flexibility but can be injection moulded without vulcanisation. ETMQ 6-Ethoxy-2,2,4-trimethyl-1,2-dihydroquinoline, antidegradant – staining. ETU Abbreviation for ethylene thiourea, an accelerator. EU Abbreviation for polyether urethane. EV Abbreviation for efficient vulcanisation. EVA Abbreviation for ethylene-vinyl acetate. Evaporation Conversion of a liquid into vapour, without necessarily raising the temperature to the boiling point of the liquid; solutions are concentrated by evaporating off the solvent. One method of concentrating natural rubber latex is by the controlled evaporation of the liquid in which the rubber particles are dispersed. Evaporative Light Scattering This is used in polymer analysis, it involves the removal of solvent from a solvated polymer as it elutes down a drift tube and the isolated polymer particles then scatter light from the light source allowing molecular weight to be calculated. Even Speed When the rolls of a mixing mill or calender are travelling at the same surface speed they are said to be running at even speed. See Friction Ratio. Exothermic Accompanied by the giving off of heat.
Expanded Rubber A form of cellular rubber in which the cells are non-intercommunicating, self-contained units. It has low thermal conductivity. Expanded rubber is buoyant and does not absorb water and was therefore initially used in both the soft rubber and ebonite forms in the construction of lifebuoys and other marine buoyancy equipment. The most commonly used polymer is now polyurethane for both flexible and rigid systems. These products are most usually formed by moulding or extrusion processes and have a solid outer skin around the cell structure. Organic blowing agents are used for this type of process. Extender In the broadest sense, any compounding ingredient added to rubber to reduce the cost of the compound. The use of the term is now usually limited to certain cheap petroleum rubber processing oils. Extending Filler A filler which is added to a rubber with the sole object of cheapening the compound. See Reinforcing Fillers. Extensibility A term descriptive of the extent to which an elastomer can be deformed by the application of a tensile stress. Extension (1) In tensile testing of rubber, another term for elongation. (2) In rubber compounding, the addition of a high proportion (40-50 phr) of a rubber processing oil to an elastomer with the object of improving the processibility of a tough polymer and/or cheapening the compound. Extensisity Factor The surface area of a filler per cubic centimetre coming into interfacial contact with the rubber. Extraction A process for removing certain constituents of a mixture by treating it with a solvent which dissolves only the desired constituents. Extrudate A term descriptive of the product of extrusion especially where no particular shape is specified. Extruder A machine for carrying out the processing operation of extrusion; also historically termed tubing machine and forcing machine. The majority of extruders use an electrically-driven screw to force the rubber to the head of the machine, but a piston-operated type has recently been introduced. See Barwell Preformer/Ram Extruder. Extrusion The process in which unvulcanised elastomer or thermoplastic compound is forced through a die to give long lengths of a definite cross-section. The compound is normally warmed by working on a mill but in some modern machines this is unnecessary and cold stock may be used. The feed strip is led into a hopper situated over a screw which compacts the stock and forces it up to the head of the machine and through the die. In the production of tubing a core-bridge is fitted in the head. The extrusion principle is used in hose
and cable covering and in the operation of straining.
) Fabric A structure of interwoven or interlaced textile fibres, yarns or threads. Factice A compounding ingredient with the main functions of a processing aid or extender. Dark factice (sulphur factice) is produced by heating certain unsaturated oils (principally rape seed oil) with sulphur. White factice (sulphur chloride factice) is prepared by treating rape seed oil with sulphur monochloride at normal temperatures. Factice is still sometimes referred to as rubber substitute or simply ‘sub’, but these terms are not recommended. In appearance factices are friable, slightly elastic materials, the colour ranging from white to dark brown depending on the method of manufacture. Factice has been popular for many years as a lowgravity resilient filler, finding particular application in spread sheeting compounds vulcanised by the cold cure method, and in erasers where the factice content may be as high as 300 phr. In recent years work has been done on the use of factice in quite small amounts, since it has been found to have accelerating powers. Factices are available for use with most synthetic rubbers: SBR, polychloroprene, butyl, nitrile and chlorosulphonated polyethylene. Factories Acts The legislation which sets out, for the United Kingdom, the regulations governing industrial health, safety, welfare, hours of work, reporting of accidents, etc. Fahrenheit A temperature scale widely used in the US industry. On this scale 32° is the freezing point of water and 212° the boiling point. See Celsius. To convert x °F to y °C: 5(x °F – 32) = y °C 9 Farina Potato starch used as a finishing agent on proofed cloths. Fatigue The weakening of an elastomer or rubber article due to subjecting it to a continually repeated series of distortions stretching, compression, bending, or any combination of these. Fatty Acids A term applied to the whole group of saturated and unsaturated monobasic aliphatic carboxylic acids. See Oleic Acid and Stearic Acid. FDA Food and Drug Administration (USA); sets regulations for materials that come into contact with food. FEA Abbreviation for Finite Element Analysis. FEF Fast extrusion furnace grade of carbon black. See Furnace Black.
Rubber Basics Festoon An assembly of weighted or tensioned rollers for suspending long lengths of rubber or fabric in a limited space. It may be arranged to store a limited amount of fabric during temporary stoppage of a following process and may then be termed an ‘accumulator’. Fibre Often used nowadays in the sense of textile material, e.g., natural fibre, man-made fibre, but correctly it refers to the comparatively short thread (staple fibre) of natural textiles. A fibre is fine, flexible, and very long in relation to its thickness. Ficus A genus of trees yielding a good type of natural rubber, of little commercial importance nowadays. The Ficus elastica is the well-known ornamental rubber plant. FID Flame ionisation detector. Field Latex Natural rubber latex, freshly tapped, before the addition of preservatives or before concentration. FIFO The first-in, first-out principle of injection moulding; the material first plasticised is the first material to be injected. Filament A fine wire or thread. In textile technology the fine thread formed at the spinnerettes in the manufacture of synthetic and man-made fibres. See Continuous Filament. Filastic Process A method of impregnating textile fibres with latex. There is no natural affinity between the textile fibre and the latex particle; this is overcome by making the latex slightly acid and the surface of the textile strongly alkaline. Filler A compounding ingredient added to rubber for the purpose of either reinforcing or cheapening the compound. See Reinforcing Filler and Extending Filler. Fine Hard Para The best grade of wild rubber formerly obtained from Hevea trees indigenous to the Amazon Valley, and originally exported from the town of Para. Finite Element Analysis A mathematical technique developed originally for predicting the stress-strain behaviour of complex shaped objects which do not lend themselves to simple analysis. The object is broken down into a large number of simple units or elements whose behaviour can be more simply calculated. The net behaviour of all the elements is then added together to give the gross behaviour of the component. The range of applications is now very wide and includes thermal behaviour, high speed impact and fatigue. Developments in the capabilities of modern computers have opened this techniques up to a much larger spectrum of the industry and its potential has allowed designers much greater freedom and shortened the time to market of new products.
FIPG Abbreviation for formed-in-place gasket. See Flowed-In Gasket. Fire Retardant An additive used in rubber compounding to reduce the fire hazard. Firing Up Another name for burning. Fischer-Tropsch Process A process for the manufacture of hydrocarbon oils, alcohols, fatty acids, etc., from coal. FKM Abbreviation for fluorocarbon rubber. Flammability The preferred term for what is generally called ‘inflammability’; it reduces the possibility of confusion between ‘non-flammable’ and ‘inflammable’. Flap A shaped strip of rubber fitted between the beads of certain pneumatic tyre assemblies to protect the inner tube from damage by the beads and the wheel rim. Flash Another term for spew. Flash Point The temperature at which a liquid heated in a special test apparatus gives off sufficient vapour to flash momentarily on the application of a small flame. Flat Bark Crepe The lowest grade of plantation crepe rubber. It is made from earth scrap (rubber from latex which has fallen on the ground) and any other plantation salvage scrap. It was formerly called Rolled Brown Crepe. Flat Curing When the curve of a particular property (usually tensile strength) of vulcanised rubber plotted against time of vulcanisation shows a levelling off or only a slow fall after the maximum has been reached, the compound or compounding ingredient under test is said to be flat curing, to have flat curing characteristics or to show a plateau effect. Flex Cracking Repeated bending or flexing of a rubber causes cracks to develop in that part of the surface where tension stress is set up during flexing or, if this part of the surface contains a crack, causes this crack to extend in a direction perpendicular to the stress. Certain soft vulcanisates, for instance those prepared from styrene-butadiene rubber, show marked resistance to crack initiation, but it is possible for these vulcanisates to have a low resistance to growth (propagation) of cracks. It is important, therefore, to measure both the resistance to crack initiation by flexing and the resistance to crack propagation. There are various test methods, one being the De Mattia Flex Test method which is suitable for rubbers that have reasonably stable stress-strain properties, at least after a period of cycling, and do not show undue stress softening or set, or highly viscous behaviour. The results obtained for some thermoplastic rubber should be treated with caution if the elongation at break is below,
or close to, the maximum strain imposed during the test. BS ISO 132, Determination of resistance to flex cracking. Fleximers Compounds of plastic resins or rubbers used for flooring and ships’ decking. Flexometer An instrument for the measurement of heat buildup in vulcanised rubber by a forced vibration method. Flocculation That type of coacervation in which are formed large numbers of very small agglomerates of polymer particles, termed floccs. Flooring The use of rubber as a floor covering (continuous sheets, tiles or mats) was one of its earliest applications but is now being challenged by a variety of plastics, mainly PVC. Flowed-In Gasket A gasket made in situ by extruding the sealing compound on to a rotating component thereby forming a layer of compound which, after curing, becomes a gasket, solid or cellular as desired. Also known as ‘formed in place gasket’. Flowers of Sulphur A form of sulphur mainly of the rhombic variety but containing a proportion (up to 30%) of insoluble sulphur. Fluid Bed Vulcanisation A continuous process for the vulcanisation of extruded sections. The heating medium is a bed of tiny glass spheres fluidised by steam or hot air. Fluidisation The technique of passing a gas into a solid which is in the form of tiny granules and thus making the solid behave as if it were a dense, viscous liquid. Fluidised materials may be easily piped from place to place, but a particular application in the rubber industry is the vulcanisation of extruded sections. See Fluid Bed Vulcanisation. Fluorinated Elastomers Elastomers containing fluorine, also called fluorelastomers. These combine the good physical properties of organic elastomers with the thermal stability of inorganic materials. Trade names are Viton, Fluorel, Kel-F and Technoflon. FMQ Abbreviation for fluoro methyl silicone. Foam Rubber A product produced exclusively from a liquid base, e.g., latex. Latex foam has an interconnecting cell structure and is most commonly used for cushioning applications. Foamback A thin layer of rubber or plastic foam applied to knitted or woven fabrics, used mainly in the garment trade and in carpet backing. Foaming Agent A substance which assists in holding the foam structure produced by whipping or frothing in the manufacture of latex foam rubber. Footwear Rubber, thermoplastic elastomers and PVC are employed in the manufacture of a wide range of footwear: trainers, shoe soles and Wellington
boots for both industrial and sports uses. See Direct Moulding of Footwear. Forced Vibration The motion resulting from the application to a rubber specimen of an oscillating force. Forcing Another name for extrusion. Formaldehyde HCHO, a gas with an irritating smell. It is made industrially by the oxidation of methyl alcohol, and is used in the manufacture of phenolformaldehyde and urea-formaldehyde resins and plastics. Former Any specially shaped device on which a rubber product may be assembled, on which a product may be fitted to bring it nearer the cured shape or on which an article may be produced by dipping Formic Acid HCOOH, an organic acid which may be used in diluted form as the latex coagulant in the production of natural rubber. Formula (1) (Mathematics) A rule expressed in algebraic symbols; (2) (Chemistry) The representation of the kind and number of the atoms in a molecule of a compound, by means of letters and figures; (3) (Rubber Technology) The statement of the kinds and amounts of elastomers and compounding ingredients which comprise a rubber compound. FPM Abbreviation for fluorocarbon rubber. Fractional Coagulation Coagulation of natural rubber latex by stages with the object of removing the yellow colouring matter in the first fraction. The latex in the second fraction produces a white crepe rubber. See Bleaching Agent. Frasch Process A method of obtaining sulphur from underground deposits where normal mining is not possible. In Louisiana and Texas the sulphur lies beneath a layer of quicksand through which is driven a pipe carrying hot water to melt the sulphur and compressed air to drive it up to the surface. Free Radical A radical which can exist in the free or uncombined state. Such radicals are extremely reactive with themselves and with other neighbouring molecules. Free radicals are considered to take part in many reactions of importance to the rubber industry - vulcanisation, oxidation, ageing, polymerisation, etc. Free Sulphur The amount of sulphur which has not combined with the rubber during the vulcanisation reaction. The determination of the free sulphur content is widely used in assessing the state of cure of a rubber product. The addition of the free sulphur curve to the modulus and tensile/time curves of the particular compound enables the state of cure of the vulcanised product to be estimated. French Chalk A hydrated magnesium silicate in the form of a soft white powder. It is used as a dusting agent,
Rubber Basics D2230 gives full details of the die and procedures used.
as an embedding agent in open steam vulcanisation and as an extending filler. Also called talc or soapstone and often referred to simply as ‘chalk’. Freshening (1) Generally, the restoration of the tack of an uncured rubber surface by washing with solvent. (2) Used in the sense of warming up rubber compound prior to calendering or extrusion. Friction See Coefficient of Friction. Frictioning A calendering process in which hot soft unvulcanised rubber compound is applied to a fabric. The cloth passes between the bottom and middle bowls of a three-bowl calender; it travels at the speed of the bottom bowl and the faster middle bowl shears the rubber into the pores of the fabric. Friction Ratio The ratio of the relative surface speeds of adjacent mill or calender rolls; usually given in the form 1.25:1, where the 1 represents the speed of the slower roll. Frosting A dulling of the surface of vulcanised rubber articles considered to result from the action of atmospheric ozone, particularly in conditions of high humidity. It is quite different from blooming. Frozen Rubber Raw natural rubber which has been kept at temperatures lower than about 10 °C (50 °F) becomes extremely hard or ‘frozen’ and must be softened by heating before it can be processed satisfactorily. FSA Food Standards Agency (UK). FT Abbreviation for Fine Thermal Carbon Black. The only form of thermal black now in common use is Medium Thermal (MT) black. See Thermal Black. Furnace Black A type of carbon black produced by burning natural gas or oil in a large furnace with a supply of air much lower than that required for complete combustion. The main types are super abrasion (SAF), intermediate super abrasion (ISAF), high abrasion (HAF), fast extrusion (FEF), general purpose (GPF), conductive (CF) and semireinforcing (SRF). FVMQ Abbreviation for fluoro vinyl methyl silicone.
Gas Chromatography GC is used in rubber analysis to obtain polymer type information by use of a pyrolysis approach, also to identify some additives. Gasket A flat sheet or shaped section of rubber compound or rubber textile composite fitted between two metal faces to make a fluid-tight joint. Gauge (1) Any instrument for measuring, e.g., pressure gauge, thickness gauge, strain gauge. (2) Sometimes used to mean ‘thickness’, e.g., a ‘gauge’ of 3 mm. (3) Also used as a verb, to measure thickness. Gauge Pressure Pressure shown by a gauge; pressure above the pressure of the atmosphere. See Absolute Pressure. Gauze (1) A light-weight fabric of open texture. (2) A similarly constructed arrangement using wire instead of textile threads. GC-MS Gas chromatography-mass spectroscopy is used to obtain extensive compositional information on rubbers. It can identify minor components of the sample such as the breakdown products of the cure system and the antidegradants. Geer Oven An electrically heated oven supplied with circulating kit, originally used in accelerated ageing tests. Gehman Test A method of determining the stiffening of vulcanised rubber at low temperatures by submitting the rubber to torsion, as in BS 903A13. Gel Chemically, a colloidal solution which has set to a jelly. The term has a special significance in rubber technology. See Bound Rubber, Carbon Gel. Gelation Setting to a jelly: in latex processing it is a type of coagulation in which very little separation of the aqueous phase takes place during the gel formation. Gel Permeation Chromatography The molecular weights of high polymers are normally measured by gel permeation chromatography (GPC) where both an average molecular weight and a molecular weight distribution are determined. A solution of the polymer is prepared which is then passed through a chromatographic column. The speed at which
* Garvey Die A small die of base of approximate dimensions 9/16 in by 1/4 in, having a shape approximately that of a vertical section through a shoe last as per the figure below. It is used in a laboratory extruder to evaluate the extrudability or processibility of a rubber compound. ASTM
the solution passes through is determined by the molecular weight of the polymer. At the end of the column there is a detector which establishes the concentration of the polymer in the solvent. Detectors can be based on viscosity, infrared absorption spectra or light scattering. Gland A device for preventing leakage at the point where a reciprocating or rotating shaft emerges from a cylinder or vessel containing a fluid under pressure. Glass Hardening See Glass Transition. Glass Temperature Another name for glass transition temperature. Glass Transition On lowering the temperature to which an elastomer is exposed the resulting changes are simple stiffening, crystallisation and glass transition (second order transition) shown by a rapid change in physical properties within a narrow temperature range. It is convenient to characterise a particular vulcanisate by the temperatures at which the stiffness is double or ten times that at room temperature, T2 and T10, and also by the temperature (Tg) at which the stiffness changes most rapidly. Glass Transition Temperature Also termed ‘glass temperature’ or Tg. The temperature at which the stiffness of an elastomer subjected to low temperatures changes most rapidly. If the glass temperature is close to the operational temperature the material will be ‘leathery’ in its behaviour rather than rubber-like. Approximate glass transition temperatures for different polymers are NR –70 °C; SBR –52 °C; IIR –75 °C; PCP –40 °C and silicone rubber –85 °C. Glycerine Glycerin, glycerol. A thick, syrupy, sweetish liquid used as a plasticiser, a mould lubricant and as a raw material for the manufacture of glyptal resins. Glyptal Resins Resins used as surface coatings prepared from glycerol and phthalic acid, now termed alkyd resins. Goodyear Charles Goodyear (1800-1860) is acknowledged by some as the discoverer of vulcanisation by the heating of a rubber-sulphur mixture. Many others including Ludersdorf and Hancock were also researching means to impart long term stability to rubber at around the same time. Goodyear did not patent his discovery until 1844, whereas Hancock obtained a British Patent for a process of vulcanisation in 1843. Gooseneck Press A type of daylight press in which the frame holding the platens is in the shape of a gooseneck or swan-neck thus permitting full access to three sides of the platen area. Gough-Joule Effect When rubber is stretched adiabatically (without heat entering or leaving the system) heat is evolved. The effect was originally discovered by
Gough in 1805 and re-discovered by Joule in 1859. See Wiegand Pendulum. GPC Abbreviation for gel permeation chromatography. GPF Abbreviation for general purpose furnace carbon black. See Furnace Black. GPO Abbreviation for copolymer of propylene oxide and allyl glycidyl ether. Graft Copolymer A copolymer in which chains or branches of one polymer are grafted on to the main chain of the other polymer. See Block Copolymer and Heveaplus. Grain Difference in physical properties along and across a section of rubber compound resulting from the passage of the rubber through a mill nip, a calender nip or through an extruder die. See Calender Grain. Green ‘Raw’ or ‘uncured’. Green Budding An improved technique of bud grafting which may reduce by up to twelve months the nonproductive period in the life of the rubber trees, i.e., between planting and first tapping. Green seedlings of 1/4 in to 1/2 in diameter, perhaps only three months old, are used as the rootstock in place of 12-month-old woody seedlings. Instead of using budwood as the grafts, dormant buds derived from green cuttings are used. Grinding Passing rubber compound through a tight nip of either a mill, a calender, or more usually a refiner to break down any agglomerates of compounding ingredients. Vulcanised scrap rubber may be reduced to crumb rubber by a grinding process. Ground Rubber Another term for crumb rubber. Guanidine Guanidine itself is imido-urea, but the term ‘guanidines’ usually refers to the accelerators of vulcanisation, diphenylguanidine and diorthotolylguanidine. Guayule Rubber obtained from the shrub, Parthenium argentatum, native to north central Mexico and the adjacent part of Texas. The rubber is not obtained by tapping but by harvesting the shrubs and crushing the woody tissue to separate it from the rubber. Intensive research, started in 1942, has not succeeded in making guayule competitive with Hevea rubber, and since 1962 there has been no commercial production. Gum Jargon for any rubber compound during processing. See High Gum and Pure Gum. Gutta Percha A hard resinous thermoplastic substance of the same chemical composition as rubber hydrocarbon but having the trans-structure. See Cis-trans Isomerism. Formerly extensively used for the insulation of submarine cables (now superseded by polyethylene) and in the early manufacture of golf balls (now superseded by
Rubber Basics Heat Build-Up The rise in temperature which occurs when rubber is deformed. The energy used in deformation is not fully returned when the rubber recovers its original shape and the ‘lost’ energy shows as a rise in temperature of the rubber. See Flexometer, Hysteresis and Resilience. Heat Capacity Heat or thermal capacity is the ratio of the change in heat energy of a unit mass of a substance to the change in temperature of the substance; like its melting point or boiling point, the heat capacity is a characteristic of a substance. The measurement of heat and heat capacity is called calorimetry. In the metric system, heat capacity is often expressed in units of calories per gram per degree Celsius (cal/g/°C); in the imperial system, British thermal units per pound per degree Fahrenheit (Btu/lb/°F) are often used. Because of the definitions of the calorie and Btu, these two heat capacity units are equivalent; the heat capacity of pure water is 1 cal/g/°C and 1 Btu/lb/°F. Heat Distortion Temperature The temperature at which polymers cannot maintain structure or sag, it is close to the glass transition. Heater A term applied to a variety of vessels used in vulcanising rubber articles. See Autoclave and Dry Heat Cure. Also refers to heater bands used on extruder barrels and similar machines. Heat History In the processing of rubber compounds (mixing, rewarmings, calendering, extrusion) heat history is a term used to indicate the total heat which has been received by the compound, particularly the temperatures reached by the rubber and the time it has been held at these temperatures. See Scorching. Heat-Sensitive Latex Latex used in the manufacture of dipped goods using a heated former. The latex is heat-sensitised by addition of polyvinylmethyl ether (PVME) or certain polyglycols and the action of the hot former causes a layer of coagulated rubber to be deposited. Hevea Brasiliensis The most important species of the Hevea genus of the order Euphorbiaceae. All but a tiny proportion of the world supply of natural rubber is obtained from the Hevea tree originally native to the Amazon valley but now cultivated on a plantation scale in Indonesia, Thailand, Malaysia and a number of other equatorial countries. Heveacrumb Natural rubber prepared to technical specifications by a process which converts the coagulum into finely divided granules which are subsequently dried and compacted into bales. The agent which brings about the crumbling is castor oil. Heveaplus The generic name of a series of raw materials made by intimate mixture or chemical combination of natural rubber and other polymeric or resinous substances.
ionomers), but has now all but disappeared from the world market.
+ HAF Abbreviation for high abrasion furnace carbon black. See Furnace Black. Hancock Thomas Hancock (1785-1865) is designated the ‘father of the rubber industry’ and to him Great Britain is indebted for the honour of being the first country to manufacture rubber successfully as a large-scale project. His first major discovery, in 1819, was the process of masticating and mixing raw rubber. His subsequent claim, in his Personal Narrative published in 1857, that this ‘was unquestionably the origin and commencement of the India-rubber manufacture, properly so called’, has been amply verified since. Hank A length of yarn which has been wound on a reel; also the standard length of yarn (which varies with different textiles) used in calculating yarn counts. Hardness Since all practical methods of measuring the hardness of rubber involve measuring the resistance to indentation, hardness may be defined simply as ‘resistance to indentation’. Hardness is an expression of the elastic modulus of the rubber. More specifically, the load required to press a ball of given diameter to a given depth into the rubber is proportional to its elastic modulus. See Hardness Testing, Pusey and Jones Plastometer, Microhardness Testing. Hardness Testing The determination of the hardness of rubber. Instruments are either dead-load (non-portable) or spring-loaded (pocket) type (BS 903-A26). See Durometer, IRHD. Hard Rubber Another term for ebonite. HBS Abbreviation for the organic accelerator cyclohexylbenzothiazole sulphenamide, also abbreviated to CBS. HCR Abbreviation for high consistency rubber, e.g., a type of so-called solid silicone rubber. HDI Hexamethylene diisocyanate. See Isocyanate. Heat (1) Energy possessed by a substance in the form of kinetic energy of its molecules. Gain or loss of heat may result in a rise or fall in temperature of the substance, or in a change of state (solid to liquid to gas). The term ‘heat’ is sometimes used in industry where temperature is meant. See Latent Heat and Sensible Heat. (2) In the rubber industry a ‘heat’ is a number of products comprising a press or autoclave load vulcanised at the same time.
Hexamethylene Tetramine Also known as hexamine, hexa or HMT, a oncepopuIar aldehyde-amine type of accelerator for natural rubber, now used as a vulcanising agent for polyacrylate rubbers. Hexane A solvent for natural and most synthetic rubbers except nitrile. It is a petroleum spirit existing in five isomeric forms; normal hexane has a boiling point of 69 °C. HF or High Frequency Heating Another term for dielectric heating. HFA Abbreviation for higher fatty acids. HFP Abbreviation for hexafluoropropylene. High Gum Compound A rubber compound containing elastomer, curatives and the minimum of fillers. Also called a pure gum compound. High-Level Tapping Another term for ladder tapping. High Polymer A chemical compound consisting of groups of atoms which are repeated almost indefinitely until very high molecular weights are achieved. High Styrene Resins Copolymers of styrene and butadiene with styrene content of 75-90%. They are organic nonblack reinforcing materials and find their greatest application in leather-type shoe soles. They facilitate the easy processing of relatively hard compounds due to a high degree of thermoplastic behaviour. High Yielding A term applied to clones of Hevea trees which give a much higher yield of latex than ordinary rubber trees. The average yield in the 1950s was under 500 kg of rubber per hectare per annum. It is now more common to achieve a two- to threefold increase on these figures from modern planting material. HMT Abbreviation for hexamethylene tetramine. HNBR Abbreviation for hydrogenated nitrile rubber. Hold The part of a cure schedule during which the temperature is held at a specified figure. Holland Cloth A plain weave cotton fabric filled with a starchy substance to give it a glossy, non-adherent surface. It was formerly much used to preserve a fresh tacky surface on unvulcanised rubber (tyre, tube and belt repair patches) but has been almost completely superseded by polyethylene film. Holofol A process for making hollow rubber articles from a single sheet of calendered unvulcanised rubber. The surface of the sheet is semi-vulcanised and the application of a swelling agent causes the sheet to split thus forming the hollow article, the vulcanisation of which is completed thereafter. Homopolymer Polymer resulting from the polymerisation of a single monomer.
Hooke’s Law Within the limits of elasticity of a material, tension is proportional to extension, or strain is proportional to the stress producing it. Hose Flexible tubing for the conveyance of fluids (fluidised solids, liquids or gases); the construction, which includes textile and/or wire reinforcement, varies according to the pressure and the type of fluid. Hose is of two main types, delivery hose for handling fluids under pressure, and suction hose where the fluids are conveyed at pressures lower than that of the atmosphere. Hoses may convey water, steam, compressed air, chemical liquids and gases, crude oil, organic solvents, edible fluids, etc. Some types of hose are required to withstand internal pressures as high as 170 MPa at temperatures as low as ~60 °C or as high as 150 °C. One development is a floating hose whereby tankers can lie offshore and discharge to the land terminal through the hose, without the need for a deep-water jetty. The three basic parts of a hose are the rubber lining, the reinforcing element and the rubber cover. Reinforcement includes fabric, braided yarns and wire braids together with wire helices; the rubber lining is made from an elastomer chosen to suit the fluid being conveyed, while the cover compounds are designed to give maximum abrasion resistance, to resist external heat and the swelling effect of oils and solvents. See Lead Moulded Hose. Hot Air Curing Another term for dry heat cure. Hot Mastication Mastication which is carried out at temperatures exceeding 115 °C. In hot mastication, the plasticising effect results from oxidative reactions. See Cold Mastication. HPLC High performance liquid chromatography, used in analysis to identify and quantify additives. HSE Health and Safety Executive (UK). H-Test A method of measuring the adhesion between tyre cord and rubber. The test takes its name from the shape of the test specimen, two end strips of rubber with the interconnecting cord forming an H-shape. HTV Abbreviation for high temperature vulcanising. Humidity See Relative Humidity. Hydraulic Accumulator See Accumulator. Hydraulic Pressure Pressure resulting from the application of a force to a liquid medium, usually water or oil. Since liquids are virtually incompressible, applied forces are transmitted equally in all directions. In the rubber industry hydraulic pressure is supplied at various pressures (e.g., 2, 7, 14 MPa) depending on the requirements of the operation.
Rubber Basics Hydraulic Ram The solid metal cylinder or plunger which is moved by hydraulic pressure to operate the apparatus, e.g., daylight press, autoclave press, bale splitter, etc. The ram diameter and hydraulic pressure determine the press tonnage. Hydrocarbon A chemical compound consisting solely of the elements hydrogen and carbon. Hydrogen Ion Concentration The number of grams of hydrogen ions per litre of solution; it is a measure of the acidity or alkalinity of a solution. The pH of a solution is –log(hydrogen ion concentration) and ranges from 0 (highly acid) through 7 (neutral) to 14 (highly alkaline). Hydrometer An instrument for measuring the specific gravity of liquids. It consists of a weighted bulb with a thin graduated stem; it floats vertically in the liquid to be tested and the specifc gravity is read off at the point where the liquid level meets the stem. Hydrophilic A substance which readily forms a solution in water or is readily wetted. Hydrophobic A substance which forms a solution in water only with difficulty. A hydrophobic surface will not be wetted, the water tending to form large droplets. Hygrometer An instrument for measuring the relative humidity of the air. Hysteresis When rubber is deformed the difference between the energy input and output is known as hysteresis. The loss of energy is consumed in internal friction and results in heat build-up. See Hysteresis Loop and Resilience. Hysteresis Loop A graphical representation of the energy loss due to hysteresis.
ICT Imaging chemiluminescence technique. Chemiluminescence analysis is suitable for studying the early stages of the thermal oxidation of rubbers. A weak emission of light formed by chemical reactions appears during the oxidative degradation of hydrocarbons. This technique can be used to depth profile the oxidation of rubbers. IIR Abbreviation for isobutylene-isoprene rubbers, popularly known as butyl rubbers. Impact Resilience See Rebound Resilience. Impregnation The saturation of the individual fibres of a textile with rubber. The rubber may be in the form of a rubber solution, a natural or synthetic latex. India Rubber An obsolete term for natural rubber. The ‘India’ is not the present-day India but derives from the West Indies since some of the first commercial rubber was obtained from there in the eighteenth century. Industrial Processing Cloth Fabrics used during the processing of rubber, e.g., liners (linings) and wrapping cloths, which do not become part of the finished product. Inflating Agent Similar to blowing agent but generally applied only to those gas producing substances used, in pellet form, in moulding hollow balls and toys. Infrared Radiation Radiant heat or invisible heat radiation. Infrared rays have wavelengths from approximately 7500 Angstrom units to 1 mm. Infrared Spectroscopy This is used to identify the polymer and additive types in rubber analysis. Injection Moulding A method of moulding rubber articles by injecting the warm stock into mould cavities. The injection head is similar to an extruder; the mould is fitted in a press of tonnage to suit the size of the product and the number of cavities. There are two preferred arrangements: (1) Extruder and separate injection ram, and (2) Reciprocating screw machines where the screw initially conveys and warms the material and in doing so pushes itself backwards to build up a charge of material in front of it. The screw then moves forward to inject the warm material into the mould. The end of the screw will have a non-return or check valve to prevent material flowing back along the screw under the high injection pressures. Inner Tube The part of the pneumatic tyre assembly which holds the inflation air under pressure. It is protected by the outer cover or tyre and, in giant sizes, protected from rim damage by the ‘flap’. Inner tubes are primarily made of butyl rubber. Some cycle tubes still use NR. See Tubeless. Inorganic Of mineral origin; inorganic chemistry is the study of all chemical elements and compounds, except carbon and its compounds; certain simple carbon compounds, e.g., oxides and sulphides,
, IARC International Agency for Research on Cancer. The World Health Organization (WHO) funds the IARC and carries out an ongoing program to evaluate the carcinogenic hazard of many different materials. The IARC classification is: Group 1 Carcinogenic to humans; Group 2A Probably carcinogenic to humans; Group 2B Possibly carcinogenic to humans; Group 3 Not classifiable for carcinogenicity to humans; Group 4 Probably not carcinogenic to humans. ICP Inductively coupled plasma spectroscopy, used to detect metals in rubber analysis. ICR Abbreviation for Initial Concentration Rubber, a form of natural rubber made by the Decan process. ICR-NAT Former trade name for initial concentration rubber. See ICR.
ISNR Abbreviation for Indian Standard Natural Rubber. ISO Abbreviation for International Organisation for Standardization. ISO/TC45 is the Rubber Committee of the ISO and ISO/TC61 the Plastics Committee. Isobutylene (2-methyl-1-propene). The chief monomer in the manufacture of butyl rubber. It is prepared by See thermal cracking of petroleum. Polyisobutylene. Isocyanates (1) Organic substances containing nitrogen and oxygen used in bonding rubber to textiles. They are prepared in the form of a solution of mixed polyisocyanates in an organic solvent, and added to the dip solution for impregnation or to the dough for spreading. It will also cause the polymer to crosslink. (2) A reactant used in the production of polyurethane. Isoelectric Point The hydrogen ion concentration at which a colloidal system is electrically neutral; the addition of acidic substances to, for example, rubber latex causes the pH value to move towards the isoelectric point, which is the region of minimum stability, and coagulation may take place. Isomerism The existence of two (or more) chemical compounds with the same molecular formula but having different properties owing to a different arrangement of atoms within the molecule. Isomers Chemical compounds having the same molecular formula. See Isomerism. iso-PBDT Abbreviation for isopropylthiobenzthiazole, a prevulcanisation inhibitor. iso-PCBS N-isopropylthio-NAbbreviation for cyclohexylbenzothiazyl-2-sulphenamide, a prevulcanisation inhibitor. Isoprene 2-Methyl-1,3-butadiene CH2C(CH3)CHCH2. A liquid hydrocarbon of boiling point 34 °C. It is regarded as the unit molecule of natural rubber, which is polyisoprene. Synthetic polyisoprene is marketed under a variety of trade names. Isotactic One of the terms coined by G. Natta to describe different arrangements of atoms in long-chain molecules. See Stereoregular Polymers. Isotactic Polymer Molecules that are polymerised in parallel arrangements of radicals on one side of the polymer chain. Isotopes Atoms of the same element (having the same atomic number) but differing in atomic weight. The isotopes of an element all have the same chemical properties. See Radioactive Isotopes. IUPAC International Union of Pure and Applied Chemistry.
are included in inorganic chemistry. See Organic Chemistry. Insoluble Sulphur An amorphous form of sulphur which is insoluble in rubber. It is used in rubber compounds which have to be stored for some considerable time in the uncured state without loss of tack, e.g., repair materials for tyres and belting. Since this form of sulphur is insoluble in the rubber it cannot bloom to the surface. The use of insoluble sulphur also gives some degree of scorch control since it is inactive until it reverts to the soluble form. Insulation Prevention of the passage of electricity or heat; also applied to the material which prevents such passage. Insulator A material which is a poor conductor of heat or electricity. Intensity Factor The specific activity of a filler at its interface with a rubber. Internal Mixer A machine for the incorporation of compounding ingredients into rubber or similar materials. Two rotors revolve in an enclosed chamber (see Open Mill). It is provided with a hopper for feeding the materials and a sliding or drop-door for discharge of the batch. Intrusion A method of injection moulding thermoplastics, which makes large-part moulding possible on injection equipment normally capable of moulding only small parts. The injection moulding machine fills the mould at relatively low pressures. See Injection Moulding. Ion An electrically charged atom or group of atoms. An atom which loses an electron becomes a positive ion (cation) and one which gains an electron becomes a negative ion (anion). In electrolysis anions are attracted to the anode and cations to the cathode. Ionomer A family of plastics, their main constituent is ethylene, the polymer chains being interlinked by metal ions such as sodium, potassium, magnesium or zinc. IPPD n-Isopropyl-n’-phenyl-p-phenylenediamine, antidegradant – staining. IR (1) Abbreviation for isoprene rubbers, synthetic. (2) Abbreviation for infrared. IRHD Abbreviation for International Rubber Hardness Degrees as measured according to BS 903-A26 Iron (1) The unit (1/48 in) formerly used for measuring the thickness of leather and rubber soling. (2) A strip of metal used to confine the edges of moulded products, e.g., belting, during press vulcanisation. ISAF Abbreviation for intermediate super abrasion furnace carbon black.
Rubber Basics ingress of heat. The name is also applied to the material itself.
Lake A shallow depression on the otherwise smooth surface of a moulded product, generally due to air trapping. LALLS Low angle laser light scattering. Lampblack An early form of carbon black produced by the burning of oils in a simple type of furnace. It was used in the compounding of rubber mainly as a black pigment; it has little or no reinforcing effect. Lanolin A wax-like material obtained from wool grease. It is readily absorbed by the skin and may be used to prevent dermatitis. Laser Induced Mass Analysis This is a surface analysis technique, used, for example, in examining causes of bonding failure. Latent Heat The quantity of heat required to change the state of 1 g of a substance from solid to liquid (latent heat of fusion) or from liquid to vapour (latent heat of vaporisation) without change of temperature. Latex An aqueous colloid/emulsion of rubber particles; can be up to 65% solids content; generally low viscosity compared to polymer solutions. Only rubbers produced by emulsion polymerisation or natural rubber can be found in this form. The rubber may be natural, in which case the latex is produced by the rubber tree. Latex of the main synthetic rubbers is produced by the technique of emulsion polymerisation. The term ‘latex’ has been broadened in recent years and a general definition is now ‘a stable dispersion of a polymeric substance in an aqueous medium’. Latices may be classified as natural (from trees and plants), synthetic (by emulsion polymerisation) and artificial (by dispersion of the solid polymer in an aqueous medium). They may also be classified according to the chemical nature of the polymer, e.g., SBR, nitrile, polychloroprene, etc. Natural latex was used locally in the districts in which it was found for the manufacture of crude articles such as footwear, bottles, balls, ponchos, etc. It coagulates very quickly after leaving the tree (spontaneous coagulation) and large scale use had to await the discovery of methods and materials for overcoming this disadvantage. Further, latex contains only about 30% of rubber and the transport of the 70% of water from the country of origin to the manufacturer is obviously uneconomical; methods of preservation and concentration had therefore to be developed. Once these methods were adopted it was thought that latex processes would supersede many of the conventional dry rubber processes, because technologists have long considered it illogical that the fine fluid dispersion called latex should be converted into an intractable solid which requires further costly treatment before it can be processed. The wholesale adoption of latex
Jacket (1) The hollow outer wall of a hot-air vulcaniser. (2) A removable layer of heat-insulating material applied to any process vessel to reduce heat loss. (3) A braided or woven fabric covering for certain types of hose. Joule Effect See Gough-Joule Effect.
. Kaolin See Clay. Katathermometer A thermometer type of instrument used to measure the cooling power of air on the human body. Kaysam Process A process for making hollow articles from latex. A heat-sensitised compounded latex is poured into a hollow non-porous mould which is then rotated about several axes until the latex has gelled on the surface of the mould. See Rotational Moulding. Similar to slip casting of ceramics. Ketones The series of organic compounds with the general formula RR'CO, where R and R' are univalent hydrocarbon radicals, e.g., methyl ethyl ketone; acetone is dimethyl ketone. Kevlar Trade name of aromatic polyamide materials produced by DuPont with high strength and impact resistance, hence used as reinforcement. Kieselguhr Diatomaceous earth, a fairly pure silica, formed from the skeletons of minute organisms, known as diatoms. In rubber compounding it is used as an inert filler. Kok-Saghyz The Russian dandelion, which may contain up to 10% of good quality rubber. The plants are harvested and the rubber obtained in the manner of sugar from sugar beet. It is claimed that the yield per acre approaches that of plantation rubber.
/ Ladder Polymer A high polymer made by linking the individual molecules in double chains as in a ladder, with consequent improvement in the properties of the polymer. Ladder Tapping The opening of a second tapping panel on rubber trees at a height of about 2.5 m above the ground, access to which requires the use of a ladder or long-handled tapping knife. Lagging The process of covering surfaces with a material of low thermal conductivity to prevent loss or
processes in rubber manufacture did not prove feasible, and the direct use of latex is mainly in cellular rubber (latex foam), in dipped goods and in adhesives. The treatment of latex which is to be shipped as latex differs somewhat from that which is to be made immediately into dry rubber. For short-term preservation it is customary to add a small amount of an anti-coagulant to the tapping cups Where the latex is to be concentrated and shipped as such, much greater preservation is necessary and additional ammonia is added, up to about 0.7%. For latex foam manufacture most of this ammonia must be removed, and to eliminate the de-ammoniation operation several low ammonia latices have been developed. Natural latex is concentrated by three main methods centrifuging, evaporation and creaming; electrodecantation once showed promise, but the output of latex concentrated by this method is now negligible. The principal branches of the latex manufacturing industry are latex foam and dipped goods. See Dipping, Casting, Adhesives and Rubberised Hair. Latex Resorcinol Formaldehyde A mixture of rubber latex and resorcinolformaldehyde resin used to treat man-made and synthetic textiles to improve rubber/textile adhesion. Latex Thread Rubber thread of circular section (see Cut Thread) made by extruding compounded latex through glass nozzles into a coagulating bath of acid. LATU Mixed ethyl butyl thiourea, accelerator. LC-MS Liquid chromatography–mass spectroscopy. LCM Abbreviation for liquid curing medium. L/D Abbreviation for length/diameter ratio, commonly used to describe machine barrels and screws. Leader A length of woven fabric attached to both ends of a roll of textile which is to be spread or calendered, the purpose being to ‘lead in’ and wind up the textile without damage. Lead Moulded Hose Hose which has been vulcanised by covering it with an extruded lead sheath which acts as a mould. The lead is stripped off after cure. Now superseded by modern continuous curing techniques. Leaker Any rubber product, usually rubber/textile composite, which permits the escape of air or other fluids, or permits the passage of fluids to sections of the product where it is undesirable. Leno Weave A type of weave in which the weft threads are kept apart, passing through loops formed by double-warp threads. Leno gauze fabrics were used as breakers in early tyres and belting.
Local Exhaust Ventilation. Light A term applied to a moulded product which has failed to fill out the pattern details, showing rounded edges and porosity, either surface and/or internal. It does not necessarily mean that insufficient weight of compound has been used. Light Ageing Oxidation of vulcanised rubber catalysed by light, resulting in the production of an inelastic skin and discoloration on the surface. Lignin An organic material which occurs in the woody tissues of plants. It is a by-product in the preparation of cellulose for the manufacture of paper, rayon and the cellulose plastics, and its use has been proposed as a reinforcing filler for rubber. LIM Abbreviation for liquid injection moulding. LIMA Laser induced mass analysis. Lime Hydrated or slaked lime Ca(OH)2 is an inorganic accelerator used in the curing of fluoroelastomers. In conventional sulphur cured polymers it counteracts the retardation of cure due to the presence of acidic substances in a rubber compound. Quicklime (CaO) dispersed in mineral oil or in wax/oil is used as a dessicant to reduce porosity in vulcanisates, particularly in fluid bed curing. Limestone A sedimentary rock comprising > 50% calcium carbonate. Line Pressure The hydraulic pressure in the pipeline feeding the press, bale-cutter or other hydraulically-operated apparatus. Liner A textile material used to prevent the tacky surfaces of unvulcanised rubber from adhering. The liner is often ‘treated’ to permit easy release from the rubber. Lining Another name for liner. Also used with the normal meaning as in chemical plant lining, hose lining, etc. Linkage See Valency and Double Bond. Lip Seal A gasket which effects a seal by means of a protruding lip. Liquid Chromatography–Mass Spectroscopy This is used in rubber analysis. HPLC combined with a mass selective detector enables unknown samples to be analysed. Liquid Curing Medium A heated mixture of low melting point alloys or of chemical salts used to provide the heat for curing extrudates in one method of continuous vulcanisation. Litharge Lead monoxide, PbO, formerly used as an inorganic accelerator but now mainly used as a vulcanising agent in some polychloroprene
Rubber Basics Lupke Pendulum An apparatus for the determination of resilience by a rebound method. Also called Lupke Impact Resiliometer. See Resilience. The relevant standard is BS 903-A 8, Method B, Method for determination of rebound resilience. Lutoids Easily deformable gelatinous particles which comprise part of the yellow fraction of fresh natural rubber latex. Lutoids break down on the addition of ammonia and pass into the latex serum. Linear Polymer A polymer in which the repeat units are joined end to end with no branches or crosslinks.
mixes. It has a stiffening effect on uncured rubber mixes and helps in reducing distortion in open steam curing. Lithium Catalyst A catalyst made from the metal lithium and used in the preparation of stereospecific polymers. Lithopone A co-precipitated mixture of approximately 28% zinc sulphide, 71% barium sulphate and 1% zinc oxide. It is used as an extending filler and white pigment. Loading A term used to describe the addition of fillers to a base compound; a heavily loaded mix is one containing a large proportion of fillers. See High Gum Compound. Long-Length Hose Machine-made hose with braided reinforcement, vulcanised in a lead sheath. It is available in lengths up to 500 ft, compared to the comparatively short lengths of hand-made hose. See Braided Hose and Lead Moulded Hose. Loop Selvedge A selvedge made by looping the weft thread round a wire (later withdrawn) parallel to the warp, thus leaving a series of small loops along the cloth edge, so that the thickness of the selvedge is the same as that of the body of the cloth. Low Ammonia Latices Natural rubber latices in which the customary 0.7% ammonia content has been reduced to 0.2% in conjunction with the addition of a secondary preservative, either sodium pentachlorophenate, zinc diethyl dithiocarbamate or boric acid; such latices have the advantage that the deammoniation process before manufacture is unnecessary. Low Angle Laser Light Scattering This analytical technique is used to determine polymer molecular weights. Low-Temperature Polymer See Cold Rubber. Low-Temperature Testing When testing the effect of low temperatures on elastomers it is rarely sufficient merely to enclose the standard apparatus in a refrigerated chamber; special procedures are necessary. The relevant standard is BS 903: Part A13. Method for determination of stiffness at low temperatures (Gehman test). LR Abbreviation for liquid rubber. LRF Abbreviation for latex resorcinol formaldehyde. LSR Abbreviation for liquid silicone rubber. LTP Abbreviation for low-temperature polymer. Lubricant Any substance used to prevent rubber sticking to itself or to the surface of a mould. The lubricant may be a dry powder such as soapstone or a liquid such as silicone emulsion. See Dusting Agent and Mould Release Agent.
0 Macro A prefix meaning large as in ‘macromolecular’, applied to the molecule of a high polymer. See Micro. Magnesia Magnesium oxide, MgO. Heavy calcined magnesia is used as an inorganic accelerator in ebonite; light calcined magnesia is the vulcanising agent (along with zinc oxide) for neoprene compounds. Magnesite Magnesium carbonate, inorganic reinforcing filler. Magnesium Carbonate MgCO3 is used as a reinforcing filler for white and light-coloured rubber stocks. Certain types have almost the same refractive index as rubber and are therefore useful in making transparent and translucent vulcanisates. Magnetic Rubber This is made by incorporating barium ferrite powder into rubber. The material is suitable for use where a large but thin magnet is required or where a magnet must be flexible to follow a curved surface. In sheet form, magnetic rubber is used for holding small iron or steel objects in place for handling or spraying. MALLS Multi-angle laser light scattering. Mandrel A solid or hollow metal pole used in the assembly or vulcanising of rubber products, e.g., the assembly of hand-built hose. Man-Made Applied to polymers, i.e., rubbers, fibres or plastics, manufactured by a process which reforms a naturally-occurring substance, e.g., rayon from regenerated cellulose. See Synthetic. Manometer An instrument, generally in the form of a liquidfilled U-tube, for measuring pressures of gases. Masterbatch A mix consisting of elastomer and generally only one other ingredient, the proportion of which is much higher than will be present in the final production mix. Masterbatches are used for cleanliness, convenience, accuracy of weighing small quantities of accelerators, etc. Although it
is simpler to write compound formulations initially on the basis of parts per hundred of polymer (phr), masterbatches are usually expressed on a percentage basis. The calculation of the weight of masterbatch required (or of the dispersions used in latex work) is: Weight of masterbatch = Weight of ingredient required x 100 Percentage concentration of masterbatch Mastication The softening of rubber by milling to enable the addition of compounding ingredients to be made. Mastication may be done on an open mill, an internal mixer or in a plasticator. See Cold Mastication and Hot Mastication. Matrix (1) A mould or removable section of a mould used in the repair or retreading of pneumatic tyres. Derived from the printing industry where it refers to the mould used for casting type. (2) Also used with its normal meaning of ‘that in which anything is embedded’, e.g., in a rubber mix the rubber is the matrix in which the compounding ingredients are dispersed. Maturation The process, now obsolescent, of permitting the coagulum of natural rubber to mature in the wet state before washing or smoking. Due to bacterial activity various natural accelerators are produced and the resulting rubber has a faster rate of cure than that prepared by the conventional method. MBI 2-Mercaptobenzimidazole, antidegradant – nonstaining. MbOCA Methylene bis-orthochloroaniline, crosslinking agent for polyurethane. MBS 2-(Morpholinothio) benzothiazole, accelerator. MBT Abbreviation for mercaptobenzothiazole, an organic accelerator. MBTS Abbreviation for dibenzthiazyldisulphide, an organic accelerator of the thiazole class. MDHS Methods for the Determination of Hazardous Substances (HSE documents, UK) MDI Diphenylmethane diisocyanate. See Isocyanate. MDR Abbreviation for moving die rheometer. Mechanicals Originally this term was applied to all rubber products used in association with machinery but its application has been widened in some respects and narrowed in others. Mechano-Chemical A term describing certain combinations of mechanical action and chemical reactions exemplified by, but not confined to, the mastication of elastomers. In this process it is considered that the deforming forces break the molecular chains into two pieces, with formation of free radicals at the chain ends. Such radicals may recombine, or combine with oxygen or other
radical acceptor to form stable substances, giving a permanent reduction in the molecular weight of the polymer. MEK Abbreviation for methyl ethyl ketone. MEL Maximum Exposure Limit. See Occupational Exposure Limits. Mercaptobenzothiazole An organic accelerator sold under a variety of trade names. It was first introduced in about 1920 and gained wide acceptance especially in tyre compounds due to its flat curing characteristics and the good age resistance it imparts to its vulcanisates. Mesh The opening between the wires of a screen, commonly used to describe particle size, e.g., of crumb rubber. The finer the mesh the more openings it will have per unit of width, i.e., 30 mesh describes 30 holes/inch. Metal Poisoning The action of certain metals (e.g., copper) on unsaturated rubbers, primarily natural rubber, is to catalyse the oxidative degradation of the polymer. The metal must be in an ionic form, i.e., straightforward contact with the metal such as a seal with a copper pipe will not promote such degradation. Methane CH4, marsh gas, fire damp. It is the first hydrocarbon of the paraffin series. Methanol Methyl alcohol, CH2OH, also called wood alcohol or wood spirit, since it was formerly obtained from the destructive distillation of wood. It has also been synthesised from carbon monoxide and hydrogen or by fermentation of various sugar containing crops. Used as a part replacement for petrol in Gasohol to deliver a more environmentally friendly fuel, i.e., from renewable resources. Methyl Cellulose A thickening agent for latex. Methyl Ethyl Ketone An organic solvent, used particularly for making nitrile rubber cements. Methyl Group The organic radical CH2. Methyl Rubber A synthetic elastomer produced by the polymerisation of dimethylbutadiene. It was manufactured in Germany during World War I to overcome the shortage of natural rubber. Methylene Bis-Orthochloroaniline MbOCA, crosslinking agent for polyurethane. Metrolac A hydrometer with a special scale, used for the determination of the approximate dry rubber content of latex. Mica The mineral muscovite, mainly an orthosilicate of aluminium and potassium, finely ground and used as a lubricant in rubber moulding and as an extended filler in latex compounds.
Rubber Basics Micelle In latex technology, a submicroscopic aggregation of oriented molecules; in polymer technology it is synonymous with crystallite. The term is also applied to the aggregates of soap molecules formed in emulsion polymerisation. Micro A prefix meaning very small or on a small scale; in metric units, a prefix denoting one-millionth. See Macro. Microanalysis Techniques of chemical analysis, qualitative and quantitative, employing only very tiny quantities of substances. Microbiological Deterioration See Biodeterioration. Microcellular Rubber Rubber of a cellular structure, the individual pores being so small as to be seen conveniently only with the aid of a lens. Microcellular rubber finds its greatest application at present in shoe soling. Microgel Gel present in natural rubber; when the crosslinked particles are at or below the limits of microscopic vision (0.1 μm) the gel is known as microgel. The term is also applied to similar structures in synthetic rubber. Microhardness Testing A procedure to enable hardness measurements to be made on specimens much thinner and smaller than those needed for the standard test. Normally the whole test equipment is scaled own to 1/6th of its original dimensions. Micrometer An instrument for the very accurate measurement of thickness, length, depth or angles. Micrometre The preferred term for micron (μm). Micromill A device which enables very small quantities of elastomers to be mixed with compounding ingredients. The prototype is a single-roll machine, the mixing being carried out between the roll (1½ in diameter by 3 in wide (3.8 cm x 7.6 cm)) and a steel plate (9 in long by 3 in wide (22.9 cm x 7.6 cm)). Enables batches of 0.5 g to 2.5 g to be handled. Micron A unit in the measurement of microscopic particles. It is one-millionth of a metre or onethousandth of a millimetre and is denoted by the Greek letter mu (μ). The particles of rubber in natural rubber latex vary in diameter from about 0.05 μm to 3 μm. Microscope An instrument used for obtaining magnified images of small objects. For illumination of the object microscopes may use ordinary light, ultraviolet light or a beam of electrons. See Electron Microscope. Microscopy The study of materials by the use of any type of microscope. The structure of latex, dispersion of compounding ingredients in elastomers and identification of blooms are typical uses in rubber technology.
Microtome An instrument used in preparing very thin slices of rubber for studying under a microscope, dispersion of compounding ingredients, migration and blooming of sulphur, etc. Microwave Curing Vulcanisation of elastomers by heat produced by high frequency radiation, approximately 12.5 cm wavelength, 2450 MHz. Migration The motion of particles, ions or molecules in a given direction under the influence of a force. In rubber compounding it denotes the movement of any compounding ingredient from an area of high concentration to one of low concentration. Mil A unit of measurement equal to 0.001 in; the term is occasionally used incorrectly to denote a millimetre. Mill A machine for masticating rubber, mixing rubber compounds and for warming up rubber compounds prior to calendering, extrusion, etc. See Open Mill. Millimicron One thousandth of a micron, denoted by the symbol mμ. The mean particle diameter of HAF black is about 40 mμ. The correct metric term is nanometre (nm). Mill Room That part of a factory which contains the rubber processing machinery known as mills. See Internal Mixer, Mill, Open Mill. Mineral Oils Petroleum and other hydrocarbons oils obtained from mineral sources. In rubber compounds they act as softeners and extenders. See Oil Extended Polymer. Mineral Rubber Originally bituminous materials such as natural asphalt but now a by-product of petroleum refining - an air-blown petroleum asphalt. In rubber compounding it is a tack-producing softener; in larger proportions it is classed as an extender. Misalignment Any mismatching or out-of-true condition of components of a product, parts of a mould, wheels of a vehicle, etc., which should bear a specified relationship to each other. Mix Another name for a rubber compound. Mixer Any apparatus for making homogeneous mixtures of materials used in rubber manufacture, e.g., blends of dry powders, rubber cements of solutions and rubber compounds themselves. See Internal Mixer, Open Mill. Mixing The operations carried out in a mixer. MMBI 4and 5-methyl-2-mercaptobenzimidazole, antidegradant – non-staining. Mn Number average molecular weight.
MOCA Abbreviation for 4,4-methylene bis orthochloroaniline, crosslinking agent for polyurethane. Modulus Except at very low strains, up to about 15%, the ratio of stress to strain in vulcanised rubber is not a constant. Modulus is the tensile stress (measured in MPa, lb/in² or kg/cm²) required to stretch the rubber to a given strain (or elongation); the elongation must always be stated, otherwise the expression is meaningless. A more precise expression is ‘stress per square unit (in² or cm²) at the given strain’. Modulus of Elasticity The ratio of stress to strain in a given material. The strain may be a change in length, a twist or shear, or a change in volume. Modulus of elasticity in this scientific sense must not be confused with the term modulus which has a particular significance in rubber technology. Moisture Regain The percentage moisture taken up by moisturefree textiles when exposed to a standard atmosphere, e.g., a temperature of 21 °C (70 °F) at a relative humidity of 65%. Molecular Formula Another term for Formula (Chemistry). Molecular Sieves Synthetic aluminosilicate materials having a structure with regularly spaced channels of molecular dimensions. Accelerators may be adsorbed on this structure and remain inactive at processing temperatures but are released at curing temperatures, thus preventing any possibility of scorching. Molecular Weight The weight of a molecule of a substance referred to that of an atom of oxygen as 16.000; the sum of the atomic weights of the atoms in a molecule. The molecular weight of a monomer is a definite figure calculated from its composition; in polymers the number of units making up the molecule varies considerably in one sample hence molecular weights are stated as averages and usually with reference to a polystyrene standard. The molecular weights of high polymers are normally measured by GPC (Gel Permeation Chromatography), where both an average molecular weight and a molecular weight distribution is determined. Molecular weights of cured polymers cannot be measured or even stated with any meaning as due to crosslinking, the whole article is in effect one molecule. Molecule The smallest portion of a substance capable of independent existence and retaining the properties of the original substance. Monomer A chemical compound consisting of single molecules; the term is generally applied to substances, the molecules of which may unite to form polymers. Mooney Melvin M. Mooney is best known for the development of an instrument for determining the plasticity (viscosity) of unvulcanised elastomers.
The name ‘Mooney’ is often used in referring to the value obtained on the Mooney viscometer. Mooney Scorch Test A development of plasticity determination by means of the Mooney viscometer. The same instrument is used but the temperature of operation is higher and the test is continued until the sample vulcanises. A curve of Mooney reading against time is drawn, from which the scorch and cure characteristics are estimated (BS 903-A58). Mooney Viscometer An instrument which determines the viscosity of unvulcanised elastomers by measuring the resistance of the rubber to the shearing action resulting from the motion of a rotor in the centre of the test piece (BS 903-A58). Mother Stock Another term for masterbatch. Mould (1) Any cavity of a form suitable for producing a desired shape in an elastomer; the mould may be of any material (plaster, ebonite, aluminium, cast iron, steel) of strength suitable to the means employed in moulding the product. (2) A defect in raw rubber, generally the result of fungoid growth; it was formerly common in unsmoked sheet rubber. Mould Dope Jargon term for mould lubricant or mould release agent. Moulding The process of making rubber products by shaping in a mould; vulcanisation is generally effected at the same time. See Compression Moulding, Injection Moulding and Transfer Moulding. Moulding Pressure The pressure which must be exerted on each square unit of the surface of the product for satisfactory moulding, i.e., proper consolidation and freedom from porosity. It is usually expressed in lb/in² or kg/cm². Moulding pressure is not critical for rubber (700 lb/in2, 5 MPa minimum) but is very critical for efficient moulding of the various types of plastics. Moulding pressures are calculated on the projected area of the product and should include the area of the spew groove. Mould Loading In sponge rubber moulding, the mould loading is the percentage of the mould volume which is occupied by the unblown blank of unvulcanised compound, e.g., the thickness of the blank to give a blowing ratio of 2:1 will be 1/3 of the height of the mould cavity, equivalent to a mould loading of 33.3%. The use of mould loading avoids possible ambiguity in blowing ratio, expansion, etc. Mould Lubricant Any substance used to prevent sticking of rubber to a mould surface, thus facilitating removal of the product without risk of tearing or splitting. The lubricant may be painted or sprayed on the mould surface or applied to the surface of the
Rubber Basics uncured product, depending on circumstances. See Mould Release Agent. Mould Release Agent Another term for mould lubricant but generally applied only to liquids particularly those based on silicones. Moving Die Rheometer (MDR) A particular type of rheometer developed by Monsanto, now known as Alpha Technologies. The mechanical portion of the rheometer consists of two dies forming a biconical cavity which contains the elastomeric specimen to be tested. The dies are heated and closely controlled and the torque required to oscillate one of the dies is accurately monitored. A graph of the torque against time is a clear indication of the progression of the curing reaction. As the material cures it gets stiffer and the torque increases. It has distinct advantages over the oscillating die rheometer (ODR) in that the rotor in the ODR is not heated and this mitigates against isothermal conditions. The MDR operates at much closer to isothermal conditions. MQ Abbreviation for polydimethyl siloxane. MRPRA Malaysian Rubber Producers’ Research Association MRX Abbreviation for mineral rubber. MT Abbreviation for medium thermal carbon black. See Thermal Black. Mu (μ) The symbol for micron (μm), for refractive index and for coefficient of friction. A high mu rubber (fomerly termed high hysteresis, high energy-loss or ‘cling’ rubber) is one specially developed for the wearing surface of pneumatic tyre treads to improve road holding. Mullins Effect Work done by L. Mullins on the prestressing of filler-loaded vulcanisates showed that such prestressing gives a stress-strain curve approaching that of an unfilled rubber. This work has thrown much light on so called permanent set and the theory of filler reinforcement. See Stress Softening. Multi-Angle Laser Light Scattering MALLS detectors can provide information on the branching ratio of a polymer and molecular weight. Mutagenicity The capacity of some agent or chemical substance to induce genetic changes resulting from chromosomal alterations, which changes may be transmitted from parent to offspring. Mw Weight average molecular weight. Mz Z average molecular weight.
1 Naphtha General name for mixtures of liquid hydrocarbons obtained from petroleum, coal tar or shale, used as solvents for unvulcanised rubber. Naphthylamines Amines resulting from the reaction of an amino group (-NH2), with naphthalene; they are used as rubber antioxidants. See PAN, PBN. Natta See Stereospecific Catalysts. Natural Gas A mixture of gaseous hydrocarbons, principally methane, which issues from the earth in certain areas, particularly near petroleum wells. Natural gas was the main source of carbon black until some 50 years ago when it was found more economic to use the gas for heating and produce carbon black from petroleum residues by the more efficient furnace process. Natural Rubber Rubber obtained from botanical sources. The bulk of natural rubber is obtained from the Hevea Brasiliensis tree with small amounts from other vines, shrubs and plants mainly the Guayule shrub and the Kok-Saghyz plant. See Isoprene. NBC Nickel dibutyl dithiocarbamate, accelerator. NBR Abbreviation for nitrile-butadiene rubber. See Nitrile Rubber. NCI National Cancer Institute (USA). NDI Naphthalene 1,5-diisocyanate. See Isocyanate. NDPA N-Nitrosodiphenylamine, retarder. Neoprene This name has been widely adopted for the elastomer obtained by polymerising chloroprene, i.e., polychloroprene. It is however the trade name of those types of polychloroprene produced by the Du Pont Co.which were originally called ‘Duprene’. Chloroprene rubber (CR) is the preferred term, but polychloroprene (PCP) is also popular. The original route to chloroprene (2-chloro-1,3butadiene) was acetylene-monovinyl acetylenechloroprene. Many properties of neoprene are similar to those of natural rubber, but neoprene has better oil resistance, a higher maximum operating temperature and resistance to the effects of sunlight and weathering. Neoprene also has high flame resistance due to the presence of the chlorine. It is a strain crystallising material (as is NR). The chlorine also lowers the reactivity of the double bond giving its improved environmental resistance. Nerve A term used to describe the toughness and elasticity of unvulcanised, unmasticated elastomers. Mastication reduces nerve, and, if the process is continued long enough, may destroy it altogether. See Dead Milled.
Neuberg Siliceous Earth Natural mixture of quartz and kaolinite, inorganic filler. Newtonian In a Newtonian material the rate of shear deformation is proportional to the shear stress; except at very low stresses this is not true of elastomers which are accordingly termed nonNewtonian. n-Isopropyl-n’-Phenyl-p-Phenylenediamine IPPD, antidegradant – staining. Nickel Dibutyl Dithiocarbamate NBC, accelerator. Nickel Dimethyl Dithiocarbamate NiDD, accelerator. NiDD Nickel dimethyl dithiocarbamate, accelerator. NIOSH National Institute for Occupational Safety and Health (USA). Nip The distance between adjacent rolls of a mixing mill or calender; the term is often applied also to the space between the rolls, leading to the nip proper. Nitrile Rubber The generic term applied to all elastomers resulting from the copolymerisation of butadiene and acrylonitrile. Nitrile rubbers are available with different butadiene/acrylonitrile ratios ranging from 18% to 50%, a high acrylonitrile content giving rubbers excellent oil resistance, a lower acrylonitrile content giving improved lowtemperature flexibility. Nitrile rubbers have high resistance to oils and organic solvents, and, although their mechanical properties are not as good as those of natural rubber, they are subject to much less deterioration in the presence of oils and solvents. They are not resistant to ozone attack. Nitroso Rubbers Elastomers produced by copolymerisation of a nitroso monomer with tetrafluoroethylene; they have excellent resistance to heat, to the action of solvents and to chemical attack, and are completely non-flammable. N-Nitrosodiphenylamine NDPA, retarder. NMR Abbreviation for nuclear magnetic resonance. No Mark Soling Soling which is compounded with light-coloured fillers instead of carbon black and thus does not leave unsightly marks on floor coverings. Nomogram A chart which enables the value of a variable to be read off, without calculation, from the values of one or two other known variables. Normal Latex Latex of natural rubber which has had a preservative (usually ammonia) added, but which has not been concentrated. See Concentrated Latex. Non-Staining Applied to compounding ingredients which do not cause a colour change either in the compounds in which they are incorporated or in
other materials with which they may come in contact; also applied to synthetic elastomers which contain non-staining antioxidants or stabilisers. See Staining. Non-Sulphur Vulcanisation Elastomers (natural and synthetic) employ as vulcanising agent a quantity (2.5 phr on average) of elemental sulphur. The use of any other substance (TMT, peroxides, quinones, etc.) is termed non-sulphur vulcanisation. Non-Woven Fabric A fabric made by uniting a mass of staple fibres into a continuous sheet by using the adhesive properties of a bonding agent, usually rubber latex, either natural or synthetic. In textile technology the term is applied to fabrics which are not woven, such as felted fabrics. Non-woven fabrics are now being termed bonded fabrics. NPD Nitrogen phosphorus detector. NR Abbreviation for natural rubber. NSR Abbreviation for Nigerian Standard Rubber. N-tert-Butyl-2-Benzothiazole Sulphenamide TBBS, accelerator. NTP Abbreviation for Normal Temperature and Pressure, i.e., a temperature of 0 °C and a pressure of 760 mm of mercury. Also known as STP. Nuclear Magnetic Resonance Spectroscopy A type of spectroscopy used in chemical analysis and the determination of the structure of organic compounds and polymers. Nuclear Soling A high styrene soling of microcellular rubber. The soling is termed ‘solid’ and has a density of about 0.9 g/cm². Nylon The first successful synthetic fibre. The term is applied to any long-chain synthetic polymeric amide and the best known commercial type is nylon 66 produced by the condensation polymerisation of adipic acid with hexamethylene diamine.
2 OBSH p,p’-Oxy-bis(benzene sulphonylhydrazide), blowing agent. Occupational Exposure Limits Occupational Exposure Limits (OELs) refer to airborne concentrations of substances and provide a guide to their toxicity. In the UK a list of occupational exposure limits is published by the HSE in Guidance Note EH40, which is updated annually. There are two kinds of occupational exposure limits: maximum exposure limits (MELs) and occupational exposure standards (OESs). For substances which have been assigned a MEL, the level of exposure should be reduced so far as is reasonably practicable and in any case should not exceed the MEL. For substances which have been assigned
Rubber Basics Open Mill A mill in which the rolls are exposed, in contrast to those of an internal mixer. Open-Steam Curing The method of vulcanising those rubber products which do not require the precision of shape given by a mould. The heat for curing is supplied by steam circulating openly in an autoclave, the products being supported on mandrels or embedded in chalk. See Moulding. Optimum Cure The best cure for a rubber product is always a compromise, but optimum cure may be defined as that time of cure necessary to bring a preselected property of the vulcanisate to near maximum (or minimum) value, at the same time ensuring that the other properties are satisfactory. All the physical properties of a rubber do not reach their optimum values at the same time of cure, and therefore the time must be selected so that the properties are near their optima, the most weight being given to the property considered most important. Maximum productivity is given by the shortest possible time of cure, provided the selected time and temperature do not produce an unacceptable level of defects or early failures in service. Sufficient cure must be given to prevent porosity, since badly undercured rubber will sponge at pressure release. It is better to risk a slight overcure rather than an undercure, since if the curatives are correctly chosen (in type and quantity) the compound should show a plateau effect, which means that a reasonable overcure will not have any marked effect on the physical properties of the product. Orbitread Process A process used in the retreading of pneumatic tyres, whereby the new tread rubber is applied by extruding and winding a ribbon of uncured rubber (approximately 35 mm wide and 2.5 mm thick) on to the buffed and solutioned tyre casing. Organic Chemistry That branch of chemistry which deals with the compounds of the element carbon; the simpler carbon-containing compounds (such as calcium carbonate) are usually classed with inorganic chemistry and an alternative definition of organic chemistry is the chemistry of the hydrocarbons and their compounds. Organometallic Compound A carbon compound containing a metal, in which there is a direct link between at least one carbon atom and the metal atom. Many stereospecific catalysts are organometallic compounds. Orientation The ordering of molecules, particles or fibres so that they point in the same direction. O-Ring An O-shaped rubber ring of round cross-section used as an oil seal. Oscillating Disc Rheometer (ODR) A particular type of rheometer developed by Monsanto, now known as Alpha Technologies. The mechanical portion of the rheometer consists of a biconical disc embedded in an elastomeric specimen contained in a specially designed
an OES, it will be sufficient to ensure that the level of exposure is reduced to that standard or that all reasonably practicable measures are being taken to remedy any temporary excursions. OESs are ‘health based’ limits. The exposure limits are defined in terms of long-term exposure limits (8 hour time-weighted average (TWA)) and short term exposure limits (15 minute TWA or STEL). See TLV. ODPA Octylated diphenylamine, antidegradant – staining. ODR Abbreviation for oscillating die rheometer. OEP Abbreviation for oil extended polymer. OEL Occupational Exposure Limit. See Occupational Exposure Limits. OES See Occupational Exposure Standard. Occupational Exposure Limits. Off Centre A defect in rubber products where a component has been misaligned in relation to the centre line, e.g., conductor in a cable, breaker strip in a conveyor belt or pneumatic tyre. Oil Black Masterbatch An oil extended polymer to which has been added at the latex stage a quantity of a reinforcing carbon black. Oil Extended Polymer A type of SBR with which has been mixed in the latex stage a quantity (usually 37.5 or 50 phr) of an emulsion of a mineral oil and the mixture coagulated and processed in the normal manner. Although other synthetic rubbers may be oil extended in this way, the abbreviation OEP usually refers only to SBR. See Oil Extension. Oil Extension The addition of a high proportion (40-50 phr) of a rubber processing oil to an elastomer with the object of improving the processibility of a tough polymer and/or cheapening the compound. See Oil Extended Polymer. Oil Resistance Resistance of an elastomer to swelling and ultimate degradation due to contact with or immersion in an oil. Oil Seal A rubber product designed to prevent oil leakage from bearings, rotary shafts, etc. The crosssection varies according to the particular application. Olefins (Olefines) A homologous series of unsaturated hydrocarbons having the general formula CnH2n, of which the first stable member is ethylene C2H4. Oleic Acid An unsaturated long-chain organic acid found in natural fats. Its uses in rubber compounding are similar to those of stearic acid. Open-Chain Compounds Another term for aliphatic compounds.
Ozone An allotropic form of oxygen (O3) (see Allotropy) of considerably greater degradative effect on rubber than oxygen itself. The ozone content of the atmosphere normally varies from 0.5 to 5.0 parts per 100 million (pphm) of air, but in certain areas (notably Los Angeles, USA) it may reach as much as 40 pphm of air. Ozone Cracking Cracking of the surface of stretched rubber exposed to ozone. The ozone will only crack unsaturated (i.e., containing double bonds) rubbers when they are subjected to tensile strain, the cracks are at 90° to the direction of the strain. Ozonide An unstable organic compound formed by the addition of ozone to an olefinic compound, the addition of one molecule of ozone taking place at each double bond. Ozonolysis A method for determining the constitution of organic compounds containing double bonds.
cavity. The cavity is heated and closely controlled and the torque required to oscillate the biconical rotor is accurately monitored. A graph of the torque against time is a clear indication of the progression of the curing reaction. As the material cures it gets stiffer and the torque increases. See Moving Die Rheometer. Oscilloscope An apparatus employing a cathode ray tube on the screen of which varying electric currents and voltages may be displayed as visible patterns. OSHA Occupational Safety and Health Administration, US Department of Labor. Osmosis The flow of water or other solvent through a semi-permeable membrane, i.e., one which permits the passage of the solvent itself but not the dissolved substance. Osmotic Pressure In the case of a solution bounded by a semipermeable membrane, the pressure which must be applied to drive the solvent molecules through the membrane is termed the osmotic pressure. See Osmosis and Molecular Weight. OVA Organic vapour analyser. Oven A hot air chamber used for heating or drying raw rubber, for vulcanising rubber products by the dry heat method, or for carrying out accelerated ageing by the air oven method. On the continent of Europe, the term oven is sometimes used in the sense of autoclave. Overcure Prolongation of cure beyond that time which gives the optimum cure. An overcure may be accidental due to variation in curing conditions; or deliberate as in laboratory determination of curing range, or with the object of enhancing a particular property of a vulcanisate, e.g., compression set. Overflow Another term for spew. Oxidation Combination with oxygen. On the basis of the electronic theory of valency the meaning of the term has been extended to include all reactions in which there occurs an increase in the ratio of the electronegative to the electropositive atoms or groups of a substance. The controlled oxidation of natural rubber produces resinous substances called Rubbones. p,p’-Oxy-Bis(Benzene Sulphonylhydrazide) OBSH, blowing agent. Oxygen An odourless invisible gas (O2) comprising approximately one-fifth of the atmosphere; it is chemically very active. Oxygen is necessary in the mastication of rubber, but also contributes to the degradation of vulcanised rubber. Oxygen Bomb Ageing Accelerated ageing carried out in a pressure vessel containing oxygen at a pressure of 300 lb/in2 and at a temperature of 70 °C. The procedure is covered by BS ISO 188.
3 P Abbreviation for (1) phosphorus, (2) propylene. PA 80 Processing aid-80, a masterbatch in the form of pressed crumb consisting of an 80:20 blend of crosslinked to ordinary natural rubber. The correct proportions of vulcanised latex and field latex are blended, coagulated and the resulting crumb pressed into 100 lb bales. The use of PA 80 confers ‘Superior Processing’ properties on any natural or styrene-butadiene rubber with which it may be mixed. See Superior Processing Rubber. PAC Abbreviation for polycyclic aromatic compounds. Packing Any material used to prevent fluid leakage in joints, flexible couplings, hydraulic glands, etc. PAH Abbreviation for polycyclic aromatic hydrocarbons. Pale Crepe Also termed ‘first latex crepe’. This is the highest quality plantation crepe rubber. Extreme care is taken in preparation to ensure that the lightest possible colour is obtained. Pallet A platform or framework of wood or metal fitted with feet or otherwise recessed so that the forks of a forklift truck may be inserted for transportation of the load (bales of rubber, bags of compounding ingredients, etc.) as a unit. PAN Abbreviation for phenyl-.-naphthylamine. Pan A jargon term for any form of autoclave. Paraffin Series A homologous series of hydrocarbons of general formula CnH2n+2, of which the first member is methane CH4.
Rubber Basics Paraffin Wax A white solid which melts in the range 50 °C to 60 °C. It is a mixture of the higher hydrocarbons of the paraffin series and is used in rubber compounding as a softener and as a processing aid in extrusion. It also acts as a protective agent against ozone attack in vulcanised rubber by blooming to the surface and forming a protective film, which replenishes itself if removed by the service conditions. Para-Quinone Dioxime A non-sulphur vulcanising agent of particular application in butyl rubber compounds, the activator being red lead. Para Rubber Hevea rubber from uncultivated trees growing in the Amazon Valley of Brazil and exported from Para, a town at the mouth of the river. Para rubber was the best variety of all wild rubber but the advent of plantation rubber steadily reduced its importance until it is now of no significance in world rubber production. Parkes’ Process Another name for cold cure, named after its discoverer Alexander Parkes. Celluloid, first known as Parkesine was another discovery of Alexander Parkes. Pascal’s Law of Fluid Pressures Pressure applied anywhere to an enclosed body of fluid is transmitted equally in all directions. This pressure acts at right angles to every portion of the surface of the container, the force per unit area being uniform throughout. Patramold Process The use of a special ebonite as the thermoplastic material in the printing process of electrotyping, a method of producing metal replicas of printing surfaces. PB Abbreviation for polybutadiene. PBN Abbreviation for phenyl--naphthylamine. PBNA Alternative abbreviation for phenyl-naphthylamine (PBN). PCP Abbreviation for polychloroprene. PCPL Pentachlorophenyl laurate, latex auxiliary. PDMS Polydimethylsiloxane, latex auxiliary. PE Abbreviation for polyethylene. Peachey Process A method of vulcanising thin rubber articles, now of historical interest only. The products are exposed successively to the gases, sulphur dioxide and hydrogen sulphide, which react to form active sulphur which brings about vulcanisation. Peaky Cure When the curve of a particular property (usually tensile strength) of vulcanised rubber plotted against time of vulcanisation shows a sharp drop after the maximum has been reached, the compound or compounding ingredient under test
is said to show a peaky cure; the opposite of flat curing. Pelletiser A machine for converting masticated rubber or mixed compound into pellet form. It consists of an extruder screw which forces the rubber through a drilled plate, the rods so formed being cut into small lengths and treated with a lubricant to prevent sticking. In some arrangements the cutting is performed underwater to improve partition. Pendulum Feed In supplying a calender with a strip of warmed compound by means of a narrow conveyor belt, the final section of the belt may be arranged to oscillate back and forth across the calender nip; the device is termed a pendulum feed. Pentachlorophenyl Laurate PCPL, latex auxiliary. Peptised Rubber Natural rubber to which has been added on the plantation a quantity of a peptising agent. Such pre-softened and easily-softened rubbers breakdown much more quickly during mastication in the factory. Peptising Agent A substance which added to rubber in very small amounts (0.1-0.2 phr) speeds up the normal mastication process and produces rubber of a given plasticity in a shorter time and with less power consumption. The accelerator MBT has a peptising action but certain thiophenols, mercaptans and particularly o-o´dibenzoylaminodiphenyl disulphide are much more effective. Perbunan The Bayer trade name for a nitrile rubber formerly known as Buna N. Perishing An inexact term for the general deterioration of vulcanised rubber. See Ageing. Permanent Set See Compression Set and Tension Set. Permeability Diffusion of a gas or liquid through a semipermeable material. The permeability of elastomers to gases varies with the elastomer type and with the gas. Butyl rubber is much less permeable to air than is natural rubber hence its use in tyre inner tubes and similar applications. The rate of permeation is generally related to the size of gas molecule, i.e., the smaller the molecule the higher the rate. The exception is CO2 which has a rate 10 to 100 times greater than that of nitrogen. Peroxide Peroxides are used in the crosslinking of rubbers. PET Abbreviation for polyethylene terephthalate. Petrochemical Any chemical derived from petroleum, the main refining processes being fractional distillation, catalytic cracking and platforming (reforming the constituents with the aid of a platinum catalyst). Since sulphur may be recovered from petroleum refining and since SBR, furnace black and processing oils are all petrochemicals it is
measures are being taken to stop the spread of the disease.
possible to visualise a vulcanised rubber derived entirely from petroleum. Petrolatum A semi-solid yellowish substance consisting of a purified mixture of hydrocarbons; also known as petroleum jelly. It is used as a softener in rubber compounding. Petroleum Naturally-occurring oil, a mixture of hydrocarbons with a small proportion of other organic compounds containing sulphur, phosphorus, oxygen and nitrogen; the exact composition varies according to source. Petroleum Oils Used as processing additives at 5-10 phr and as a rubber extender and softener at >10 phr. Petroleum Rubber Solvent A solvent for natural rubber; a petroleum distillate with a boiling range of 100-160 °C. pH See hydrogen ion concentration. Phenol A white crystalline solid, C6H5OH, with a characteristic odour. It is used in the manufacture of the phenolic plastics, of dyestuffs and of rubber antioxidants. Highly toxic, avoid skin contact. Phenol-Formaldehyde Resin Thermosetting resin produced by the reaction of phenol and formaldehyde in the presence of either an acid or an alkaline catalyst. In rubber compounding these resins are used as plasticisers and reinforcing materials. Phenyl-.-Naphthylamine One of the earliest organic antioxidants, now obsolescent due to its severe staining properties, health problems, and to the production of more effective antioxidants. Phenyl--Naphthylamine A general purpose antioxidant for natural rubber, SBR and nitrile rubbers. Staining, now obsolescent. N,N´-(m-Phenylene)Dimaleimide Diamine accelerator. Photosynthesis Synthesis by the action of light. The term is generally applied to the formation of carbohydrates from carbon dioxide and water in the presence of sunlight and chlorophyll in green plants. PHR or phr Abbreviation for parts per hundred of rubber. Phthalocyanine Dyes Dyes manufactured from the family of chemical compounds known as the phthalocyanines. Copper phthalocyanine is a pigment where, it should be noted, the copper atom is well protected by organic radicals and does not catalyse the deterioration of the rubber compound into which it has been incorporated. Phytophthora A disease of rubber trees affecting the pods and leaves. The resulting pod-rot and leaf-fall seriously reduces the latex yield. It is common in most rubber growing countries with, until recently, the exception of Malaysia, where urgent
Pick In textile technology, a weft thread; also termed a filling thread or shot. Pico Abrasion Test A type of test for determining abrasion resistance. Fixed knives, under constant load, scrape across a rotating rubber test piece. The resulting loss in weight is a measure of the abrasion resistance. Pig A roll of masticated rubber cut from an open mill also known as a dolly. Pigment Pigments are coloured, black, white or fluorescent particulate organic or inorganic solids, which are insoluble in, and essentially physically and chemically unaffected by, the vehicle or substrate in which they are incorporated. They alter appearance by selective absorption and/or scattering of light. Pigment A colouring material mixed with rubber to give the desired colour in the product. The term has been used in the sense of any powdered compounding ingredient. Pile Curing Premature curing whilst in storage also known as bin curing. Pine Tar A tar obtained by the distillation of pine wood. It is an excellent softener and tack-producing agent in rubber compounding. Piperidine Pentamethylene Dithiocarbamate An ultra accelerator of particular application in the manufacture of dipped latex products. Plain Weave The simplest type of woven fabric construction; each thread passes alternately over and under the thread it intersects. There is thus an intersection of adjacent threads at every possible point and no thread passes over or under more than one thread at a time in either direction. Planimeter An instrument for measuring by mechanical means, the area of a plane surface, the perimeter of which is traced out by a moving arm. Plantation Rubber Natural rubber obtained from cultivated trees as opposed to that obtained from trees growing ‘wild’ in the jungle. The size of a plantation varies from the large estate of several thousand acres down to the smallholdings of a few acres worked by the owner and his family. Such smallholdings produce a significant proportion of the world’s NR output. Plasticator A machine for masticating rubber. The principle is that of an extruder, the rubber being softened by working between the threads of the screw and the surface of the barrel. The best known type is the ‘Gordon Plasticator’. Now obsolete. Plasticiser Also termed softener and processing aid. A compounding ingredient which facilitates processing by making the unvulcanised compound more plastic, aids in the incorporation
Rubber Basics PMQ
of powders, reduces the processing temperature and assists mould flow. It should be noted that the softness is carried through to the vulcanisate. Plasticisers comprise fatty acids, vegetable oils, mineral oils, and esters. See Peptising Agent. Plasticity A convenient term for the rheological properties of an unvulcanised elastomer (see Rheology). It has been defined as the ‘susceptibility to, and retentivity of deformation’, and also ‘the degree of flow which takes place under given conditions of temperature and pressure’. The use of the term viscosity is a more appropriate description. Plasticity Retention Index There are obvious advantages in a technique whereby the behaviour of a rubber in a vulcanisate could be assessed by a test carried out on the raw rubber. The PRI test consists in measuring the Wallace Plasticity of the raw rubber before and after ageing for 30 minutes at 140 °C, the aged plasticity being expressed as a percentage of the unaged (BS 903-A59.2). Plasti-Corder See Brabender Plasti-Corder. Plastics A truncation of the term thermoplastics. Generally organic materials which in the manufacturing stage are caused to flow by the application of heat and pressure and thus take up a desired shape, which shape is retained when the applied heat and pressure are removed. Plastics are high polymers and are classified into amorphous and semicrystalline thermoplastics and thermosetting materials. Plastimeter An instrument for measuring the plasticity of an elastomer, e.g., Wallace Rapid Plastimeter Plastisol A paste of polyvinyl chloride and plasticiser. The name originated in the USA and is now in general use. Plastograph See Brabender Plastograph. Plastometer Any instrument for measuring the plasticity of an elastomer. See Mooney Viscometer and Williams’ Plastometer. Plateau Effect See Flat Curing and Peaky Cure. PLC (1) Abbreviation for programmable logic control. (2) Abbreviation for pale latex crepe. Plucking Tearing out of small areas of rubber from the surface of a rubbered fabric, during the subsequent assembly of the uncured product. Ply (1) A sheet of rubber or layer of rubbered fabric when prepared as a component of a composite rubber article. (2) A single yarn of a multi-ply yarn. (3) The term has wide application with its normal meaning of layer, thickness, fold or strand. Ply Separation Lack of adhesion between the plies of a composite rubber article.
Abbreviation for phenyl methyl silicone. Pneumatic Tyre An assembly of outer cover (or tyre) fitted with an inner tube and mounted on a metal rim or wheel, the inner tube is inflated with air under pressure which supports the load of the vehicle. In the tubeless tyre no separate inner tube is fitted, the outer cover itself being so constructed as to retain the inflation air. PO Abbreviation for copolymer of propylene oxide and allyl glycidyl ether. Pocket An undesired discontinuity in a rubber article (uncured or cured) resulting from ply separation or from the trapping of air during assembly or during vulcanisation. Poise The unit of viscosity of fluids in CGS units. It is measured in dynes/cm2 per unit velocity gradient. Poisson’s Ratio Poisson’s ratio is a measure of the simultaneous change in elongation and in cross-sectional area within the elastic range during a tensile or compressive test. During a tensile test, the reduction in cross-sectional area is proportional to the increase in length in the elastic range by a dimensionless factor, Poisson’s ratio. For thermosetting elastomers, typical values of 0.48 to 0.499 are seen whereas thermoplastics and metals have values of around 0.3. Polyamide The generic name given to the nylon type of polymer, which consists of short carbon chains connected by amide groups -NHCO-. See Nylon. Polybutadiene Polymerised butadiene, made by the use of stereospecific catalysts. cis-1,4-Polybutadiene is widely used in tyre tread compounds. An inherently low temperature and low loss polymer. Polycarbonates Thermoplastic materials of the polyester family, characterised by high impact strength and dimensional stability up to 140 °C. Polychloroprene See Neoprene. Polydimethylsiloxane PDMS, latex auxiliary. Polyesters Members of the family of polyurethane elastomers. Polyethers Members of the family of polyurethane elastomers. Polyethylene (PE) Tough, waxy material made by polymerising ethylene gas either at high pressure and temperature (30,000 lb/in² and 200 °C) or at atmospheric pressure and moderate temperature by the use of aluminium catalysts developed by Karl Ziegler. This ‘low pressure’, ‘high density’ or ‘Ziegler’ polyethylene has improved properties compared to the ‘high pressure’ variety—higher softening point, higher bursting strength and higher impact strength. See Stereospecific Catalysts.
Polyethylene Terephthalate A condensation product of terephthalic acid and ethylene glycol. Polyisobutylene Polymerised isobutylene, a non-vulcanisable, rubber-like polymer. See Butyl Rubber. Polyisoprene Polymerised isoprene. Naturally-occurring polyisoprenes are natural rubber (cis-form) and gutta percha (trans-form). The use of stereospecific catalysts has made possible the manufacture of synthetic cis-polyisoprene and trans-polyisoprene both of which are now available commercially. Polymer A polymer is a large molecule (macromolecule) constructed from many smaller structural units called monomers. When only one species of monomer is used to build a macromolecule, it is known as a homopolymer, two species a copolymer, three species a terpolymer. Polymeric 2,2,4-Trimethyl-1,2-Dihydroquinoline TMQ, antidegradant – staining. Polymerisation A chemical reaction by which small molecules (of monomer) are joined together to form large molecules (of polymer). Polymerisation may be effected by (a) addition, in which the polymer molecule is a multiple of the monomer molecule, (b) by condensation, in which the empirical formula of the polymer differs from that of the monomer, and (c) by copolymerisation, in which the polymer molecule is built up from two or more different monomers There are three main techniques of polymerisation; bulk, solution and emulsion. In bulk or mass polymerisation, the catalyst is added directly to the monomer and heat may be applied to start the reaction. In solution polymerisation, the monomer is dissolved in an organic solvent. In emulsion polymerisation, the monomer or monomers are stirred up with water and an emulsifying agent to form a stable emulsion. Control of the reaction is obviously much easier with either solution or emulsion polymerisation than with bulk polymerisation. Polyphenylene Oxide (PPO) An engineering plastic. It is chemically an aromatic polyether; it can be used across a very wide temperature range, from –170 °C to +190 °C. Polypropylene (PP) Polymerised propylene, a polyolefin plastic with properties similar to those of polyethylene. Polypropylene Glycol (PPG) A heat-sensitive gelling agent for latex. See HeatSensitive Latex. Polystyrene (PS) Polymerised styrene, a hard, transparent, rather brittle thermoplastic material. Polysulphide Rubbers This group of synthetic elastomers is better known under the trade name ‘Thiokol’. Polysulphide rubbers are condensation polymers of sodium polysulphide and dichloro-compounds; they have outstanding resistance to swelling by oils and solvents but tensile strength is
comparatively low; they are of particular interest in the sealant field. They are recognisable by their very distinctive and pungent smell. Polytetrafluoroethylene (PTFE) A wax-like polymer with resistance to a wide range of temperatures, high resistance to chemical attack and very low frictional resistance. It is widely used in O-rings, seals and gaskets; it may also be sintered on to a mould surface to assist the release of the product. Polythene A shortened form of the correct chemical name, polyethylene. Polyurethane Elastomers Elastomers resulting from a series of organic reactions, e.g., a polyglycol ester of adipic acid reacted with an aromatic diisocyanate and cured with water, glycol or further reaction with an aromatic diisocyanate. These elastomers have high tensile strength, very high abrasion resistance, and lower hysteresis than natural rubber. A major use is in the manufacture of foamed polymers. Polyvinyl Alcohol (PVA) A synthetic polymer which is being developed as a textile for tyre cord, etc. Polyvinyl Chloride (PVC) Polymerised vinyl chloride, one of the polyvinyl plastics. Polyvinyl Methyl Ether (PVME) A heat-sensitive gelling agent for latex. See HeatSensitive Latex. Porosity The presence of small cells or voids in rubber articles. Porosity may be unwanted due to lack of pressure during vulcanisation, or intentional as in cellular rubber. Positex The trade name for a positively-charged natural rubber latex. The normal negative charge is reversed by pouring the diluted latex into a solution of cetyltrimethyl ammonium bromide. Positex thus has greater affinity for negativelycharged textile fibres than normal latex, and is used to confer non-shrink qualities to textiles. Post Cure Refers to an operation carried out immediately following the cure proper, e.g., post cure inflation of nylon pneumatic tyres. Seals are often postcured to optimise their stress relaxation properties. See Aftercure. Pot Heater A term used to describe certain types of vertical autoclaves for the vulcanising of large-size pneumatic tyres; sometimes called a ‘kettle’. Pot Life The time a rubber solution or dough will remain usable after the addition of the curatives. Potassium Hydroxide Number In latex testing an expression for the ammonium salt content of the latex, it is the number of grams of potassium hydroxide required to decompose the ammonium salts present in 100 g of latex solids. Potting The embedding or encapsulation of articles against breakage or for protection of electrical
Rubber Basics Pressure Sensitive Adhesive A rubber-based adhesive usually applied to a backing material which may therefore be applied to a surface by quite light pressure. PRI Abbreviation for plasticity retention index. Printers Blanket Printers blankets are of several different types: (1) In presswork - a sheet of rubber used on a press platen or impression cylinder to cushion the impression in printing. (2) In lithography - a rubber coated fabric mounted on a cylinder that receives the inked impression from the plate and transfers (offsets) it to the paper. Such blankets are also mounted on the impression cylinders of sheeted gravure presses. (3) In stereotyping and electrotyping - a yielding resilient material for backing the mat or lead sheet that is pressed into the printing form to produce the mould. (4) A sheet of rubber used in newspaper and poster work on the tympan of cylinder presses to secure a smooth, but not too hard, printing surface. Processibility The ability of a rubber compound to meet the requirements of processing, i.e., to cope with the day-to-day variations in ambient temperature, in temperature of cooling water, in amount of uncured waste available, etc., while still maintaining an acceptable level of product quality. See Processing Safety. Processing A general term applied to the variety of operations required to convert a raw elastomer into finished products. See Calendering, Compounding, Curing, Extrusion, Mastication, Mixing, Spreading. Processing Safety Indicates the ability of an unvulcanised rubber compound to accept the heat history required in processing without risk of scorching. Profiling Production of long lengths of a given crosssection of rubber compound by calendering. One or more of the calender bowls are grooved (in the negative) with the profile desired, which may be cut from the solid or obtained from two easilyreplaceable half-shells fitted over the bowl. Programmable Logic Control The application of instrumentation to the automatic control of a sequence of operations, e.g., injection moulding processes. Once the mould has been loaded with inserts (assuming a rubber to metal bonded part) into the press, the operation of a push-button starts the controller which closes the press, injects the rubber, controls the cure cycle, recharges the injection unit, opens the press, operates the ejectors and presents the mould for cleaning and loading of inserts. Promoter The name given to certain nitroso-secondary aromatic amines which, added in small quantities to butyl rubber, result in improved resilience and higher tensile strength.
components, by pouring around them a vulcanisable liquid polymer such as silicone or epoxy. Powdered Rubber Unvulcanised rubber in the form of granules. It is used for dissolving in hot bitumen for making the surfaces of so-called rubberised roads Power Factor The power factor of an insulating material indicates its tendency to generate heat in service. The electrical energy loss is directly proportional to the frequency and at high frequencies only materials of very low power factor may be used as cable insulation. PP Abbreviation for polypropylene. PPD Abbreviation for piperidine pentamethylene dithiocarbamate. PPG Abbreviation for polypropylene glycol. pphr Parts per hundred rubber. PPO Abbreviation for polyphenylene oxide. PE Abbreviation for polyethylene. Precipitated Whiting Calcium carbonate produced by the chemical process known as precipitation. Precipitation The formation (‘throwing down’) of a precipitate, an insoluble substance in a fine state of division, as a result of a chemical reaction between substances in solution. Preform An imprecise term, mostly used in the sense of a blank for moulding or a subsequent process. Premasticated Rubber Rubber which has been masticated in an operation entirely separate from the mixing process proper. See Mastication and Mixing. Premix An imprecise term used sometimes in the sense of masterbatch, sometimes with the meaning of a blend of compounding ingredients for subsequent addition to the elastomer on a mill or in an internal mixer. Premix moulding is the same as dough moulding. Press Curing Vulcanisation of rubber products carried out in a daylight press. Press Table A movable platform (compressed air or hydraulically operated) which facilitates mould changing in a hydraulic press. The table is raised to the level of each daylight in turn and the mould is easily transferred from or to the platen. Press Tonnage The total pressure in tons exerted by the ram on the platens of a hydraulic press. It is calculated by multiplying the area of the ram by the hydraulic pressure and converting to tons; sometimes called press capacity or ram pressure.
Proofing Short for waterproofing, usually refers to the application of a rubber coating to fabrics by the process of spreading. Propylene CH2CHCH3, propene, the second member of the olefine series of hydrocarbons. It is the monomer used in the preparation of polypropylene and ethylene-propylene rubbers. Protective Agents Materials used to protect vulcanisates from deterioration, including surface coatings as well as the ingredients added to the rubber at the mixing stage. See Antioxidant, Antiozonant, Paraffin Wax. Protective Colloids In the manufacture of articles direct from latex it is necessary to stabilise the latex (to prevent premature coagulation) by the addition of protective colloids such as casein soaps, gelatine and proprietary anionic surface active agents. PSA Abbreviation for pressure sensitive adhesive. PSI or psi Abbreviation for pounds per square inch; although this abbreviation is very popular it has never had official approval, the correct imperial unit is lbf/in2. PSIG or psig Abbreviation for pounds per square inch gauge. See Gauge Pressure. PTFE Abbreviation for polytetrafluoroethylene. PU Abbreviation for polyurethane. Pure Gum Mix Another term for high gum compound. Pusey and Jones Plastometer This is an instrument for hardness testing and not a plastometer. The Pusey and Jones tester is used for determining hardness particularly on curved surfaces, such as rubber-covered rolls. It operates on a dead-weight principle. PVA Abbreviation for polyvinyl alcohol. PVC Abbreviation for polyvinyl chloride. PVI Abbreviation for prevulcanisation inhibitor. PVME Abbreviation for polyvinyl methyl ether PVMQ Abbreviation for phenyl vinyl methyl silicone. Pyrometer An instrument for measuring temperatures, in the rubber industry the term is usually applied to an instrument for determining the surface temperature of mill and calender rolls, moulds, etc. The instrument is usually based on thermocouples or, where higher accuracy is required, platinum resistance thermometers. Infrared (IR) techniques are now used which have the advantage of non contact but require careful calibration for the emissivity of the surface.
4 Qualitative Chemical Analysis Analysis to determine the chemical nature of the constituents of a material, irrespective of their amounts. Quality Control As well as the usual meaning of the control of quality this phrase is particularly used with reference to manufactured products. See Statistical Quality Control. Quantitative Chemical Analysis The determination of the amounts in which the various constituents of a material are present. Quaternary Ammonium Compounds Organic compounds having four alkyl groups attached to nitrogen. A quaternary ammonium salt is employed in reversing the electric charge on natural rubber latex; quaternary ammonium dithiocarbamates are ultra-accelerators for rubber vulcanisation. Quebrachitol Methylinositol, one of the constituents of natural rubber latex. Although it is present at about 1% it does not appear to have any effect on the properties of either field latex or concentrated latex. Quicklime CaO, calcium oxide, which combines with water to give slaked lime. A dispersion of quicklime in oil or in wax is now available for use in absorbing moisture and thus reducing porosity in vulcanisates especially those cured by a fluidised bed or in a molten salt bath. Quinone Dioxime See Para-Quinone Dioxime. Quinones Quinone and some of its derivatives may be used in the non-sulphur vulcanisation of natural rubber. The best-known derivative is paraquinone dioxime used as a curing agent for butyl rubbers.
5 Racked Rubber Unvulcanised natural rubber which has been cooled quickly while under tension. In this condition it behaves like a relatively inextensible fibrous material. Radial-Ply Tyre Formerly termed braced tread, rigid breaker or belted tyre. A pneumatic tyre in which the cords of the casing plies run directly across the tyre section from bead to bead, and not at an angle as in a cross-ply tyre; the breaker in a radial-ply tyre is an inextensible band which runs circumferentially round the tyre between tread and casing. It is made up of layers of bias cut fabric set at discrete angles to confer the required stability in the tread but maintain the flexibility in the sidewall. Radical (1) A molecule or atom with an odd number of electrons, often short lived, reacting rapidly with other molecules.
Rubber Basics Reclaimed Rubber The product resulting from the treatment of waste rubber (flash, used tyres, etc.) by heat and chemical agents, which effect sufficient break down and softening so that the reclaim may be used as a compounding ingredient in fresh compound without excessive degradation of physical properties. Use peaked in the 1950s and has fallen steadily since then. Recent environmental pressures have raised the profile of recycling and reclaiming and there is now much research in this field with a view to finding effective disposal methods for waste tyres. See Refining. Reclaiming The variety of processes used in the manufacture of reclaimed rubber. Reclaiming Agents Substances used to assist in the reclaiming of rubber. Many plasticisers and some peptisers function as reclaiming agents. Recovery The degree to which a raw elastomer or unvulcanised compound returns to its original dimensions on the removal of an applied stress which has caused deformation. Die swell in extrusions and increase of thickness of calendered sheet are examples of recovery. Red Iron Oxide Ferric oxide prepared for use as an inorganic colouring agent for rubbers. The colour varies according to type, brick-red, orange, bluish-red, etc. Red Lead Trilead tetraoxide, vulcanising agent. Redox Catalysis A chemical reaction employing a catalyst which includes both a reducing agent and an oxidising agent. The system is used in the production of ‘cold’ styrene-butadiene rubbers. See Cold Rubber. Reduction The removal of oxygen or the addition of hydrogen to a compound; the opposite of oxidation. On the basis of the electronic theory of valency the meaning of the term has been extended to include all reactions in which there occurs an increase in the ratio of the electropositive to the electronegative atoms or groups of a substance. Reed In weaving of textiles, a comb-like arrangement of flattened steel wires fixed in a frame. The reed keeps the warp threads in position, acts as a guide for the shuttle and beats up the weft to the cloth; it also determines the number of warp threads per inch of width of the cloth. Refiner A two-roll machine similar to an open mill but of more robust construction, having a higher friction ratio and capable of very close nip adjustment. Refining The operation of processing rubber on a refiner, the object being to break down any agglomerates of compounding ingredients or to remove small particles of scorched rubber. Refining is one of
(2) In a chemical compound, a group of atoms which maintains its identity during chemical changes which affect the remainder of the molecule. Radical Acceptor In cold mastication of rubber, a substance which prevents the recombination of the free radicals produced by the mechanical shearing forces. See Cold Mastication, Free Radical and MechanoChemical. Radioactive Isotopes These are unstable forms of elements which decay by the emission of radiation. A radioactive isotope of an element behaves chemically in the same way as the non-radioactive form, but its radiation may be detected and measured by a suitable instrument. In the rubber industry radioactive isotopes are used in beta ray thickness gauges, in studying the precise role of sulphur in vulcanisation, in the speedy determination of tread wear in tyres, etc. See Beta Rays. Ram The solid metal cylinder or plunger which is moved by liquid pressure, air pressure or a combination of both, in such machinery as moulding presses, bale splitters, internal mixer floating rams and bottom doors, etc. Ram Pressure Another term for press tonnage. Rasping The process of roughening the surface of vulcanised rubber preparatory to applying a layer of unvulcanised rubber as in tyre re-treading, conveyor-belt repairing, etc. Rate of Cure The time of vulcanisation required by the compound in question to reach a given state of cure compared to the time required by a standard compound to reach the same state of cure. Rayon This term was originally intended to denote all kinds of man-made textile fibres, but is now applied only to cellulose types. Viscose rayon (regenerated from a solution of cellulose xanthate in sodium hydroxide) accounts for the greater part of world rayon production. Acetate rayon and cuprammonium rayon are relatively unimportant. Reactor The vessel in which a chemical reaction takes place; the term is usually applied to the vessel used in pilot plant or large-scale commercial processes. Rebound Resilience Resilience measured by an impact or rebound method. See Lupke Pendulum, Tripsometer. Recapping A tyre retreading process in which new material is applied as tread and over the shoulders of the tyre. Recipe Another term for formula. Reciprocating Screw Machine See Injection Moulding. Reclaim Another term for reclaimed rubber.
Resin Rubbers Blends of natural rubber or styrene-butadiene rubber with high styrene resins used as soling material in footwear manufacture. Such resin rubbers should not be confused with combinations of rubber and phenolic resins synthesised by a controlled chemical reaction, e.g., materials sold under the trade name ‘Fortiflex’. Resistivity Specific resistance. See Surface Resistivity and Volume Resistivity. Resorcinol m-Dihydroxybenzene, used along with latex and formaldehyde in preparing adhesives for bonding rubber to textiles. See Latex Resorcinol Formaldehyde. Retarder A compounding ingredient which retards the rate of cure of a rubber compound, thus increasing processing safety. Reticulation The formation of a network or net-like structure. In rubber technology this term was first applied to the anisotropy of carbon black particles, which were described as having a ‘reticulate chain structure’, later abbreviated simply to ‘structure’. Retracted Spew Another term for backrinding. Retreading The fitment of a new wearing surface to a worn pneumatic tyre. The operations comprise rasping to remove the remaining old tread, solutioning, fitment of unvulcanised tread and, finally, curing in a suitable press or autoclave. Reversion Degradation of a molecularly crosslinked rubber network occurring at vulcanising temperatures. All rubber compounds in which elemental sulphur is the crosslinking gent are subject to reversion, usually shown by reduced tensile strength, reducing modulus, increased elongation and the development of tackiness. RF Heating Another term for dielectric heating. RFK A rubber to fabric bonding system comprising resorcinol, a formaldehyde donor and a hydrated silica filler. Incorporated as dry ingredients in the rubber compound and activated by heat. RHC Abbreviation for rubber hydrocarbon. Rheogoniometer An instrument for the study of the rheological properties of substances. The name is usually applied to the particular instrument designed by Professor Weissenberg. Rheology The science of the deformation and flow of matter; the study of a range of phenomena extending from the plastic flow of solids to the behaviour of fluids under extreme conditions. Rheometer An instrument for the study of the rheological properties of a substance. The name has been applied to several modified versions of the Mooney Viscometer and to the Monsanto (now
the final stages in the manufacture of reclaimed rubber. Refractive Index The ratio of the sine of the angle of incidence to the sine of the angle of refraction when light passes from air into the substance in question. In compounding transparent and translucent rubbers it is advisable to choose fillers with refractive indices near to that of the rubber itself. Register In rubber moulding, those areas which contact each other when the mould is closed. Also used in the usual sense of alignment. Reinforcement (1) The incorporation into rubber of certain compounding ingredients of small particle size which confer on the vulcanisate high tensile strength, high resistance to tearing, high resistance to abrasion and some increase in stiffness. See Reinforcing Fillers. (2) The term may also be used with the meaning of structural reinforcement of rubber products, generally by combining the rubber with a textile material. Reinforcing Filler Compounding ingredients which bring about reinforcement of rubbers. The most widely used are carbon black, silica and silicates, zinc oxide, treated whitings, high styrene resins and phenolic resins. Relative Density The official ISO term for specific gravity. Relative Humidity A measure of the dampness of the atmosphere. It is the ratio of the weight of water vapour per unit volume of the air to the weight of water vapour per unit volume of saturated air at the same temperature, usually expressed as a percentage. Release Agent Another term for mould release agent. Reodorant A compounding ingredient which masks or changes the odour of a rubber product. Resilience The ratio of the energy given up on recovery from deformation to the energy required to produce the deformation, expressed as a percentage. See Heat Build-Up, Hysteresis and Rebound Resilience. Resiliometer An obsolescent name for any apparatus for measuring resilience, formerly commonly applied to the Lupke Pendulum. Resin An omnibus term for a variety of hard, brittle, solid or semi-solid organic substances. Resins may be either natural such as rosin, or synthetic such as coumarone-indene and phenolformaldehyde. Resin Cure Vulcanisation of elastomers effected by the incorporation in the compound of certain polymeric resins derived from the condensation of formaldehyde with 4-alkyl phenols. Most frequently used with butyl and EPDM compounds for enhanced heat resistance.
Rubber Basics Ross Flex Machine A machine for determining the resistance of elastomers to flex cracking. It is used particularly in the evaluation of shoe soling materials. Rotational Moulding A development of slush moulding used for the production of hollow articles from plastisols. The moulds are continuously rotated in two directions during the curing cycle. Rotocure Trade name for an apparatus used for the continuous vulcanisation of belting, matting, etc. Rotomill A continuous mixing device for elastomers, consisting essentially of a fluted rotor surrounded by a stator. Rotor In general a rotating part of a machine; in the rubber industry the term refers particularly to the contoured rolls of an internal mixer and to the mushroom-shaped rotor of the Mooney Viscometer. Rough Bore Hose Suction hose in which the fabric plies are built on to a wire helix, the wire being exposed in the bore. RPA Abbreviation for rubber process analyser. rpm Abbreviation for revolutions per minute. RSS Abbreviation for ribbed smoked sheet. RTECS Registry of Toxic Effects of Chemical Substances (USA) RTV Abbreviation for room temperature vulcanisation. Rubber The name ‘rubber’ derives from the fact, noted in 1770 by Joseph Priestley the English chemist, that caoutchouc would erase or ‘rub out’ lead pencil marks. Priestley did not actually name it rubber, but at some time between 1770 and 1778 the term became popular. Rubber Derivatives Many chemical derivatives of rubber, produced in the course of attempts to elucidate the structure of rubber, became of practical commercial value but have been superseded by the diversity of synthetic polymers. See Cyclised Rubber, Chlorinated Rubber, Rubber Hydrochloride, Rubbone. Rubber Fume The fumes given off from hot or previously heated rubber, a very complex mixture. Exposure to rubber fumes may be a factor in the increased incidence in certain types of cancer and also in the causation of some other diseases. Fume comprises visible and invisible components. The aerosol (visible) fraction is ‘rubber fume’ as defined by the UK HSE, i.e., the fume evolved in the mixing, milling and blending of natural rubber and rubber or synthetic elastomers, or of natural rubber and synthetic polymers combined with chemicals, and in the processes which convert the resultant blends into finished process dust products or parts thereof, and including any
Alpha Technologies) Oscillating Disc Rheometer. Other rheometers are the Yarsley piston rheometer and the capillary rheometer. RI Refractive index. Ribbed Smoked Sheet Plantation rubber in the form of sheets which have been dried in an atmosphere of wood smoke and finally sheeted in a mill having rolls engraved with a ribbed design. Ribbed smoked sheet comprises about 60% of the output of a plantation. See Plantation Rubber. Rigidity Modulus The ratio of shear stress to shear strain. A property which determines the rate at which elastomers stiffen as the temperature is lowered. The force required to twist the test piece through 90° is measured at each temperature and the modulus calculated from a formula. RIM Abbreviation for reaction injection moulding. Rind Another term for spew. Ring Compound A chemical compound in the molecule of which some or all of the atoms are joined together in one or more closed rings. Rise In open steam curing that period of time during which the temperature is raised gradually from room temperature to the actual curing temperature. Roelig Machine An apparatus for measuring the dynamic modulus and hysteresis of elastomers. The stress-strain oscillogram is shown on a ground-glass screen by means of an optical system. Now superseded by modern computer controlled servo hydraulic and dynamic mechanical thermal analysis machines. Roll Bending The correction of calender bowl deflection by application of hydraulic pressure to counteract the forces tending to produce deflection. Roll Crossing See Crossed Axes. Rolled Brown Crepe Former name for flat bark crepe. Rolling Ball Loss Spectrometer An instrument designed to follow hysteresis losses in polymers by measuring the resistance to the rolling of small balls over the surface of the test piece; it can investigate transitions in polymers to as low a temperature as –120 °C. Superseded by modern dynamic mechanical thermal analysis equipment. Rolling Resistance The force or effort required to maintain the advance of a rolling tyre; usually expressed in pounds per ton of load. Room Temperature Vulcanisation Vulcanisation which takes place at normal atmospheric temperature Rosin The residue remaining after the distillation of turpentine. Wood rosin is obtained by the extraction of pine wood. Rosin is used in rubber compounding as a tack-producing softener.
inspection procedures where fume continues to be evolved (EH40/2000). The maximum exposure limit of 0.6 mg/m3 (EH40/2000) relates to material as determined by the HSE method MDHS 47, ‘Rubber fume in air measured as total particulates and cyclohexane soluble material’. Rubber Hydrocarbon The hydrocarbon present in an elastomer; in natural rubber the amount varies from 93% to 96% according to type. Rubber Hydrochloride This derivative of natural rubber produced by the action of hydrogen chloride (liquid or gaseous) found application as a transparent food packaging film, but has now been superseded by modern packaging materials such as PET. Rubberised Hair A product used in upholstery and as a resilient packaging material. It is made by spraying a loose mat of curled animal hair with latex and applying heat to vulcanise the rubber. The resilience of the product comes from the fibres, the junction points of which are anchored by the rubber. Rubber Plant Lining Employing the corrosion- and abrasion-resistant properties of elastomers by applying a lining of suitable material to vessels, tanks, valves, pipes, etc., handling corrosive liquids. Rubber Powder Another term for powdered rubber. Rubber Process Analyser (RPA) A development of the moving die rheometer where the operation of the unit is fully computer controlled. The rate of oscillation, temperature and level of strain can all be run through a series of options. The torque measurements are also highly sophisticated. As a consequence, the unit can be set up to monitor processing parameters, then the cure behaviour and finally the finished dynamic properties of the cured material. It is manufactured by Alpha Technologies. Rubber Process Dust Rubber process dust is dust arising in the stages of rubber manufacture where ingredients are handled, weighed, added to or mixed with uncured material or synthetic elastomers. The aggregated maximum exposure limit in the UK is 6 mg/m3 (EH40/2000). The exception is chemicals for which specific exposure limits exist. Rubber Substitute Former name for factice. Rubber Webbing Rubber in strip form widely used in upholstery for domestic furniture and all forms of transport seating. There are two main types of rubber webbing - solid rubber and rubber reinforced with threads or fabric. There is also a woven type in which the warp threads consist of rubber filaments wrapped together in a cotton covering, the weft threads being of jute. Rubbone The trade name for a variety of resinous substances produced by the oxidation of rubber. Rubbones, designated A, B and C depending on the degree of oxidation, were once used in certain
paints and heat-resistant finishes, but are no longer available commercially. RUBIAC Rubber Industry Advisory Committee (HSC, UK). Running Nip A space where fabric, rubber sheet, rubbered fabric or similar material running over, under, or on to, a roller, makes a nip with itself or with any adjacent surface. Russell Effect The name given to the behaviour of many organic and inorganic substances in producing, especially after exposure to light, an image on a photographic plate in darkness. This effect, which is shown by unvulcanised rubber after exposure to light is considered to result from the formation of peroxides. The Russell effect shown by vulcanised rubber is very weak. Rutile One of the crystalline forms of titanium dioxide.
6 SAF Abbreviation for super abrasion furnace grade of carbon black. See Furnace Black. Safety Discs Metal discs of specified shearing strength at the end housings of a roll mill; their function is to break when the mill suffers a sudden overload, thus preventing breakage of the roll neck itself. Safety Mills Two-roll horizontal mills, the design of which conforms to the Lunn Principles for safety in operation. Salicylic Acid Used as a retarder of vulcanisation. Saturated Solution A solution which can exist in equilibrium with an excess of the dissolved substance. The amount of dissolved substance a liquid will ‘hold’ depends on the temperature. Saturated Steam Steam at the same temperature as the water from which it was formed. Saturation Saturated chemical compounds are those the molecule of which contains no double or triple valency bonds; such compounds do not form addition compounds. SBP Abbreviation for special boiling point, a term descriptive of a series of petroleum rubber solvents of different degrees of volatility. Boiling ranges are as follows: SBP 1, 31-115 °C; SBP 2, 70-95 °C; SBP 3, 100-120 °C; SBP 4, 40-150 °C; SBP 5, 90-105 °C; SBP 6, 140-160 °C. SBR Abbreviation for styrene-butadiene rubber. SBS Abbreviation for styrene-butadiene-styrene block copolymer, a thermoplastic elastomer. Scanning Electron Microscope This is used for surface analysis. See Electron Microscope.
Rubber Basics Scion In bud grafting, the shoot that develops from the grafted bud. Scleroscope An instrument for measuring the resilience of rubber by dropping a flattened steel cone vertically on the test piece and measuring the rebound. Scorching Undesired premature vulcanisation of a rubber compound during the processing operations of mixing, extruding or calendering. See Heat History. Scorch Testing The determination of the ability of a rubber compound to withstand scorching. See Mooney Scorch Test. SCR Abbreviation for styrene-chloroprene rubbers. Scrap Rubber A term which generally applies to vulcanised rubber unfit for any other use than reclaiming or grinding to crumb rubber. In the rubber factory ‘scrap’ may also refer to unvulcanised trimmings which can be reprocessed. SDBC Sodium dibutyl dithiocarbamate, accelerator. SDC Society of Dyers and Colourists SDEC Sodium diethyl dithiocarbamate, accelerator. SDMC Sodium dimethyl dithiocarbamate, accelerator. Sealants Rubber-like materials now superseding the traditional mastics and putties used in the building industry. Such sealants (also termed mastics) are based on butyl rubber, liquid polysulphides, silicone rubbers, polybutylene, nitrile rubbers and plasticised vinyl polymers. SEBS Abbreviation for styrene-ethylene-butylenestyrene block copolymer, a thermoplastic elastomer. Second-Order Transition Another term for glass transition. Secondary Ion Mass Spectrometry A surface analysis technique used in bonding failure analysis, for example. Selenium A non-metallic element with chemical properties similar to those of sulphur. It has been used as a compounding ingredient in low sulphur compounds to resist reversion and improve ageing. It is classed as a secondary vulcanising agent. Self-Curing Another term for self-vulcanising. Self-Reinforcing Elastomer A term applied to certain styrene-butadiene copolymers with a combined styrene content between 35% and 50%. Self-Vulcanising Applied to a rubber compound, dough or cement which will vulcanise at room temperature. The time taken to effect vulcanisation may be as short as 30 minutes or as long as several days.
Selvedge That edge of a woven fabric which runs parallel to the direction of the warp threads. SEM Abbreviation for scanning electron microscope. Semi-Cure A preliminary or pre-cure given to a product or part of a product, e.g., a moulding may be given a semi-cure in a press and the cure completed in open steam; a thick section of a product may be semi-cured before assembly to the product; a component may be semi-cured to reduce the flow during the subsequent vulcanisation of the product. Semi-Solid Tyre A non-pneumatic tyre which has an internal cavity which may be filled with sponge rubber or may be pressurised by inflation with an air needle. Sensible Heat The heat which produces a rise in temperature when it enters a substance. In the generation of steam it is the amount of heat which has been added to the water to bring it up to boiling point. See Latent Heat. Sequestering Agent A substance which prevents the participation of a metal or its compounds in a chemical reaction. The catalytic effect of heavy metals, mainly copper and mangagese, on the oxidation of unsaturated compounds (e.g., rubber) results in very poor ageing. If the metal can be converted into what is known as a chelate co-ordination compound, by the use of a sequestering agent, ageing is considerably improved. See Chelating Agent. Serum In rubber latex, the aqueous phase in which the rubber globules are suspended. Set See Compression Set, Permanent Set and Tension Set. Setting Up Another name for bin curing. sg Abbreviation for specific gravity. Shape Factor (1) In rubber deformation, the ratio of the area of one loaded surface to the free area is termed the ‘shape factor’. (2) The term is sometimes used to indicate simply the ratio of length to breadth of a body. Shear A type of deformation in which parallel planes in a body remain parallel but are displaced in a direction parallel to themselves, i.e., the stress is applied in the plane of one of the faces. Many designs of rubber mountings utilise rubber in shear, the rubber often being bonded to a metal support plate. Shear Discs Another term for safety discs. Shearing Disc Viscometer Another term for Mooney viscometer.
Sheeting A calendering process in which rubber compound (suitably warmed) is passed through the nip between two bowls set at a specified distance apart to produce a comparatively thin sheet of rubber. The name ‘sheeting’ is also given to the vulcanised product. Shelf Ageing Ageing which takes place during the storage of a rubber product, i.e., between time of manufacture and time of putting into service. Shelf Life The time during which an unvulcanised rubber compound (e.g., tyre, tube and belting repair materials) or a vulcanised rubber product will remain usable when stored under normal atmospheric conditions of temperature and humidity. Shell A hollow roller of wood or metal with an internal square housing to fit a suitable shaft, used for winding up fabric, rubber sheet, rubberised fabric, linings, etc.; also termed roller or box. Shore Durometer See Durometer. Shore Hardness Hardness measured on a Shore durometer. In addition to the commonly used Shore A scale there are several others O, OO, B, C and D, designed to open out either the soft or the hard end of the A scale. Short (1) In rubber moulding, another name for light, i.e., a product where the mould has not been completetly filled. (2) In calendering the term indicates poor extensibility of rubber sheet usually due to the use of insufficiently warmed compound. Short Stop In the manufacture of synthetic rubber, the short stop or stopping agent is the substance added to the reactor to stop the polymerisation reaction. Shrinkage Change in dimensions of an unvulcanised rubber (calendered sheet or extruded section) on cooling from the processing temperature. Also the volume contraction of a moulded rubber product on cooling from vulcanising temperature. See Coefficient of Thermal Expansion (Volume). Shrinking The process of controlled, gentle warming of unvulcanised calendered sheet rubber to reduce its anisotropy and prevent subsequent distortion of articles made from the sheet and cured by embedding in chalk in open steam. Shy Another term for light. Side Chain Alkyl radicals attached to benzene or another cyclic group in the molecule of an organic compound. Sighting Colours Soluble non-fugitive dyestuffs used as identifying colours in rubber compounds.
Silica Precipitated amorphous hydrated silica and fumed anhydrous silica, inorganic reinforcing agent. Silica Gel A colloidal solution of silicic acid concentrated until it contains only about 7% water. It has very high absorbent properties and is used as a desiccant. Silicates Calcium silicate, sodium aluminium silicate and treated varieties of aluminium silicate used as reinforcing fillers in rubber compounding. Silicone Rubber An elastomer of the silicone family (see Silicones). It is a polyorganosiloxane, the backbone structure consisting of alternating silicone and oxygen atoms with organic groups, usually methyl, vinyl or phenyl radicals, attached to the silicon member. Silicones A range of silicon-containing organic compounds. The backbone of the polymer chain is composed of silicon and oxygen combined as siloxanes to which the organic groups are attached. Silicones may exist as non-volatile oils, greases, resins and rubbers, their outstanding characteristics being water repellency and resistance to high temperatures. The rubber industry is interested mainly in the elastomers (see Silicone Rubber) and certain of the oils (see Mould Release Agent). SI Metric Units The Système International d’Unités (International System of Units) has the abbreviation SI. It includes base units, supplementary and derived units which together form a coherent system of units. Prefixes are used to form decimal multiples and sub-multiples of the SI units. SIMS Abbreviation for secondary ion mass spectrometry. Sipe A narrow slit in the tread pattern of a pneumatic tyre, formed by fitting a thin blade in the mould: often termed ‘knife-cut’. SIR (1) Abbreviation for Standard Indonesian Rubber. (2) Abbreviation for styrene-isoprene rubbers. SIS Abbreviation for styrene-isoprene-styrene block copolymer, a thermoplastic elastomer. Skein Another term for hank. Skim Coating Coating carried out on a calender. Skim Rubber When natural rubber latex is concentrated by centrifuging there are produced approximately equal volumes of concentrate containing most of the rubber, and skim latex with a low proportion of rubber. The rubber obtained by coagulation of skim latex is termed skim rubber. Due to the high content of non-rubber substances such rubber may give difficulty in processing.
Rubber Basics Skiving Bevelling or cutting a rubber section at an angle with the object of making a stronger splice or of tapering off a square edge to prevent air-trapping during assembly. Slaked Lime Calcium hydroxide, inorganic filler. Slitter A machine fitted with knives, spacer bars, let-off and take-up rollers, used for slitting rubber sheet, rubbered fabric, liner material, polyethylene film, etc., into narrower widths. SLR Abbreviation for Standard Lanka Rubber. Slub A defect in woven fabrics where the yarn has lost its twist and thus appears as a thicker part on the surface of the cloth. Slubs may be introduced deliberately for cloth ornamentation. Slush Moulding A method of manufacturing articles from latex or from a plastisol. A heated metal mould is filled with the latex compound and, after an interval for gelation, the excess ungelled latex is poured out. Further heating sets the deposit, which is removed from the mould, dried and vulcanised. See Kaysam Process and Rotational Moulding. Smoked Blanket Crepe See Blanket Crepe. Smoked Sheet See Ribbed Smoked Sheet. Smooth-Bore Hose Suction hose in which the internal wire reinforcement is completely embedded in the carcase of the hose. SMR Abbreviation for Standard Malaysian Rubber. Snell’s Law When a ray of light is refracted at a surface separating two media, the ratio of the sine of the angle of incidence to the sine of the angle of refraction is a constant. See Refractive Index. Soak Cure A method of obtaining an even state of cure in thick articles. The source of external heat is shut off before cure is complete and the heat permitted to penetrate to the interior of the article. See Drop, Hold, Rise. Soapstone Another term for French chalk. Sodium Bicarbonate NaHCO3, a blowing agent, often used with a weak acid to activate its decomposition to produce CO2 Sodium Bisulphite NaHSO3, is added to latex from which pale crepe rubber is to be made. It prevents discoloration of the crepe and destroys microorganisms which may cause later deterioration of the rubber. Sodium Dibutyl Dithiocarbamate SDBC, accelerator. Sodium Diethyl Dithiocarbamate SDEC, accelerator. Sodium Dimethyl Dithiocarbamate SDMC, accelerator.
Sodium Hydroxide NaOH, caustic soda, a white solid which dissolves in water to give a strongly alkaline solution. Sodium PCP Sodium pentachlorophenol, latex auxiliary. Sodium Pentachlorophenate A preservative for concentrated natural rubber latex, the use of which eliminates the ammoniation process necessary with ammoniapreserved latex. See Low Ammonia Latices. Sodium Silicofluoride The gelling agent used in the manufacture of latex foam by the Dunlop process. Softened Rubber Another term for peptised rubber. Softeners Compounding ingredients added to elastomers (25 phr) to increase plasticity and facilitate processing. In larger proportions (20-50 phr) certain oil softeners are classed as extenders. See Peptising Agent. Sole Crepe Crepe rubber which has been plied up to thicknesses of 1/8 in, 3/16 in or 1/4 in and used in the soling of footwear. It has now been almost entirely superseded by a vulcanised rubber of similar appearance to that of the unvulcanised crepe. Solid Tyre A tyre which is composed of solid rubber bonded to a suitable wheel and without an internal air space, as in the pneumatic tyre or an internal cavity as in the semi-solid tyre. The main uses of solid tyres are on forklift trucks and armoured fighting vehicles (tanks). Solubility The degree to which one substance will dissolve in another. In rubber compounding it should be noted that many compounding ingredients are soluble in rubber and may also be soluble in each other. See Blooming, Insoluble Sulphur, Staining. Solution A true solution consists of molecules or ions of a solid substance uniformly distributed throughout a liquid. A rubber ‘solution’ is colloidal, i.e., intermediate between a true solution and a coarse suspension. Rubber solutions are used as adhesives and in the manufacture of rubber products by the dipping process. Solution Polymerisation See Polymerisation. Solutioning Another term for spreading. Solvent A solvent is a substance, usually liquid, in which another substance can be dissolved. Rubber solvents comprise coal-gas products, petroleum distillates, and various chlorinated solvents such as carbon tetrachloride and trichloroethylene. They are used in making rubber solutions for adhesives, doughs for spreading and in freshening uncured rubber surfaces prior to assembly with other components. Solvent Recovery Recovery for re-use, of the solvents used in the processes of spreading and dipping. The solvent
vapour is adsorbed on activated carbon from which it is removed by steam and separated out from the condensed water. Spandex The generic name given, in the USA, to stretch fibres based on elastomeric long-chain polyester polyurethanes. Trade names are, e.g., ‘Lycra’ and ‘Vyrene’. SPC Abbreviation for statistical process control. Specific Gravity The ratio of the weight of a given volume of a substance to the weight of an equal volume of water at 4 °C. The number denoting the specific gravity of a substance is the weight in grams of 1 cm3 of the substance. Specific Heat The quantity of heat (J/kg/K) required to raise the temperature of unit mass of the substance through 1 °C. The specific heat of rubber (around 2000) is much higher than that of metals (around 400 for steel) and it is therefore much more expensive to heat rubber than the mould, mandrel or last on which it is cured. Spectroscopy The identification of chemical substances by examination of their spectra (singular, spectrum). Both infrared and ultraviolet spectroscopy are used in the study of rubber problems such as identifying the type of polymer or the nature of a contaminant. Spew In moulding the rubber articles, it is necessary to use a blank of slightly greater volume than the mould cavity. This excess is forced out at the mould register during vulcanisation and is known as ‘spew’. It is usually accommodated in the spew groove. The term spew is also applied to the rubber extruded through release holes drilled at the edges of some extruder dies to even up the flow of rubber and produce an accurate section. Spew Groove A channel cut in the register of a mould to accommodate the spew. SPH Styrenated phenol, antidegradant – non-staining. Spider In the extrusion of rubber tubing, a central core determines the inside diameter. This core is supported by the spider or core-bridge which is itself fitted in the head of the extruder and may be adjusted laterally and vertically to produce a concentric tube. Spinning This term has two distinct meanings in textile technology: (a) the process of twisting a fibrous material into a yarn or strand, and (b) the process of producing continuous filaments of man-made fibres by extruding through a fine hole, e.g., a viscose solution to give viscose rayon, or a nylon melt to give nylon. Spinning Cot A revolving rubber roller which acts, in conjunction with a fluted steel roller, in consolidating the loosely formed yarn (slub) during spinning. Two sets of cots and rollers, running at different speeds, act in conjunction
with the drafting aprons, in stretching and consolidating the yarn prior to twisting. Split Batch Technique A procedure to prevent premature vulcanisation of very fast-curing rubber compounds, doughs or solutions. One part of the batch contains the vulcanising agent and the other contains the accelerator; requisite quantities of the two parts are mixed together immediately prior to use. Split Curing A technique of press curing in which the moulds are serviced while the press is closed. For example, in a two daylight press operating on a 60 minute cure, the press will be opened at 30 minutes and the mould from platen 1 removed and replaced with another mould loaded with the moulding blank. At the end of a further 30 minutes the procedure is repeated for platen 2, and the cycle of operations continued. Sponge Rubber One type of cellular rubber. Conventional sponge rubber has a porous structure, the cells being open and inter-communicating; it shows very high absorption of water. The rubber compound for this product has to be of low viscosity to allow the generated gas to expand rapidly as it is formed. Inorganic blowing agents are normally used for this type of product with often a small additional amount of organic blowing agent to regularise the size of the cells being formed. SPR Abbreviation for superior processing rubber also known as SP Rubber Spreader (1) Another name for a spreading machine. (2) Also a curved or fluted roller used on any machine which processes rubber-coated fabrics, with the object of ‘spreading’ the fabric from the centre of its width outwards and thus removing wrinkles. (3) A tyre ‘spreader’ is a device for holding open the beads of a pneumatic tyre so that the inside may be examined or repaired. Spreading Coating of a textile with rubber by first making the compound into a stiff dough by dissolving or ‘letting-down’ the compound into a suitable solvent and then applying at the back edge of a doctor knife under which the fabric is passed. Spreading Machine A machine which carries out the operation of coating textiles with rubber by the process of spreading Sprues In transfer moulding, the channels in the mould which transfer rubber compound to the actual moulding cavities. Spue An obsolescent term for spew. Square Woven Fabric A woven fabric having approximately the same number of warp threads per inch of width as weft threads. SQC Abbreviation for statistical quality control.
Rubber Basics SRF
which it is designed. The tyre circumference shows a series of flats since the part in contact with the ground has not had sufficient time to recover before it again meets the ground. Staple Fibre Man-made fibres produced as continuous filaments and then cut into short lengths to match those of some natural fibres such as cotton or wool. The ‘staple’ of cotton, wool, staple fibre, etc., is an indication of the average fibre length. Stark Rubber Another name for frozen rubber. State of Cure The degree of vulcanisation of a rubber compound is assessed technically by the indefinite terms of undercure, correct cure, optimum cure and overcure. It may be given precision by (a) measurement of stress-strain relationship of a range of cures, (b) measurement of the modulus at 100% elongation, (c) measurement of the volume swelling in benzene, or (d) by the use of instruments such as the oscillating disc rheometer and the moving die rheometer. Static Electricity Electricity at rest as opposed to moving or current electricity. Static electricity can build up on the surface of insulating materials and may either spark across to an adjacent object or give a shock to anyone handling the material. See Anti-Static Rubber. Statistical Quality Control The control of quality of a process or product by the application of the techniques of mathematical statistics. Statistics The classification, tabulation and study of numerical facts. Mathematical statistics is the study of the variation of natural phenomena and employs the techniques of probability theory. Steam Water in the gaseous state; it is a convenient source of heat widely used in the curing of rubber products. See Open-Steam Curing, Press Curing. Steam is really a colourless gas and what is usually termed ‘steam’ (issuing from an autoclave, a press, thermometer bleed pipe, etc.) is really droplets of water which result from the steam meeting the cooler air of the atmosphere. Steam Trap A device fitted to steam supply pipes and all steam-heated equipment to ensure that condensate formed when the steam has given up its heat is quickly discharged from the system without loss of live steam. Stearic Acid C17H35COOH, one of the fatty acids found in animal fats. Commercial stearic acid is a mixture of stearic and palmitic acids. It is used in rubber compounding as an organic activator of accelerators. Stefan’s Law Also known as the Stefan-Boltzmann law. The total radiation from a black body is proportional to the fourth power of its absolute temperature.
Semireinforcing furnace, carbon black grade. SSR Abbreviation for Specified Singapore Rubber. Stabiliser In latex compounding, same as protective colloid. Stabilisers are incorporated in synthetic raw rubbers to protect the rubbers from oxidation during storage. Since the chemical behaviour of these protective materials is not significantly different from that of antioxidants in a vulcanisate, it has been proposed that the use of stabiliser in this sense be dropped in favour of antioxidant. Staining Change of colour of a vulcanised rubber when exposed to light or change of colour in a material in contact with, or adjacent to a vulcanised rubber. Stand (1) On a rubber plantation, the tree population per acre. The initial stand is sufficient to allow for losses due to disease and provides a final stand of 90-100 trees per acre. (2) Another name for hold. Standardisation An international committee (ISO/TC45) deals with the standardisation of test methods for rubber and the standardisation of rubber product specifications. There is a parallel committee for plastics, materials and products; ISO/TC61. Individual countries also have standard setting bodies such as BSI and ASTM. Standard Malaysian Rubbers The introduction of Standard Malaysian Rubbers represented a significant development in the marketing of natural rubber. The SMR scheme offers a complete range of technically specified natural rubbers guaranteed to meet a national standards code covering quality and presentation. The system has superseded the largely arbitrary, visual grading methods - there were thirty-one internationally recognised visual grades and, additionally, a great number of private grades used by local producers. The first three grades of SMR were technically specified in terms of guaranteed cleanliness: SMR 5 with a guaranteed cleanliness level of 99.95%; SMR 20 a guaranteed cleanliness level of 99.8%; SMR 50 a guaranteed cleanliness level of 99.5%. Colour plays no part in technical specification, but there is a special grade of light-coloured SMR for those who need it - SMR 5L - made to SMR 5 standards. In addition SMR is characterised by the plasticity retention index, which gives opportunity for close control of processing and properties. SMR is not only technically specified clean. It is delivered clean because it is film-wrapped, in small convenient bales. SMR is available either in standard forms of sheet and crepe, or compacted crumb forms of NR. Standing Wave A phenomenon occurring in a pneumatic tyre running at a speed much higher than that for
STEL Short Term Exposure Limit. See Occupational Exposure Limits. Step Cure In the vulcanisation of thick rubber articles the temperature may be stepped up in stages to ensure adequate heat penetration to the interior before the external surface begins to cure. Such a cure schedule is termed a step cure. Step post cures are used with thick section rubber articles to ensure that volatiles are released gradually without causing damage, such as porosity, due to an over rapid release. Stereochemistry Chemistry which takes into consideration the arrangement in space of the atoms in a molecule. Assuming that a molecule is three-dimensional, space isomerism is thus possible. Stereoregular Polymers High polymers in which the side chains are arranged either above or below the plane of the main carbon chain of the molecule in a regular pattern. In the isotactic molecular structure the substituent groups are all on the same side of the main chain, either all above or all below. In the syndiotactic structure the substituent groups alternate regularly above and below the plane of the main chain. In an atactic structure the substituent groups are arranged irregularly above and below the plane of the main chain. Stereoregular polymers are made by reactions involving the use of stereospecific catalysts. Stereospecific Catalysts Catalysts which bring about a spatially regular (stereoregular) configuration in high polymers. The main types are Ziegler, Phillips, Standard Oil and Metallocene Stereospecific Polymers Polymers synthesised by the use of certain catalysts which direct the propagation reaction so as to bring about a known and desired orderliness in the molecular chain. See Stereoregular Polymers. Steric Hindrance In organic chemistry, the retarding influence of neighbouring groups on reactions between molecules. Stiffener A compounding ingredient used to reduce the plasticity (increase the stiffness) of rubber compound and thus enable, e.g., an extruded section, to retain its shape or to reduce air trapping in moulding soft rubbers. Stock (1) Another name for a rubber compound. (2) In bud grafting, the plant on which the bud is grafted. Stokes’ Law The rate of settling of solid particles in a fluid depends on the particle-size of the solid and the nature of the fluid. The terminal velocity (v) is given by: 2gr 2 (d1 −d 2 ) v= 9η
where the particles have radius r, density d1 falling through a liquid of density d2 and coefficient of viscosity η. STP Abbreviation for standard pressure. See NTP.
STR Abbreviation for Standard Thai Rubber. Strain The change in dimensions resulting from the application of a stress. In tensile testing of rubber strain is synonymous with elongation. Strainer A machine similar in principle to an extruder but fitted with a special head containing a wire gauze through which rubber or rubber compound may be passed to free it from foreign matter or from agglomerates of compounding ingredients. In the extrusion of thin-walled tubing a strainer plate and gauze may be fitted in the actual extrusion machine so that foreign matter is removed immediately prior to the extrudate issuing from the die-box. Strainer-Slabber A strainer equipped with a special die which extrudes the strained rubber as a tube, which is then slit at the head to produce a continuous sheet, which may then be cut into slabs of convenient length. Strain Gauge A device for measuring very small strains. The electrical type consists of a grid of thin resistance wire suitably attached with adhesive to the surface to be tested; the resistance of the wire is proportional to the strain. Straining Removing foreign matter and agglomerates of compounding ingredients from rubber or rubber compound by passing it through a strainer. Stress Force per unit area. The applied stress may deform an elastomer in three ways, i.e., extension, compression or shear. Stress Decay Another term for stress relaxation. Stress Relaxation The reduction in stress which takes place in a test strip of rubber held at constant elongation. Stress relaxation measurements are used in the study of the ageing of rubber vulcanisates, the degradation of the network structure resulting in a reduction of the tension. Stress Softening Another term for Mullins effect. Stress-Strain Testing The determination of the relationship of stress to strain when a rubber is deformed, the result being shown in the form of a stress-strain curve; unless compression stress-strain is specifically stated, the expression normally applies to the tensile characteristics of a rubber. Strip Knives A set of knives fitted to a mill to cut off a strip of rubber compound for continuous feeding of an extruder or calender. Similar knives may be fitted to a calender roll to produce strip or sheet rubber of specified width.
Rubber Basics Stripping (1) The removal of uncured assemblies or cured products from a former, mandrel or mould. (2) The removal of unreacted monomers in the manufacture of synthetic rubber. (3) Determination of adhesion between textile and rubber in tyres, hose, belting, etc., by measurement of the force necessary to strip one from the other. Stroboscope An instrument used for examining any regularly repeating motion, e.g., speeds of rotating shafts. The frequency of flashing of a bright light illuminating the shaft is varied until the shaft appears stationary and a simple calculation gives the shaft speed. Structural Formula A formula showing how the individual atoms in a molecule are linked together by valency bonds. Structure This term has its normal meaning as in the ‘structure of vulcanised rubber’ but it now has a particular significance in relation to carbon black. See Carbon Black Structure. S-Twist In textile technology that direction of twisting yarns or threads which runs from left to right downwards, as the centre part of a letter S, when the yarn is held vertically. Styrenated Phenol SPH, antidegradant – non-staining. Styrene One of the monomers used in the manufacture of styrene-butadiene rubber. It is vinylbenzene, a liquid boiling at 146 °C and having the formula C6H5CHCH2. Styrene-Butadiene Rubber A general purpose synthetic rubber made by the copolymerisation of styrene and butadiene in the proportions of approximately 25 styrene to 75 butadiene. Sub An obsolescent abbreviation for rubber substitute. Substitution Chemical reaction typical of saturated organic compounds, replacing one chemical group, e.g., hydrogen, by another. Substrate (1) The substance on which an enzyme acts, as in the formation of volatile fatty acids in latex. (2) The underlying layer, e.g., the metal in rubber-to-metal bonding. Sulphenamides Organic accelerators of the thiazole class having delayed action and finding particular application in tyre compounds containing furnace blacks. Sulphenamides are manufactured from mercaptobenzothiazole by reaction with an amine, the nature of which determines the degree of delayed action. Sulphur Elemental sulphur mixed into rubber compounds is the agent responsible for the vulcanisation of the majority of rubber products made from natural rubber, SBR, butyl rubber and nitrile rubber. Sulphur-vulcanisable varieties of many of the newer synthetics are also available. The bulk
of the world’s sulphur is produced by the Frasch process. See Flowers of Sulphur and Insoluble Sulphur. Sulphur Bridges In sulphur vulcanisation of rubber, crosslinking is considered to be effected by sulphur atoms, which are therefore termed sulphur bridges. See Vulcanisation. Sulphur Donor A curing agent which splits off active sulphur during the vulcanisation reaction. One example is di-morpholinodisulphide (Sulfasan R). Sulphur MC A magnesium carbonate coated grade of sulphur used in curing nitrile rubber. Sulphur Monochloride S2Cl2, a by-product in the manufacture of carbon tetrachloride from carbon disulphide. Was used, dissolved in solvent naphtha, in the vulcanising of rubber by the cold cure process and the vapour cure process. The process was fraught with health and safety problems and has been superseded by low temperature accelerators and room temperature vulcanising (RTV) systems for silicone and polyurethane. Superheated Steam Steam heated out of contact with the water from which it was formed and subsequently passed over an additional heat source, known as a superheater, and is therefore at a higher temperature than that corresponding to saturation. It should be noted that a ‘leak’ of superheated steam cannot easily be seen. See Steam and Saturated Steam. Superior Processing Rubber A modified type of natural rubber which has many processing advantages over normal sheet and crepe rubbers. It shows reduced shrinkage, reduced die swell and much better retention of dimensions especially in complicated extrusions. It is made by adding a quantity of vulcanised latex to normal latex before coagulating. See PA 80. Surface Active Agent Materials used in latex compounding, having the power to displace other substances already adsorbed on the rubber particles. See Emulsifying Agent, Protective Colloids and Wetting Agents. Surface Resistivity The electrical resistance between opposite edges of a square or between 2 electrodes on the same surface of the material, under specified conditions of testing, e.g., BS 903-C1. Surface Tension The open surface of a liquid tends to contract inwards towards the bulk of the liquid, as if it were covered with an elastic skin. This phenomenon is termed surface tension. Surfactant Another term for surface active agent. Suspension A solid/liquid mixture consisting of very small solid particles suspended in a liquid. The action of gravity or the process of filtration can effect separation of the solid from the liquid. SVR Abbreviation for Standard Vietnamese Rubber.
Swan-Necked Press Another term for gooseneck press. Sweetening The process of treating cold-cured proofings with a weak alkali to neutralise any remaining acid and so prevent subsequent tendering of the fabric. Swelling Increase in dimensions of an elastomer due to the absorption of any organic liquid with which it may come in contact or in which it may be immersed. Measurement of the swelling of vulcanised rubber in solvents can be used to determine state of cure and to assess the suitability of elastomers for such uses as chemical plant lining or oil seals. SWG Abbreviation for Standard Wire Gauge (British). Syndiotactic or Syndyotactic One of the terms coined by G. Natta to describe different arrangements of atoms in long-chain molecules. See Stereoregular Polymers. Syneresis The expulsion of liquid from a gel as in the coagulation of latex, where the structure of rubber particles contracts and expels the serum. Synergistic The ‘working together’ of two substances to give a result of greater effect than would be expected by the simple addition of the effects of the two substances working alone. Synthetic The adjective from the noun synthesis; it is correctly applied to the product resulting from the combination of two or more chemical substances to form a new substance, the process being carried out by man in either the laboratory or the factory; ‘synthetic’ does not mean inferior. Synthetic Rubber A convenient term for any material possessing the properties of a rubber but produced from other than natural sources. A synthetic version of natural rubber has been available for many years with the same chemical formula, i.e., cis-1,4polyisoprene, but it has not displaced the natural form. See also Butyl Rubber, Chloroprene Rubber, Ethylene-Propylene Rubber, Nitrile Rubber, Silicone Rubber and Styrene-Butadiene Rubber. Semicrystalline A polymer in which most of the molecules are packed in a regular manner forming crystalline regions (50-95%)in the solid state, the remainder of the material forms amorphous regions.
reduced by the use of dusting agents; assembly of uncured components is facilitated by good tack which is enhanced where necessary by the addition to the compound of tackifiers. Certain freshly-cured rubber products have a very tacky surface, and if the use of a dusting agent is undesirable the tack may be removed by treatment with chlorine water or with ‘cold cure’ solution (see Cold Cure). See Tackiness. Tackifier A compounding ingredient which enhances the surface tack of uncured rubber compounds. Tackifiers, exemplified by pine tar are classed under ‘softeners and processing aids’. Tackiness Although tack and tackiness generally have the same meaning, the term tackiness is usually confined to surface stickiness due to environmental degradation whereas tack refers to the adhesiveness of uncured material. Tackmeter An instrument for measuring the surface tack of sheet materials. Tactic Polymers High polymers which show the stereochemical configurations known as isotactic and syndyotactic. See Stereoregular Polymers. TAIC Triallyl isocyanurate, peroxide co-agent. Tail Gas The lighter gases produced in the distillation of petroleum or the residual gas in the manufacture of carbon black by the furnace process. Talalay Process A method of manufacturing latex foam. Compounded latex is partially frothed and fully expanded by application of vacuum to the mould; the gel is frozen, set by carbon dioxide and vulcanised by raising the temperature of the mould. See Dunlop Process. Talc Another term for French chalk. Tall Oil A mixture of monobasic organic acids (abietic, oleic and linoleic), produced either as a byproduct of paper production or synthetically. It is used as an extender. Tapping The operation of making a carefully-controlled incision in the bark of the Hevea tree to permit the latex to flow out. Using a specially shaped knife the tapper makes a 6 mm deep cut in the bark at an angle of 30° from left to right. The cut is shaped into a groove from which a shaving of bark about 1 mm thick is removed in subsequent tappings. See Tapping Systems. Tapping Systems Length of cut and frequency of tapping are varied to suit particular clones, e.g., a half-spiral cut every second day being denoted as ‘S/2, D/2, 100%’, the 100% representing normal tapping intensity. TBBS N-tert-Butyl-2-benzothiazole sulphenamide, accelerator. TBTU 1,1,3-Tributyl thiourea, accelerator.
7 TAC Triallyl cyanurate, peroxide co-agent. Tachometer An instrument for measuring the speed of a revolving shaft or of belting, etc.; it may indicate the speed in either revolutions per minute (rpm) or in length per minute. Tack The adhesiveness of raw rubber or rubber compounds. Where tack is undesirable it may be
Rubber Basics TBUT Tetrabutyl thiuram disulphide, accelerator. TBZTD Tetrabenzyl thiuram disulphide, accelerator. TCP Tricresyl phosphate, ester plasticiser. TCR Abbreviation for technically classified rubber. TDI Toluene diisocyanate. See Isocyanate. Tear Resistance Resistance to extension of a cut or tear in a rubber sample. See Tear Strength. Tear Strength This is determined by cutting a nick of accurate depth in a crescent-shaped test piece, measuring the load required to complete the tearing. Technically Classified Rubber Technically Classified Rubber was introduced in about 1951. It was natural rubber which had been tested on the plantation for rate of cure. Each bale was marked with a coloured circle, red denoting slow curing, yellow medium curing and blue fast curing. When the scheme was first introduced, the shape of the symbol indicated the plasticity of the rubber, a bar for low Mooney viscosity, a circle for medium Mooney and a cross for high Mooney. The plasticity grading was then discontinued due to the plasticity change between plantation testing and receipt of the rubber by the consumer. This system was superseded in 1965 by Technically Specified Rubber. Technically Specified Rubber This is the generic name for the scheme originally introduced in Malaysia as Standard Malaysian Rubber (SMR). In effect it is the same specification but applied to rubber produced in other countries, e.g., Standard Indonesian Rubber (SIR). Both SMR and SIR are Technically Specified Rubbers. Technology The practice and description of any or all of the applied sciences which have commercial value. Tellurium A brittle, non-metallic element with chemical properties similar to those of sulphur. It has been used as a secondary vulcanising agent. Tellurium Diethyl Dithiocarbamate TDEC, accelerator. TEM Abbreviation for transmission electron microscopy. Temperature A measure of the ‘hotness’ or ‘coldness’ of a substance; it is measured in degrees. See Celsius and Fahrenheit. Temperature Coefficient of Vulcanisation This is the ratio of the rates of vulcanisation at two temperatures 10 °C (or 18 °F) apart. For rubber vulcanisation the coefficient is approximately 2 but it varies slightly with the temperature, the type of compound and the accelerator. Temperature Control Maintaining a specified temperature within narrow limits is essential in many processes carried out in the rubber industry, e.g.,
polymerisation temperature in the manufacture of synthetic elastomers, vulcanising temperature in the manufacture of rubber products. Control systems vary in their sophistication. Sensors are commonly based on thermocouples or platinum resistance thermometers and the most common system can be described as having three term controllers, i.e., PID or Proportional, Integral and Derivative. To be effective the PID terms need to be tuned to the process and equipment, modern systems are generally self tuning. Temperature Scales See Celsius and Fahrenheit. Tenacity The breaking strength of a textile filament, yarn or cord, expressed in grams per denier. Tendering Weakening of a fabric from any cause, but particularly the weakening of a proofed fabric by the acid resulting from insufficient sweetening, after vulcanisation by the cold cure process. Tensile Strength The breaking stress in tension of an elastomer expressed in Mpa, kg/cm2 or lb/in2. It is calculated on the original (unstressed) area of cross-section of the test specimen. Tension Set The elongation remaining after a rubber test piece has been stretched for a given time and allowed to rest for a given time; it is expressed as a percentage of the original distance between the bench marks. The term ‘permanent set’ (correctly, permanent set in tension) is still popularly used to denote tension set, see standard BS903-A5. Terpenes A class of hydrocarbons occurring in many essential oils of plants. They can be regarded as low-molecular weight polymers of isoprene (C5H8)n. Dipentene is a terpene, while natural rubber, gutta percha and balata have been termed polyterpenes. Terpolymer A copolymer consisting of three monomers polymerised together, e.g., ethylene-propylenedicyclopentadiene terpolymer. Terracing The cutting of terraces on rubber plantations situated on hilly areas, with the object of preventing the loss of top soil during heavy rain. Terylene The trade name of a polyester fibre used as textile reinforcement for rubber in products such as tyres, belting and hose. It is a truly synthetic fibre made from polyethylene terephthalate, a condensation product of terephthalic acid and ethylene glycol. TETD Tetraethyl thiuram disulphide, accelerator. Tetrabenzyl Thiuram Disulphide TBZTD, accelerator. Tetrabutyl Thiuram Disulphide TBUT, accelerator. Tetraethyl Thiuram Disulphide TETD, accelerator. Tetramethyl Thiuram Disulphide TMTD, accelerator
Tetramethylthiuram Monosulphide An accelerator similar in properties to tetramethylthiuram disulphide, except that it cannot be used without added sulphur. Tex A system of designating the fineness (linear density) of yarns and fibres. It was proposed for universal adoption, to supersede the multiplicity of existing systems of yarn counts. The Tex unit is the weight in grams of 1000 metres of yarn. A 23s cotton becomes 25.6 tex and a 1260 denier yarn becomes 140 tex. See Count and Denier. Textiles In a limited sense, any material suitable for weaving or being made into a woven fabric. In the rubber industry the term is widened to include any material used for the structural reinforcing of a product and thus includes such materials as steel and glass not normally classed as textiles. See Cotton, Nylon, Rayon and Terylene. TFE Abbreviation for tetrafluoroethylene. Tg Abbreviation for glass transition temperature. TGA Abbreviation for thermogravimetric analysis. T-Head An extruder die-box or head in the shape of a letter T used in wire covering. The rubber flow is thus at right angles to the direction of travel of the wire. Thermal Black Carbon black produced by the thermal decomposition of natural gas or atomised oil in a pre-heated refractory furnace where the fuel is cracked into carbon and hydrogen. The process is cyclic, two furnaces being used as one production unit, one furnace being heated up as the other is producing. Thermal Conductivity The thermal conductivity of a substance is the quantity of heat in cal/sec passing through a body 1 cm thick with a cross section of 1 cm2 when the temperature difference between the hot and cold sides of the body is 1 °C. The thermal conductivity of compounded rubber is an additive property of the rubber and the compounding ingredients, and may be calculated from the mix formula and the individual thermal conductivities. Thermal Decomposition Breaking down of a chemical substance by means of heat. See Cracking and Thermal Black. Thermal Diffusivity A coefficient which determines the rate of rise of temperature of a point in a body which is being heated at some other point; it is equal to the thermal conductivity of the substance divided by the product of its specific heat and its density. Thermal Expansion See Coefficient of Thermal Expansion. Thermal Liquids Liquids of high boiling point and having good heat transfer properties, used in industrial heating. They operate at atmospheric pressure but at temperatures up to 400 °C (752 °F).
Thermocouple An assembly of two dissimilar metals often in the form of wires, used in measuring temperature by means of the thermo-electric effect. Thermo-Electric Effect The production of a current of electricity by heating a junction formed by two dissimilar metals. For temperature measurement the metals are usually in the form of wires (see Thermocouple) and the circuit has two junctions, the ‘hot’ junction which is exposed to the temperature to be measured and the ‘cold’ junction which is kept at a standard temperature. The thermo-electric effect is also termed the ‘Seebeck Effect’ after its discoverer. Thermogram The form of graph on which are displayed the results of tests done by the technique of differential thermal analysis. Thermogravimetric Analysis This is an analytical technique used to obtain accurate quantification of the principal compound constituents such as plasticiser, polymer, carbon black and inorganic species, by monitoring weight loss across a temperature range. Thermoplastic Applied to high polymers which soften by the application of heat and which may be resoftened by heating, provided chemical decomposition does not take place. Thermoplastic Elastomers These were originally described as ‘thermoelastic polymers’. The first were block copolymers of butadiene and styrene, at room temperature one and the same molecule has segments in it which are rubber-like, as well as segments which are below their glass transition temperature and hence are rigid. The benefits of these unique rubbers lie in the fact that at temperatures of 285430 °F (140-220 °C) they may be shaped and reshaped by the processing techniques used for thermoplastics, and on cooling their elastomeric character is regained. Thus, traditional mixing and vulcanising equipment is unnecessary and scrap may be recycled. There are a wide range of thermoplastic elastomers with properties generally intermediate between those of rubbers and plastics. Thermosetting Applied to a high polymer which undergoes a chemical change when it is subjected to heat, after which its shape cannot be changed by the application of further heat and pressure. Although vulcanisation of rubber is a thermosetting process the term is usually applied to ‘plastics’. See Thermoplastic. Thermostat A device for maintaining a constant temperature. It may employ a bimetallic strip the twisting movement of which (due to the different coefficients of expansion of the two metals) switches heating elements on or off to maintain the specified temperature. THF Abbreviation for the solvent tetrahydrofuran.
Rubber Basics Thiamer A term that was used as a generic name for a new family of elastomers related to EPT. They are terpolymers and sulphur-vulcanisable. Sulphur atoms separate each of the ethylene and propylene repeating units in the backbone of the polymer chain, hence the name thiamer. Thickening Agent A substance used in latex compounding to increase the viscosity of the mix. Examples are alginates, casein, certain clays and methyl cellulose. Thin Layer Chromatography This is an analytical technique used for the separation and identification of additives. It can also be used in a preparative way for the isolation of sample fractions for subsequent chromatographic or spectroscopic analysis. Thiocarbanilide Symmetrical diphenylthiourea, one of the oldest accelerators. It is slow-curing but scorchy and is little used nowadays. It survived as the accelerator for pneumatic tyre curing bags until the late 1960s. Thiokol See Polysulphide Rubbers. Thixotropy The property possessed by certain colloids of forming a gel-like structure on standing but which revert to a liquid form when subjected to agitation. The term has also been applied to the stiffening effect shown by uncured rubber compounds containing fillers, particularly carbon black. Threading Diagram A diagram showing how rubber sheet, fabric, linings, etc., are ‘let off’ through tensioning devices into calenders, spreading machines, etc., and finally taken up on box rollers. Direction of travel and position of rubber nips are usually included in such diagrams. Titanium Dioxide A white pigment for rubbers and plastics characterised by high tinctorial power, fastness to light, and chemical stability. Titanium dioxide pigments are made in two crystal forms, rutile and anatase, which differ in crystal structure and crystal size. TLC Abbreviation for thin layer chromatography. TLV Threshold Limit Values are established in the USA by the American Conference of Governmental Industrial Hygienists (ACGIH). Three categories of TLV are now commonly quoted as follows: (1) Threshold Limit Value - Time Weighted Average (TLV-TWA), this is the timeweighted concentration for a normal 8-hour work day or 40 hour working week, to which nearly all workers may be repeatedly exposed, day after day, without adverse effects. (2) Threshold Limit Value - Short Term Exposure Limit (TLV-STEL). The maximum concentration to which workers can be exposed for a period of up to 15 minutes
continuously without suffering from intolerable irritation, chronic or irreversible tissue change, or narcosis of sufficient degree to increase accident proneness, impair selfrescue or materially reduce work efficiency; provided that no more than 4 excursions per day are permitted, with at least 60 minutes between exposure periods, and provided that the daily TLV-TWA also is not exceeded. (3) Threshold Limit Value - Ceiling (TLV-C). The concentration that should not be exceeded even momentarily. In the USA compliance with TLV standards is generally considered to be mandatory, although not statutory. See Occupational Exposure Limits. TMCH 1,1-Bis(tert.-butylperoxy)-3,3,5trimethylcyclohexane, organic peroxide. TMQ Polymeric 2,2,4-trimethyl-1,2-dihydroquinoline, antidegradant – staining. TMT Abbreviation for tetramethylthiuram disulphide. TMTD The preferred abbreviation for tetramethylthiuram disulphide to prevent confusion with tetramethylthiuram monosulphide. TMTM The preferred abbreviation for tetramethylthiuram monosulphide. TNPP Tris(nonylphenyl) phosphite, antidegradant – non-staining. Toggle Press A press for vulcanising rubber products, operated by electricity and held shut by a mechanical toggle or elbow joint. See Daylight Press. Tolerance The permissible deviation from the specified dimensions of any component or product, or from the specified conditions of temperature, pressure, time, etc., laid down for the carrying out of any processing operation. Toluene Toluol or methylbenzene; a hydrocarbon of the benzene series, used as a solvent for rubbers. p-Toluene Sulphonyl Hydrazide TSH, blowing agent. o-Tolyl Biguanidine OTBG, accelerator. Ton The British or ‘long’ ton weighs 2240 pounds; the American or ‘short’ ton is 2000 pounds, and the metric ton (tonne) of 1000 kilograms is equivalent to 2205 pounds. Top Capping The process of adding new tread to a worn tyre. Topping See Coating. Torque The turning force produced by two equal and opposite parallel forces acting on a body. Toxicity The term toxicity, when used in the context of industrial materials and processes, refers to the potential of chemical substances to cause adverse
effects in human beings as a result of skin contact, inhalation, or ingestion. Toxic effects may become apparent either immediately or shortly following exposure (acute toxicity) or they may become evident only after repeated exposure to amounts of chemicals which are individually too small to give rise to acute effects (chronic toxicity). Substances giving rise to chronic or delayed effects include cumulative poisons and carcinogenic chemicals. TPAU Abbreviation for thermoplastic polyester urethane. TPEU Abbreviation for thermoplastic polyether urethane. TPT-MA Trimethylolpropane trimethacrylate, vulcanising agent. TPU Abbreviation for thermoplastic urethane elastomer. TPX Polymers A series of thermoplastics based on 4-methylpentene-1. Polymethylpentene is the lightest of all known polymers with a density of 0.83 g/cm3. It has excellent electrical insulating and chemical resistance properties, and offers a very high melting point. Because of its low density, TPX has high acoustic efficiency (a high damping factor due to large internal losses). It also displays exceptionally low distortion and high power handling characteristics. Trans See Cis-Trans Isomerism. Transfer Moulding A method of moulding rubber products which has certain advantages over compression moulding. The transfer mould has an upper cavity or pot into which the uncured blank is placed. The closing of the mould transfers the rubber through a series of holes (feed ports) into the mould cavity proper. Cure times are shorter than for compression moulding since the rubber gains some frictional heat as it is forced through the feed ports. Transmission Electron Microscopy TEM is used to investigate the phase morphology of polymer blends and the dispersion of fillers. See Electron Microscope. Tread That portion of a vehicle tyre (pneumatic, semipneumatic or solid) which contacts the road surface. The tread pattern is so designed as to give the best combination of properties suitable for the conditions under which the tyre will be used. Tread Rubber The preferred, but ambiguous, name for camelback. Treated Applied to certain compounding ingredients (particularly zinc oxide and precipitated whiting) which have been surface-treated to improve their reinforcing power or their ease of incorporating into rubber. Also applied to a lining which has
received some treatment to facilitate the removal of the unvulcanised sheet or rubbered fabric. Tree Lace See Tree Scrap. Tree Scrap Strips of naturally-coagulated rubber removed from the tapping cut, vertical channels and spout prior to making the next tapping. The rubber is washed, dried, creped and sold as blanket crepe. Triallyl Cyanurate TAC, peroxide co-agent. Triallyl Isocyanurate TAIC, peroxide co-agent. Triangular Calender The three-bowl version of the Z calender. Tricap Triethylene glycol dicaprylate/caprate, ester plasticiser. Tricresyl Phosphate TCP, ester plasticiser. Triethanolamine A basic substance used particularly in compounds containing large quantities of white factice to offset the retarding effect of the factice. Also used to prepare emulsifying agents in latex compounding. Triethylene Glycol Dicaprylate/Caprate Tricap, ester plasticiser. Trimethylolpropane Trimethacrylate TPT-MA, vulcanising agent. Triple Bond The type of bond in which three valency bonds link two atoms in a molecule. See Acetylene. Tripsometer An apparatus for the determination of resilience by a rebound method. Usually termed Dunlop tripsometer. See Resilience. Tris(Nonylphenyl) Phosphite TNPP, antidegradant – non-staining. Tritolyl phosphate TTP, ester plasticiser. Trixylyl Phosphate TXP, ester plasticiser. TSH p-Toluene sulphonyl hydrazide, blowing agent. TSR Abbreviation for technically specified rubber. TTP Tritolyl phosphate, ester plasticiser. TTR Abbreviation for Thai Tested Rubber. See STR. Tube Normally refers to the inner tube of a pneumatic tyre assembly but may refer to any component of a rubber product which is in tubular form, e.g., the inner lining of a fire hose. See Tubing. Tubeless Applied to a pneumatic tyre with no separate inner tube. An air-impermeable lining, usually of a halogenated butyl, is applied to the inside of the casing. The bead construction is such as to ensure an airtight fit on the wheel rim. Inflation is done through a valve fitted directly into a valve hole in the rim. Tuber Another name for extruder.
Rubber Basics Tubing (1) Another name for extrusion. (2) Rubber in tubular form such as gas tubing. Tubing differs from hose in that it has no structural textile reinforcement. Tumbling A process for removal of the spew or flash on moulded rubber products, by tumbling or rotating the parts in a barrel maintained at a temperature low enough to harden the spew, which is rubbed or chipped away by friction between the articles. The low temperature is usually obtained by using liquid nitrogen. TWA Time Weighted Average. See Occupational Exposure Limits. Twaddell A scale for expressing the specific gravity of liquids, named after William Twaddell, whereby 200 degrees Twaddell equates to a sg of 1. Twist The coiling together of textile staple fibres, yarns or threads to give the structure the required degree of strength, extensibility, flex resistance, etc. Twist is designated as so many turns per inch and either right hand (Z) or left hand (S). See STwist and Z-Twist. TXP Trixylyl phosphate, ester plasticiser. Tyndall Effect If a beam of light is passed through a colloidal solution, the colloidal particles will reflect or scatter the light so that the beam becomes visible when the solution is viewed from the side against a dark background. This Tyndall effect is used in the ultramicroscope. Tyre See Pneumatic Tyre, Semi-Solid Tyre and Solid Tyre. Tyre Cord A particular construction of filaments of rayon, nylon, Terylene, Kevlar or steel used as the structural reinforcement of pneumatic tyres. The cords were originally woven (cord fabric) but are now invariably used weftless. T-50 Test One method for determining the state of cure of a rubber compound. A sample of the rubber is stretched, cooled to a temperature of around –70 °C while stretched and then released. As the temperature rises the rubber retracts and the T-50 value is the temperature at which it has lost 50% of its original elongation. The T-50 test is now obsolescent.
termed ‘elongation at break’ (BS903:Part A2 Determination of tensile stress strain properties). Ultra Accelerators A term applied to a class of organic accelerators with a very fast and powerful accelerating action: examples are the thiuram disulphides, dithiocarbamates and xanthates. See TMT, ZDC and ZIX. Ultramicroscope An instrument used to observe particles too small to be seen by the ordinary light microscope. The ultramicroscope makes use of the Tyndall effect. Ultrasonics Pressure waves of the same nature as sound waves but of greater frequency, i.e., shorter wavelength, and therefore inaudible. Ultrasonic waves have been used for the detection of ply separations and other voids in rubber-textile composites such as tyres, and for thickness measurement of coatings, etc., where access is possible from only one side. Ultraviolet Radiation Electromagnetic waves with wavelengths between those of visible light waves and X-rays. Ultraviolet radiation is used in the examination of elastomers by spectroscopy. Undercure The opposite of overcure. Uni-Rotor Mixer A mixing machine for rubber and plastics, the ingredients being mixed by a single rotor blade in a cup-shaped chamber being grooved so as to force the mixture to the closed end of the chamber. The principle has been evaluated on laboratory-size machines and is being extended to larger mixers. Unsaturated Polymer Any polymer having more than one bond between two adjacent atoms usually carbon atoms and being capable of adding other atoms at that point to reduce it to a single bond. Unsaturation In organic compounds the linking of some of the atoms of the molecule by more than one valency bond, i.e., double or triple bonds. Upside Down Mixing The simultaneous addition of the elastomers and all the compounding ingredients to an internal mixer at the beginning of the mixing cycle. A saving in mixing time is claimed but dispersion may be adversely affected. Urethane RNHCOOR´; basic unit of polyurethane, formed by the reaction of an isocyanate group with an alcohol. U-Ring A sealing of U-section which is located in a housing so that the fluid pressure tends to expand the flanges of the U into fluid-tight contact with the walls of the housing. USF Rubber This is a type of natural plantation rubber made by flocculating formaldehyde-preserved latex. Formaldehyde is added to the latex as soon as possible after tapping, dirt is allowed to settle out; the latex is bulked, flocculated with acid and the floccs coalesced by steam heat. The coagulum is
8 UHF Abbreviation for ultra high frequency. UL Rating Underwriters’ Laboratory rating; a material is aged at various temperatures and a propery is monitored, e.g., tensile strength. Ultimate Elongation In tensile testing of rubber, the elongation reached by the sample at its breaking point; also
Value Engineering The application of value analysis to new products in the research and development stage. Van der Waals’ Forces Attractive forces acting between atoms or molecules of all substances. These forces are generally very small compared to other molecular forces, and are sometimes termed ‘secondary forces’. Vapour Cure An obsolescent variation of the cold cure. The articles are vulcanised by exposing them to the vapour of sulphur monochloride in a closed chamber. Vapour Pressure The pressure exerted by a vapour, either alone or in a mixture of gases. When a mixtrure of gases is involved the partial (vapour) pressure is a measure of the relative concentrations of the constituents of the mixture. The saturated vapour pressure, the pressure of a vapour in contact with its liquid form is often termed simply vapour pressure. Variable Intermeshing Clearance (VIC) Rotor Internal Mixer The variable intermeshing clearance rotor mixer is designed to allow a variable clearance between the intermeshing rotors of the mixer. Varnish Used with the normal meaning as in a protective varnish for rubber products, but sometimes used in the sense of rubber cement. V-Belt A rubberised fabric belt used for the transmission of power. In cross-section the belt is rectangular with sloping sides similar to the upper part of a letter V; it operates between sheaves into which the V-shape fits. VCV Abbreviation for vertical continuous vulcanisation. VdMi Verband der Mineralfarbenindustrie. Veneer A thin rubber sheet applied in the replacement of the sidewall pattern details in the retreading of pneumatic tyres. A similar film of rubber specially compounded to resist oxygen or ozone or to prevent the migration of carbon black into a lighter rubber, e.g., a tyre white sidewall. Vent A channel or shallow groove cut on the surface of a mould or a hole drilled right through a mould wall. The object is to permit the escape of air in the initial stages of moulding and prevent the defect known as ‘light’ or ‘bare’ moulding. Vermillion The red form of mercuric sulphide once popular as an inorganic colouring agent for rubber. Vertical Continuous Vulcanisation Applied at present mainly in the vulcanisation of cables, and in fluid bed vulcanisation of extruded sections. VF2 Abbreviation for vinylidene fluoride. VFA Abbreviation for volatile fatty acid.
dried without smoking. The initials USF denote US Rubber Company Formaldehyde. U-Test A static test for determining the adhesion of tyre cord in rubber. The test piece is in the form of a loop shaped like the letter U. U-Value A measure of heat transmittance; the number of British Thermal Units transmitted per square foot of surface per hour for 1 °F difference in temperature between the two surfaces. See Thermal Conductivity. UV Ultraviolet.
9 VA Abbreviation for vinyl acetate. Vacuum Empty space in which there are no atoms or molecules. A perfect vacuum cannot be attained in practice and the term denotes a space containing air or other gas at a very low pressure. In industry ‘vacuum’ is measured in inches of mercury (in Hg) ranging from 0 in at atmospheric pressure to around 30 in at zero absolute pressure. Vacuum Extrusion Extrusion with the aid of a vacuum applied to the screw. The process is applied particularly in the preparation of extrudates to be vulcanised by either the liquid curing medium or fluid bed techniques. It assists in removing the volatiles from the compound and thus improves the quality of the extrudate. Vacuum Forming In rubber processing this means the same as vacuum moulding. In plastics manufacture it refers to the use of a controlled vacuum to support and form a sheet of heat-softened material into a desired contour. Vacuum Moulding A method of making products such as car floor mats where the ‘mould’ or contoured former is drilled with a series of small holes which lead into a backing chamber connected to a vacuum line. The vacuum holds the sheet of rubber firmly in contact with the former during curing. Valency The combining power of an atom; the number of hydrogen atoms which one atom of the element will combine with or replace. Valency Bond The link which holds the atoms together in a molecule. See Covalency and Electrovalency. Valency Electrons The electrons in the outermost shell of electrons surrounding an atomic nucleus, the number of which determines the valency of the atom. Value Analysis An analytical technique designed to examine all the functions of an existing product in order to determine whether or not any cost item can be reduced or eliminated while retaining all the functional and quality elements.
Rubber Basics Vinylacetylene This is reacted with hydrogen chloride to produce chlorobutadiene (chloroprene) which is polymerised to polychloroprene. See Neoprene. Vinyl Chloride The monomer from which the vinyl plastic polyvinyl chloride (PVC) is prepared. Vinyl chloride was originally made by passing acetylene and hydrogen chloride over a mercury chloride catalyst at a temperature of about 180 °C. Now made from ethylene chloride which is converted to vinyl chloride by contact with a catalyst at about 500 °C (900 °F) or by reaction with dilute caustic alkali at about 150 °C (300 °F). Ethylene chloride is produced by the reaction of ethylene and chlorine; it is denser than water and practically insoluble in it. It is an effective solvent for fats, waxes, greases, and numerous other organic compounds, but its use as a solvent has been largely discontinued in favour of tetrachloroethylene. Vinyl Group The unsaturated univalent radical CH2CH. Many vinyl compounds undergo polymerisation forming plastics, fibres and resins. See Vinyl Chloride. Vinyl Pyridine One component of a terpolymer of butadiene, styrene and vinyl pyridine used in latex form to promote good adhesion between rubber and textiles, particularly rayon and nylon. Viscoelasticity That particular combination of properties possessed by high polymers, characterising the rubber-like state. Depending on the temperature and the time of stressing, a high polymer may show viscous flow or high elasticity. See Elasticity, Glass Transition, Thixotropy and Viscosity. Viscometer An apparatus for measuring the viscosity of unvulcanised elastomers. The best known is the Mooney viscometer. Viscose Rayon That type of rayon which is regenerated from viscose, a syrupy liquid consisting mainly of a solution of cellulose xanthate in dilute sodium hydroxide. Viscosity Resistance to flow or resistance to relative motion within a substance. Although viscosity is usually applied to liquid it is replacing the less precise term ‘plasticity’ in relation to unvulcanised elastomers. See Viscoelasticity. Viscosity Gravity Constant (VGC) A measure of the average aromatic content of a petroleum oil. Viscosity Retention Index Another term for plasticity retention index. Viscosity-Stabilised Natural Rubber Natural rubber of consistent Mooney viscosity; storage hardening has been inhibited by incorporating a small quantity of a compound which reacts with the aldehydic groups present in the rubber.
Viscurometer An early cure instrument which combined in one operation the functions of a Mooney viscometer and of a curometer or vulcameter, i.e., it measures in one quick test the plasticity (viscosity) of the (uncured) mix, its scorch time and cure rate. Now superseded by instruments such as the moving die rheometer. Vitacap Process An obsolete process for retreading pneumatic tyres. The vulcanisation of the new tread rubber is not done in a mould but by the open steam method in an autoclave, and the desired pattern is cut on the tread after cure. VMQ Abbreviation for vinyl methyl silicone. Volatile Fatty Acid A test which is claimed to be a more reliable guide to the condition of a natural rubber latex than the KOH number. The test is performed by steam distillation of the latex and titration of the distillate with standard alkali solution. The VFA number is a measure of the state of degradation of the latex. Volume Resistivity The electrical resistance of a cube of side 1 cm to a current passed between opposite faces (BS 903:Part C2, Determination of volume resistivity). Volume Swelling This is the percentage increase in volume attained by immersing a vulcanised sample of rubber in a specified solvent. Volume swelling measurements are useful in determining the resistance of rubbers to solvents, but are also of value in measuring the crosslink densities of rubber vulcanisates. VRI Abbreviation for viscosity retention index. Vulcameter A general term applied to a variety of instruments for determining the curing characteristics of elastomers. The spelling ‘Vulkameter’ refers to a particular instrument developed by Farbenfabriken Bayer and marketed by Agfa Ltd. Vulcanisate A name given to a vulcanised rubber sample or product particularly where the shape or form of the rubber is not required to be specified. Vulcanisation This term was originally limited to the chemical reaction of rubber with sulphur to bring about the following effects: (a) reduced thermoplasticity, (b) increased tensile strength and resistance to abrasion, and (c) reduced solubility in organic solvents. Since many other substances can bring about the above changes the term has now been widened to include any treatment which will introduce crosslinks in the rubber matrix. Vulcanised Latex By suitable treatment (addition of curatives and careful heating) latex may be vulcanised without coagulation. The latex remains liquid and may be manufactured into products, the coagulum consisting of vulcanised rubber. A less ambiguous term is prevulcanised latex.
Vulcaniser A traditional term applied to almost any apparatus in which the process of vulcanisation is carried out. It is not normally applied to a daylight press. Vulcanising Agents Any substance which will bring about vulcanisation. Elemental sulphur remains a widely used vulcanising agent, but sulphurcontaining substances (such as thiuram disulphides) have important uses. Organic peroxides (benzoyl and dicumyl) and nitroso derivatives (e.g., benzoquinone dioxime) are used in vulcanising certain synthetic elastomers. Vulcanite Another name for ebonite.
absorb a sufficient quantity of waste to solve the problem nor does it produce a rubber which can meet high quality standards. Recent (1995) developments on recycling agents have yet to make any significant inroads into the problem Wax Although the true waxes, such as beeswax, are esters of fatty acids with alcohols, the term is often applied to certain solid substances which melt at fairly low temperatures, e.g., paraffin wax. Paraffin waxes (crystalline and microcrystalline) are obtained from the refining of petroleum, and are used in rubber compounding as protective agents. They have the property of blooming to the surface of the product, forming a thin film which replenishes itself if removed in service. Weathering The action of the weather on exposed materials. See Ageing. Weaving The process of interlacing two sets of textile yarns or threads to form a fabric. See Warp and Weft. Web A textile term denoting a width of cloth as woven in the loom. The meaning has been broadened in the rubber industry to include almost any sheeting such as might be positioned by a web guide, or the mat of fibres later impregnated with latex in the manufacture of non-woven fabrics. See Rubber Webbing. Web Guide A device for centring or controlling one or both edges of any material in sheet form. Weft The threads of a woven structure which run across the fabric from selvedge to selvedge at right angles to the warp threads. Weftless Applied to a tyre-cord fabric without any weft or cross-threads. The individual cords are spaced out by a reed, passed into an adhesive such as LRF, dried and coated with rubber compound by calendering. Wet and Dry Bulb Hygrometer One instrument for determining the relative humidity of the atmosphere. It consists of a pair of thermometers, the bulb of one of which is surrounded by a fabric wick kept moist from a small water reservoir. Due to evaporation the temperature indicated by the wet bulb thermometer is lower than that of the other. The difference in the readings compared to the dry bulb reading enables the relative humidity to be obtained from tables. Wet Frictioning Frictioning using a rubber dough instead of a conventional soft ‘friction’ compound. See Frictioning. Wet Mill An open mill on which the final stages of preparing spreading doughs are carried out. Wetting In rubber reinforcement, wetting denotes the covering or completeness of contact between the
: Wallace Rapid Plastimeter A plastimeter of the parallel plate type which enables a determination of plasticity to be made within about 1 minute (BS 903-A59.1). Wallace Shawbury Curometer An apparatus developed by Rapra for the determination of the scorch and cure characteristics of rubber compounds. The principle of operation is summarised thus: two small cylinders of the rubber are placed one on each side of a small paddle and the assembly inserted between electrically-heated platens. An electrically-driven mechanism subjects the specimen to a sinusoidal force and the movement of the paddle is magnified and printed on a chart. From the envelope so formed an estimate of plasticity, scorch time and cure time may be made. Now superseded by various rotorless machines such as the moving die rheometer. Warming Plasticising of mixed compound by working on an open mill or in an internal mixer, preparatory to extrusion or calendering. Warp The threads of a woven structure which run lengthwise of a fabric parallel to the selvedge. Washer A machine of the open-mill type having grooved rolls and means for directing jets of water on the rubber passing through the nip, the object being to remove impurities such as sand and bark from the rubber. The washing process is rarely necessary nowadays except in times of emergency when wild rubber may have to be processed. See Strainer. Waste Rubber Rubber products which have ended their useful lives; a proportion of this waste may be made usable again either by grinding down into crumb rubber or by the process of reclaiming. The term ‘waste’ is also applied to the uncured trimmings from various processing operations, which may be remilled, and added to new mixed compound. The disposal of old tyres is a worldwide problem. Dumping is obviously an unsatisfactory and unsightly answer, indiscriminate burning offends the Clean Air Act, and reclaiming does not
Rubber Basics rubber and the particles of the reinforcing agent, especially carbon black. Wetting Agents Substances used particularly in latex compounding to decrease surface tension, thus increasing wettability and facilitating the impregnation of fibres and fabrics. White Factice Also termed sulphur chloride factice or cold factice. That type of factice prepared by treating unsaturated oils, such as rape oil or castor oil, with sulphur monochloride. Since the reaction is exothermic care must be taken to keep the temperature as low as possible. See Factice. White Metal An alloy of lead, tin and antimony with a melting point about 180 °C, used as a material for making moulds for articles such as soles, heels and interlocking tiles. When the mould becomes offsize or damaged it is melted down and recast. White Spirit A petroleum distillate of boiling point range 150200 °C used as a solvent. See Naphtha. Whiting Finely-divided calcium carbonate obtained from natural sources (chalk, limestone or marble) or as a by-product of another chemical process precipitated whiting. Strictly speaking, the term ‘whiting’ should be applied only to ‘material prepared by grinding natural chalk’. WHO World Health Organization. Whole Tyre Reclaim Reclaimed rubber made from pneumatic tyres which have ended their useful lives. Tyres form the main source of material for reclaiming. See Reclaimed Rubber. Wiegand Pendulum An apparatus which demonstrates the GoughJoule effect. It comprises a pendulum adjusted so that a rubber sample is under stretch. Heat from a lamp causes the rubber to contract and swing the pendulum. This pulls the rubber into a shaded section where it extends and moves the pendulum back to the original position, whereupon the cycle is repeated. Many attempts have been made to develop the Wiegand Pendulum into a rubber ‘engine’, and although a variety of devices have been demonstrated, none has reached commercial utilisation. A ‘Polymotor’ was developed by Professor Natta using trans-butadiene as the polymer. Wig-Wag The form of or act of laying strip material taken off a mill or extruder into a basket in an oscillating manner. Such material is then suitable for subsequent automatic feeding of production equipment such as injection moulding machines. Wild Rubber Natural rubber obtained from trees growing ‘wild’ and not cultivated in either plantations or native small holdings. The output of wild rubber is now insignificant. Williams’ Plastometer The earliest and best-known of parallel plate plastometers. The original model has been
modified in several ways to improve its ease of operation and its accuracy. Now obsolete. Wintering The annual leaf loss suffered by rubber trees. It coincides with the dry season in February and March. Since the trees are then using their reserves for refoliation there is a temporary drop in yield, and changes occur in the composition of the latex. Wire Cord In most modern pneumatic tyres the ‘textile’ reinforcement is in the form of steel wire constructed in the manner of cord fabric. Wood Flour Finely divided wood, used as an inert filler and stiffener in rubber compounds. Wood Rosin See Rosin. Wound Response In a rubber tree which is being tapped for the first time there is a high percentage of rubber in the latex (about 60% as against the normal 30%) and only a low yield is obtained. As tapping is continued the latex becomes more dilute and a higher yield is given. This phenomenon is known as wound response. Wrapped Hose Hose constructed by wrapping the reinforcing fabric and the calendered cover on to the inner tube which has been fitted over a mandrel of the desired diameter. The application of the fabric, the cover and of the wrapper may be done either by hand or by machine. Wrapper A length of narrow textile material which is tightly wrapped round a product, e.g., wrapped hose, to apply pressure during vulcanisation. The term is used also in the sense of lining.
; Xanthates Salts of the series of xanthic acids of the general formula ROCSSH. Certain xanthates such as ZIX are ultra accelerators for rubber. Cellulose xanthate is the intermediate product in the manufacture of viscose. See Viscose Rayon. Xanthogen Sulphide Diisopropyl xanthogen polysulphide, accelerator. XNBR Abbreviation for carboxylated nitrile rubber. X-Ray Diffraction The technique of using the diffraction of X-rays to study the structure of fibres, plastics and elastomers, to determine the crystalline nature of such polymers, and to measure the particle size of finely divided materials. X-Ray Fluorescence Spectroscopy This is a semi-quantitative elemental analysis technique. X-Ray Photoelectron Spectroscopy This is a surface analysis technique. X-Rays Electromagnetic waves of short wavelength 0.01 to 50 Ångström units, which are produced when
Young’s Modulus The modulus of elasticity of a material; it is the ratio of the stress to the strain produced by the stress in the material. Hooke’s law is obeyed by metals but rubber obeys Hooke’s law only at small strains in shear. At low strains up to about 15% the stress-strain curve is almost linear, but above 15% the stress and strain are no longer proportional. See Modulus.
streams of high energy electrons impinge on matter, usually metal in commercial systems. XPS X-ray photoelectron spectroscopy. XRF X-ray fluorescence spectroscopy. Xylene Xylol (dimethylbenzene), used as a rubber solvent. Xylene exists in three isomeric forms, commercial xylol being a mixture of all three. Xylyl Mercaptan An efficient peptising agent for natural rubber; it is also used as a bleaching agent in the preparation of pale crepe rubber.
= Z Calender A four-bowl calender in which rolls 1 and 2 are situated in one horizontal plane and the other two, 3 and 4, in a lower horizontal plane. Roll 3 is below roll 2, 1 and 4 being therefore ‘offset’. See Triangular Calender. ZBED Zinc dibenzyl dithiocarbamate, accelerator. ZDBC Zinc dibutyl dithiocarbamate, accelerator. ZDBCX Amine-activated zinc dibutyl dithiocarbamate, accelerator. ZDC Zinc diethyl dithiocarbamate, accelerator. ZDEC Zinc diethyl dithiocarbamate, accelerator. ZDMC Zinc dimethyl dithiocarbamate, accelerator. Zeolites Naturally occurring hydrated silicates of calcium and aluminium; the name is also given to synthetic substances with a similar crystalline structure used as the basis of molecular sieves. ZEPC Zinc ethylphenyldithiocarbamate, accelerator. Ziegler Catalyst A catalyst of aluminium and other metal alkyls in combination with metallic halides, e.g., the catalyst obtained by the interaction of a trialkylaluminium with titanium tetrachloride. Such catalysts, discovered by Karl Ziegler, are used in making stereospecific polymers. Zinc Borate Flame retardant. Zinc Dibenzyl Dithiocarbamate ZBED, accelerator. Zinc Dibutyl Dithiocarbamate ZDBC, accelerator. Zinc Diethyl Dithiocarbamate An ultra accelerator too scorchy for use as the sole accelerator in ‘dry’ rubber compounding, but popular in latex work. In dry rubber compounding it is a useful booster for thiazole type accelerators. In some low ammonia latices it is used as a preservative. Zinc Di-Isononyl Thiocarbamate Accelerator. Zinc Dimethyl Dithiocarbamate ZDMC, accelerator. Zinc Ethylphenyldithiocarbamate ZEPC, accelerator.
90%) have a Tg around –90 °C, and hence exhibit excellent low temperature flexibility only exceeded by the phenyl silicones. They also exhibit excellent resilience and abrasion resistance; unfortunately the high resilience gives poor wet grip in tyre treads, and hence this rubber finds limited use as the sole base for such compounds. As the cis 1,4 content decreases, and 1,2 vinyl content increases, the low temperature properties, abrasion resistance and resilience become inferior. The polymerisation of butadiene results in a polymer with a narrow molecular weight distribution which can be difficult to process. Indeed, commercially available grades present a compromise between processibility and performance. Most polybutadiene rubbers are inherently difficult to break down during mixing and milling, have low inherent tack, and the inherent elasticity of the polymer gives poor extrudability. Peptisers can be used to facilitate breakdown and hence aid processing. Due to the unsaturation present in the main chain, protection is required against oxygen, UV and ozone. Oil resistance is poor and the polymer is not resistant to aromatic, aliphatic and halogenated hydrocarbons. Polybutadiene based compounds can be cured by sulphur, sulphur donor systems and peroxides. Less sulphur and a higher level of accelerators are required when compared to NR. The cure of polybutadiene by peroxides is highly ‘efficient’ in that a large number of crosslinks are produced per free radical, the resultant highly crosslinked rubber exhibiting high resilience; this factor is utilised in the manufacture of ‘superballs’. Compounds based on this polymer only give optimum properties at high filler and oil loadings. Uses Most polybutadiene is used in tyre applications, and the majority of this use is in blends with other polymers, such as NR and SBR, where polybutadiene reduces heat build-up and improves the abrasion resistance of the blend. The friction on ice of winter tyres is also improved by using higher levels of polybutadiene in the tread blend. When polybutadiene is used in blends for other applications, it is where the improved abrasion and low temperature flexibility conferred on a blend is advantageous, e.g., in shoes, conveyor and transmission belts.
3.4 Nitrile Rubbers (NBR/HNBR) Designation in ISO 1629 - NBR Repeat Unit
General Nitrile rubbers are copolymers of butadiene and acrylonitrile which are produced by emulsion polymerisation; ‘hot’ and ‘cold’ polymerised types are available. The ‘hot’ polymerised types generally have higher green strength and are slightly harder to process than ‘cold’ copolymers. The introduction of acrylonitrile into the polymer backbone imparts oil resistance and affects many other properties. Grades which vary in acrylonitrile (ACN) content from 18-50% are commercially available, the percentage of acrylonitrile present forming the basis of the following grade descriptions: Low Medium low Medium Medium high High
18-24% 26-28% 34% 38-40% 50%
ACN ACN ACN ACN ACN
Many properties are influenced by the acrylonitrile content, e.g.: % Acrylonitrile content 18% : 50%
: : : : : : : 8 8 :
Oil resistance improvement Fuel resistance improvement Tensile strength improvement Hardness increase Abrasion resistance improvement Gas impermeability improvement Heat resistance improvement Low temperature flexibility improvement Resilience improvement Plasticiser compatibility
A typical figure for the Tg of an 18% ACN copolymer is –38 °C, and that of a 50% ACN copolymer –2 °C. Carboxylated nitriles, hydrogenated nitrile, liquid nitriles and blends with PVC are also commercially available. The carboxylated types (XNBR) contain one, or more, acrylic type of acid as a terpolymer, the resultant chain being similar to nitrile except for the presence of carboxyl groups which occur about every 100 to 200 carbon atoms. This modification gives the polymer vastly improved abrasion resistance, higher hardness, higher tensile and tear strength, better low temperature brittleness, and better retention of physical properties after hot-oil and air ageing when compared to ordinary nitrile rubber.
Rubber Basics Low molecular weight liquid nitrile grades are available and these can be used as compatible plasticisers in the compounding of nitrile rubber. Such plasticisers can be partially crosslinked to the main chain during cure, and hence exhibit low extractability. PVC/NBR polymer blends can be produced as colloidal or mechanical blends, the former generally giving superior properties. Commercially available blends have PVC contents ranging from 3055%. The blends have reduced elasticity, which gives improved extrudability, but they also exhibit superior ozone resistance, improved oil swell resistance, and tensile and tear strength; this, however, is achieved at the expense of low temperature flexibility and compression set. The ozone resistance of such blends is, however, only improved if the PVC is adequately distributed and fluxed. This is harder to achieve in mechanical blends, but if it is not achieved failure due to ozone attack can occur. Another method by which the ozone resistance of nitrile rubber can be improved is the removal of the double bonds in the main chain of the copolymer by hydrogenation. Hydrogenated nitrile rubbers (HNBR) also exhibit much greater resistance to oxidation, and extend the useful service temperature range of nitriles up to ca. 150 °C. Commercially available grades offer different degrees of hydrogenation with residual double bonds ranging from ca. 0.8%-6%. Nitriles have good resistance to oil, aliphatic and aromatic hydrocarbons and vegetable oils, but are swollen by polar solvents such as ketones. The unsaturated main chain means that protection against oxygen, ozone and UV light is required. In compounding, choice of the correct grade is required if the required balance of oil resistance and low temperature flexibility is to be achieved. Nitrile rubber can be cured by sulphur, sulphur donor systems and peroxides. However, the solubility of sulphur in nitrile rubber is much lower than in NR, and a magnesium carbonate coated grade (sulphur MC) is normally used; this is added as early in the mixing cycle as possible. Less sulphur and more accelerator than is commonly used for curing natural rubber is required. A cadmium oxide/magnesium oxide cure system gives improved heat resistance, but the use of cadmium, a heavy metal, will increasingly be restricted. The hydrogenated nitrile (HNBR) grades which contain the lowest level of residual double bonds can only be crosslinked by the use of peroxides and radiation, whilst those with a level of residual double bonds greater than about 3.5% can be cured by sulphur. In addition to the normal sulphur cure systems, metal oxides can be used to cure the carboxylated nitriles. The low temperature properties of nitriles can be improved by the use of suitable plasticisers, e.g., ester plasticisers. Uses Nitrile rubber, due to its oil resistance, is widely used in sealing applications, hose liners, roll coverings, conveyor belts, shoe soles and plant linings. Nitrile rubber is also available as a latex.
3.5 Epichlorohydrin Polymers (CO/ECO/ETER) Designation in ISO 1629 - CO & ECO Repeat Unit Epichlorohydrin homopolymer (CO)
CH 2 Cl Epichlorohydrin copolymer with ethylene oxide (ECO)
CH 2 Cl General Epichlorohydrin is also available as a terpolymer with a small amount of unsaturated allyl glycidyl ether. There is no ISO designation for the terpolymer, but ETER is used by ASTM. As with EPDM, the unsaturation is pendant to the main chain and this allows vulcanisation with sulphur, whilst preserving the stability of the main chain. The ability to be cured by sulphur also allows the terpolymer to be used in blends with other polymers, e.g., nitriles. As might be expected, the homopolymer having the highest polarity exhibits the best oil resistance, but this is at the detriment of low temperature flexibility. The homopolymer also has a low permeability to gases. The unsaturated backbone gives these materials good resistance to oxygen, ozone and light. Resistant to oils, aliphatic hydrocarbons and alcohols, alkalis and dilute mineral and oxidising acids. Attacked by strong mineral and oxidising agents and chlorine. The main method of crosslinking the homopolymer and copolymer is by use of thioureas, and, as the cure reaction requires basic conditions, an acid acceptor is also added. Litharge, red lead, magnesium oxide and dibasic lead phosphite are commonly used acid acceptors, and the most commonly used thiourea is ethylene thiourea, but this has a tendency to promote mould fouling. The Echo S cure system has been commercialised by BFGoodrich and this is said to give improved scorch safety and reduced mould fouling over the use of thioureas. Inorganic acid acceptors other than those based on lead are recommended for use with the Echo S cure system. The terpolymers can, in addition to the use of thioureas, be cured by the use of sulphur and peroxides. Uses The main use of epichlorohydrin is in the automotive sector for various seals and hoses, gaskets, orings and diaphragms. The terpolymer is used in roller production and in many low temperature applications.
3.6 Polychloroprene (CR) Designation in ISO 1629 - CR Repeat Unit
General This polymer is frequently, but incorrectly, referred to as Neoprene which is a trade name. Polychloroprene is produced by emulsion polymerisation, during which the following forms of addition are possible: CH 2
CH 2 C
C CH 2
Cl trans - 1,4 addition
cis - 1,4 addition
Cl CH 2
CH 2 CH 2
CH 2 3,4 addition
Since it is not possible to commercially produce a polymer that is based on the cis 1,4 form, commercial polymers are based on the trans 1,4 form which has a crystalline melting point, Tm, of +75 °C and a Tg of –45 °C. Pure 1,4 trans polychloroprene thus crystallises readily and would normally be considered to be of limited use for a rubber. Such a polymer, however, does not crystallise when dissolved in a solvent, but will do so when the solvent evaporates. This feature is used to good effect in the production of contact adhesives. The temperature of polymerisation, however, influences how closely the polymer attains the trans 1,4 form. Raising the polymerisation temperature from –40 °C to +40 °C increases the percentage of 1,2 and 3,4 forms both of which reduce the regularity and hence the tendency to crystallise. Thus chloroprene based polymers that are intended to be rubbery are polymerised at higher temperatures. The 1,2 grouping in the main chain is the site of crosslinking reactions during cure. The ability to crystallise can also be controlled by copolymerising chloroprene with small amounts of other monomers. Two different mechanisms are used to control the molecular weight of the polymer during polymerisation:
^ In the so-called G types, sulphur is copolymerised with the chloroprene to yield a product as shown schematically below: Sx
The G types are stabilised with TETD, with the result that the G types do not require further acceleration to cure.
^ In the so-called W types, the molecular weight is controlled by the use of a mercaptan. The following differences are apparent between the G and W types: G types G types can break down during mixing or milling via cleavage at the Sx group; this decreases molecular weight and hence reduces the elasticity, or nerve, during processing. The extent of breakdown is somewhat dependent on the exact grade, Neoprene GW being virtually unaffected by milling. Cleavage at the Sx group can also occur during long-term storage, and the G types therefore have the disadvantage of a limited storage life. The G types do not require further acceleration during cure, but exhibit slightly inferior ageing characteristics. Resilience and tack are generally better than with the W types. W Types These types exhibit superior storage life, and ageing characteristics, but require the addition of accelerators to achieve an acceptable rate of cure. They do not break down during mixing. During processing they are less prone to scorch, and will accept higher loadings of filler. The cured compound generally exhibits a lower compression set, and a greater ability to resist heat ageing. The chlorine atom in the repeat unit has a tendency to deactivate the double bond in the main chain, thus polychloroprene tends to resist oxidation, ozone and UV light to a higher degree than the other unsaturated rubbers, although they still require protection if the maximum performance is to be obtained. Unfortunately, this deactivation of the double bond means that the polymer cannot be crosslinked by sulphur. The chlorine atom also confers an increased level of resistance to oils, so that the oil resistance of polychloroprene is roughly intermediate between natural rubber and nitrile rubber, and is often sufficient for many applications. Polychloroprene is also self-extinguishing in flame tests. Metal oxides are principally used for curing these materials; peroxides are generally not used. The most widely used cure system is based on magnesium oxide/zinc oxide, the cured properties achieved being dependent on the ratio of the two; the most common ratio is magnesium oxide 4.0 and zinc oxide 5.0. As the zinc oxide tends to promote scorch it is added late in the mixing cycle, whilst magnesium oxide is added early. One drawback of the MgO/ZnO cure system is that chlorine liberated during cure reacts with the oxides to yield chlorides which are hydrophilic and compounds containing this cure system can swell in hot water; even in cold water swell can be progressive and eventually large. Lead oxide (PbO or Pb3O4) up to levels of 20 phr can be used to improve resistance to water as the chloride formed during cure is insoluble. The W types require additional acceleration and ethylene thiourea (ETU), gives the best balance of all properties. However, the use of this accelerator is increasingly being restricted due to fears of its effects on pregnant women, and more recently men. DETU, thiurams and guanidines can also be used. Sulphur is sometimes used to increase the degree of cure in the W types, but this detracts from the ageing performance of the vulcanisate.
Rubber Basics Uses Due to its balance of strength, oil resistance, inflammability, increased resistance to ozone, ageing and weathering, polychloroprene finds widespread industrial use. Typical uses are V-belts, conveyor belts, wire and cable jacketing, footwear, wet suit applications, coated fabrics, inflatables, hoses, extrusions and many other goods. Adhesives are also a strong market area.
3.7 Polynorbornene Designation in ISO 1629 - N/A Repeat Unit
CH CH 2
General The large ring structure in the main chain gives this material a high Tg of +35 °C, and thus it is not rubbery at normal ambient temperatures and requires plasticisation to achieve elastomeric behaviour. This material exhibits some desirable advantages. It can be extended by large quantities of oils to give very soft vulcanisates (ca. 20 Shore A) with acceptable strength, and it gives high damping which can be useful for vibration and noise reduction applications. However, since plasticisation is required particular care has to be exercised in the choice of plasticiser if exposure to higher than ambient temperatures is anticipated. Polynorbornene is not oil resistant, and solvents which can extract the plasticiser will obviously be detrimental to its performance. The material can be cured by both sulphur and peroxides, but requires protection against oxygen, ozone and UV light. Uses Roll covers, and elements designed to utilise the high damping properties of this material are thought to be the major uses.
3.8 Butyl Rubbers (IIR/BIIR/CIIR) Designation in ISO 1629 - IIR, BIIR & CIIR Repeat Unit (IIR)
CH 3 General Commercial grades of IIR (butyl rubber) are prepared by copolymerising small amounts of isoprene with polyisobutylene. The isoprene content of the copolymer is normally quoted as the ‘mole percent unsaturation’, and it influences the rate of cure with sulphur, and the resistance of the copolymer to attack by oxygen, ozone and UV light. The polyisobutylene, being saturated, however, naturally confers on the polymer an increased level of resistance to these agencies when compared to natural rubber. Commercial butyl rubbers typically contain 0.5-3.0% mole unsaturation. The close packing of the isobutylene chain confers on the polymer a high degree of impermeability to gases, but also results in a very ‘lossy’ rubber. The high hysteresis loss can be utilised in some circumstances to provide good friction in wet conditions. Chlorobutyl (CIIR) and bromobutyl (BIIR) are modified types containing 1.2% wt of chlorine or bromine, the isoprene unit being the site of halogenation. Introduction of the halogen gives greater cure flexibility, and enhanced cure compatibility in blends with other diene rubbers. It also confers increased adhesion to other rubbers and metals. Butyl rubber is not oil resistant. Butyl, and the halogenated butyls, can be cured by sulphur, dioxime and resin cure systems. In addition, the halogenated types can be crosslinked with zinc oxide, and diamines. Peroxides cannot be used because they tend to depolymerise the polyisobutylene. Due to the low level of unsaturation in the main chain, sulphur cures require the more active thiuram and dithiocarbamate accelerators to achieve an adequate state of cure. Dioxime cures yield vulcanisates with good ozone resistance and moisture impermeability and, as such, are frequently used for curing electrical insulating compounds. Resin cures utilise phenol-formaldehyde resins with reactive methylene groups and a small added amount of either a chlorinated rubber, e.g., polychloroprene, or stannous chloride. If halogenated phenolic resins are used the additional source of a halogen may not be required. Resin cures give butyl compounds excellent heat stability and are used to good effect where this is required, e.g., in tyre curing bags which have to resist service at 150 °C in a steam atmosphere. Calcium stearate has to be added to stabilise the chlorobutyl during processing. Uses The main applications of butyl rubber are in wire and cable applications, inner tubes, inner liners in tubeless tyres, tyre curing bladders, and pharmaceutical closures, the latter utilising the low
Rubber Basics impermeability of butyl to gases. Other applications include vibration isolation, caulk and sealants, and sheeting for pond liners and roofing.
3.9 Styrene-Butadiene Rubber (SBR) Designation in ISO 1629 - SBR Repeat Unit
General When the USA and Germany were cut off from the supplies of natural rubber during the Second World War both countries sought to produce a synthetic alternative; SBR was the result, and at one stage it was the most commonly used synthetic rubber. It can be produced by both emulsion and solution polymerisation techniques, with the emulsion grades being the most widely used. Emulsion polymerisation yields a random copolymer, but the temperature of the polymerisation reaction also controls the resultant properties obtained. ‘Cold’ polymerisation yields polymers with superior properties to the ‘hot’ polymerised types. Solution polymerisation can yield random, di-block, tri-block or multi-block copolymers. It is important to note that the tri-block, or multi-block copolymers, belong to that class of material termed thermoplastic elastomers and it is only the random copolymer types that are considered here. Both random emulsion and solution polymerised SBR contain about 23% styrene. SBR continues to be used in many of the applications where it earlier replaced natural rubber, even though it requires greater reinforcement to achieve acceptable tensile and tear strengths, and durability. SBR exhibits significantly lower resilience than NR, so that it has a higher heat build-up on flexing which restricts its use in lorry tyres with their thicker sections. This inferior resilience to natural rubber is an advantage in passenger car tyre treads because the higher hysteresis loss gives increased wet grip and this, combined with the good abrasion resistance that can be obtained from tyre tread compounds, ensures that SBR has a high volume use in tyre production. The oil resistance of SBR is poor, and the polymer is not resistant to aromatic, aliphatic or halogenated solvents. Due to the unsaturation in the main chain, protection is required against oxygen, ozone and UV light. Oil extended SBR, and SBR carbon black masterbatches are supplied by the polymer producers and such grades give the advantage of reducing the necessity of further additions of filler and oil at the mixing stage. SBR can be cured by the use of sulphur, sulphur donor systems and peroxides. Sulphur cures generally require less sulphur (1.5-2.0 phr) and more accelerator than is normally required to cure natural rubber.
Uses The major use of SBR is in tyres, predominantly car and light truck; in the latter use it is frequently blended with NR and BR. SBR also finds use in conveyor belts, moulded rubber goods, shoe soles, hose and roll coverings. SBR is also available as a latex which is used in carpet backing and other applications.
3.10 Ethylene-Propylene Rubber (EPM/EPDM) Designation in ISO 1629 - EPM / EPDM Repeat Unit Ethylene-propylene rubber (EPM)
)x ( CH 2
Ethylene-propylene-diene-methylene rubber (EPDM)
)x ( CH 2
)x ( CH 2
Terpolymer: ethylidene norbornene
)x ( CH 2
CH 2 CH Terpolymer: 1,4 - hexadiene
CH CH 3
General The copolymerisation of ethylene and propylene yields useful copolymers, the crystallisation of both polymers being prevented if the ethylene content is in the range 45-60%; grades with higher ethylene contents, 70-80%, can partially crystallise. The lower ethylene types are generally easier to process, whilst green strength and extrudability improve as the ethylene content increases. One disadvantage of the copolymer is that it cannot be crosslinked with sulphur due to the absence of unsaturation in the main chain. To overcome this difficulty a third monomer with unsaturation is introduced, but to maintain the excellent stability of the main chain the unsaturation is made pendant to it. The three types of third monomer used commercially are dicyclopentadiene, ethylidene norbornene, and 1,4-hexadiene. Generally 4-5% of the termonomer will give acceptable cure characteristics, whilst 10% gives fast cures; dicyclopentadiene gives the slowest cure rate and ethylidene norbornene the highest. Since the main chain of both EPM and EPDM rubbers is saturated, both co- and terpolymers exhibit excellent stability to oxygen, UV light, and are ozone resistant. EPM and EPDM are not oil resistant, and are swollen by aliphatic and aromatic hydrocarbons, and halogenated solvents. They have excellent electrical properties and stability to radiation. Their densities are the lowest of the synthetics, and they are capable of accepting large quantities of filler and oil. They exhibit poor tack, and even if tackifiers are added, it still is not ideal for building operations. Adhesion to metal, fabrics and other materials, can be difficult to accomplish. The copolymers can only be cured by peroxides or radiation, whilst the terpolymers can be cured with peroxides, sulphur systems, resin cures and radiation. The dicyclopentadiene terpolymer can give higher states of cure with peroxides than the copolymer, although in peroxide curing of both the copolymer and terpolymer it is common practice to add a coagent, to increase the state of cure. Triaryl isocyanurate or sulphur are the most common coagents. Bloom can be a problem in sulphur cures, so selection of the accelerator system is important. Resin cures utilise the same resins that are used for butyl rubber, but more resin (ca. 10-12 phr) and a halogen donor (10 phr), typically bromobutyl, or polychloroprene, are required. Although heat stability is slightly improved by resin curing when compared to sulphur cures, the effect is not as marked as in the resin curing of butyl.
Uses Wire and cable applications and extrusion profiles, e.g., window seals and car door seals, probably form the major applications for EPM and EPDM rubber, although they are also used in a wide variety of other extrusion and moulding applications. Washing machine door seals moulded from EPDM are starting to replace NR as washer/dryers are becoming more common.
3.11 Chlorinated Polyethylene (CPE, CM) Designation in ISO 1629 - CM Repeat Unit
Cl General Although polyethylene has a low Tg it is highly crystalline and hence it is a thermoplastic and not a rubber at ambient temperatures. If the regularity of the main chain could be interrupted, and crystallisation effectively prevented, a useful elastomer might result. The chlorination of polyethylene is one method by which crystallisation can be prevented and chlorinated polyethylene is commercially available; the degree of chlorination, however, determines how rubbery the modified polymer is. Polymers with a chlorine content of ca. 25% are still relatively crystalline, whilst those with a chlorine content of greater than 40% become increasingly brittle due to interaction between the now highly polar polymer chains. The most desirable polymers, in terms of the absence of crystallinity and flexibility of the chains, are obtained when the degree of chlorination is around 35%. As with other polar polymers, these materials will resist oil, and the absence of a double bond in the main chain confers excellent stability to the deleterious effects of oxygen, ozone and light. Due to the absence of double bonds in the main chain, these materials can only be crosslinked by the action of peroxides or radiation. It is recommended that metal oxides are added to act as acid acceptors during vulcanisation, the oxides of magnesium and lead being used; zinc oxide is not used as it decreases the stability of the polymer. Uses It is fairly true to say that the use of chlorinated polyethylene has not been large, possibly due to the greater ease with which the chlorosulphonated polyethylene (Hypalon), a closely related competitor material, can be cured. When used, chlorinated polyethylene has found its major use in the wire and cable industry. It is also used in pond liners.
3.12 Chlorosulphonated Polyethylene (CSM, CSPE) Designation in ISO 1629 - CSM Repeat Unit
CH 2 CH
General The level of chlorination in these materials varies, and influences the properties of the material in exactly the same manner as the closely related chlorinated polyethylene. The introduction of the chlorosulphonyl group in small amounts,